# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy1_a
_database_code_depnum_ccdc_archive 'CCDC 1893226'
loop_
_audit_author_name
_audit_author_address
ddzhang
;Henan University
China
;
_audit_update_record             
;
2019-01-24 deposited with the CCDC.	2020-02-27 downloaded from the CCDC.
;
_audit_creation_date             2018-01-25
_audit_creation_method           
;
Olex2 1.2
(compiled 2017.08.10 svn.r3458 for OlexSys, GUI svn.r5381)
;
_shelx_SHELXL_version_number     2018/1
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         '0.25(Cs8 K4 O156 Se16 Ta24), 4(O)'
_chemical_formula_sum            'Cs2 K O43 Se4 Ta6'
_chemical_formula_weight         2394.46
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_H-M_alt        'C 1 2/c 1'
_space_group_name_Hall           '-C 2yc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'

_cell_length_a                   13.111(2)
_cell_length_b                   17.693(3)
_cell_length_c                   17.135(3)
_cell_angle_alpha                90
_cell_angle_beta                 93.414(3)
_cell_angle_gamma                90
_cell_volume                     3967.8(11)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    871
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      20.95
_cell_measurement_theta_min      2.32
_shelx_estimated_absorpt_T_max   0.306
_shelx_estimated_absorpt_T_min   0.176
_exptl_absorpt_coefficient_mu    22.183
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.4938
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
'SADABS-2016/2 (Bruker,2016/2) was used for absorption correction. wR2(int) was 0.1127 before and 0.0586 after correction. The Ratio of minimum to maximum transmission is 0.6622. The λ/2 correction factor is Not present.'
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    4.008
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4188
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.07
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0855
_diffrn_reflns_av_unetI/netI     0.1002
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            10234
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.935
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                2166
_reflns_number_total             3531
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         2.087
_refine_diff_density_min         -1.932
_refine_diff_density_rms         0.403
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.014
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     146
_refine_ls_number_reflns         3531
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1017
_refine_ls_R_factor_gt           0.0524
_refine_ls_restrained_S_all      1.014
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0418P)²+43.6701P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1040
_refine_ls_wR_factor_ref         0.1264
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.70519(6) 0.65386(5) 0.27876(5) 0.0211(2) Uani 1 1 d . . . . .
Ta2 Ta 0.38746(7) 0.80820(5) 0.31328(5) 0.0234(2) Uani 1 1 d . . . . .
Ta3 Ta 0.48575(6) 0.65770(5) 0.41060(5) 0.0237(2) Uani 1 1 d . . . . .
Se1 Se 0.22512(16) 0.69512(13) 0.40845(12) 0.0279(5) Uani 1 1 d . . . . .
Se2 Se 0.63300(19) 0.49665(15) 0.16986(14) 0.0437(7) Uani 1 1 d . . . . .
Cs1 Cs 0.66710(12) 0.45876(10) 0.41232(10) 0.0530(5) Uani 1 1 d . . . . .
K1 K 1.000000 0.6317(5) 0.250000 0.045(2) Uani 1 2 d S T P . .
O1 O 0.3234(12) 0.9058(9) 0.2911(9) 0.045(4) Uiso 1 1 d . . . . .
O2 O 0.6522(10) 0.5482(8) 0.2519(8) 0.031(4) Uiso 1 1 d . . . . .
O3 O 0.5672(12) 0.4241(9) 0.2030(9) 0.047(4) Uiso 1 1 d . . . . .
O4 O 0.3966(11) 0.9086(8) 0.3636(8) 0.036(4) Uiso 1 1 d . . . . .
O5 O 0.5384(11) 0.5484(8) 0.1232(8) 0.038(4) Uiso 1 1 d . . . . .
O6 O 0.500000 0.8231(10) 0.250000 0.023(5) Uiso 1 2 d S T P . .
O7 O 0.8134(10) 0.5908(8) 0.3285(8) 0.033(4) Uiso 1 1 d . . . . .
O8 O 0.4827(11) 0.7769(8) 0.4084(8) 0.034(4) Uiso 1 1 d . . . . .
O9 O 0.2681(10) 0.7817(8) 0.3837(8) 0.031(4) Uiso 1 1 d . . . . .
O10 O 0.2103(9) 0.6497(7) 0.3204(7) 0.023(3) Uiso 1 1 d . . . . .
O11 O 0.8322(10) 0.6750(8) 0.3433(8) 0.032(4) Uiso 1 1 d . . . . .
O12 O 0.2910(10) 0.7727(8) 0.2228(7) 0.026(3) Uiso 1 1 d . . . . .
O13 O 0.5310(11) 0.6011(8) 0.5046(8) 0.034(4) Uiso 1 1 d . . . . .
O14 O 0.5445(11) 0.6827(8) 0.5150(8) 0.033(4) Uiso 1 1 d . . . . .
O15 O 0.6126(10) 0.6557(7) 0.3602(7) 0.025(3) Uiso 1 1 d . . . . .
O16 O 0.3357(10) 0.6573(8) 0.4480(8) 0.029(3) Uiso 1 1 d . . . . .
O17 O 0.4039(9) 0.6916(7) 0.3069(7) 0.020(3) Uiso 1 1 d . . . . .
O1W O 0.2396(13) 0.8430(9) 0.0904(10) 0.059(5) Uiso 1 1 d . . . . .
O2W O 0.5876(16) 0.8654(12) 0.5092(12) 0.086(7) Uiso 1 1 d . . . . .
O3W O 0.9317(14) 0.4983(11) 0.1726(10) 0.067(5) Uiso 1 1 d . . . . .
O4W O 1.0361(16) 0.7719(12) 0.3364(12) 0.082(6) Uiso 1 1 d . . . . .
O5W O 0.8693(17) 0.4796(13) 0.5226(13) 0.101(8) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta2 3.3452(13) 2_655 ?
Ta1 Cs1 4.1881(19) . ?
Ta1 K1 3.9450(13) . ?
Ta1 O2 2.037(13) . ?
Ta1 O7 1.959(14) . ?
Ta1 O10 2.084(12) 2_655 ?
Ta1 O11 1.979(14) . ?
Ta1 O12 2.104(13) 2_655 ?
Ta1 O15 1.904(12) . ?
Ta1 O17 2.096(13) 2_655 ?
Ta2 Ta3 3.3581(13) . ?
Ta2 Cs1 4.3483(19) 3_455 ?
Ta2 O1 1.948(16) . ?
Ta2 O4 1.976(14) . ?
Ta2 O6 1.901(3) . ?
Ta2 O8 2.069(14) . ?
Ta2 O9 2.087(13) . ?
Ta2 O12 2.040(13) . ?
Ta2 O17 2.078(12) . ?
Ta3 Cs1 4.2468(19) . ?
Ta3 Cs1 4.2652(18) 5_666 ?
Ta3 O5 2.037(14) 2_655 ?
Ta3 O8 2.109(14) . ?
Ta3 O13 1.959(14) . ?
Ta3 O14 1.955(14) . ?
Ta3 O15 1.919(12) . ?
Ta3 O16 2.105(13) . ?
Ta3 O17 2.108(13) . ?
Se1 Cs1 4.281(3) 5_666 ?
Se1 O9 1.694(14) . ?
Se1 O10 1.710(13) . ?
Se1 O16 1.701(14) . ?
Se2 Cs1 4.206(3) . ?
Se2 Cs1 4.154(3) 2_655 ?
Se2 O2 1.682(13) . ?
Se2 O3 1.666(16) . ?
Se2 O5 1.703(15) . ?
Cs1 O1 3.146(15) 3_545 ?
Cs1 O2 3.168(13) . ?
Cs1 O3 3.605(16) 2_655 ?
Cs1 O4 3.292(14) 3_545 ?
Cs1 O5 3.154(15) 2_655 ?
Cs1 O7 3.395(14) . ?
Cs1 O9 3.447(14) 3_545 ?
Cs1 O13 3.516(14) . ?
Cs1 O13 3.214(14) 5_666 ?
Cs1 O15 3.657(13) . ?
Cs1 O16 3.156(13) 5_666 ?
Cs1 O5W 3.18(2) . ?
K1 O7 2.951(13) 2_755 ?
K1 O7 2.952(13) . ?
K1 O10 2.961(13) 1_655 ?
K1 O10 2.961(13) 2_655 ?
K1 O11 2.899(14) 2_755 ?
K1 O11 2.899(14) . ?
K1 O3W 2.83(2) 2_755 ?
K1 O3W 2.83(2) . ?
K1 O4W 2.91(2) . ?
K1 O4W 2.91(2) 2_755 ?
O1 O4 1.53(2) . ?
O7 O11 1.528(18) . ?
O13 O14 1.464(18) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ta2 Ta1 Cs1 151.48(4) 2_655 . ?
Ta2 Ta1 K1 110.69(10) 2_655 . ?
K1 Ta1 Cs1 97.81(10) . . ?
O2 Ta1 Ta2 122.2(4) . 2_655 ?
O2 Ta1 Cs1 46.9(4) . . ?
O2 Ta1 K1 101.8(4) . . ?
O2 Ta1 O10 88.5(5) . 2_655 ?
O2 Ta1 O12 157.3(5) . 2_655 ?
O2 Ta1 O17 85.7(5) . 2_655 ?
O7 Ta1 Ta2 154.5(4) . 2_655 ?
O7 Ta1 Cs1 53.1(4) . . ?
O7 Ta1 K1 46.2(4) . . ?
O7 Ta1 O2 78.7(6) . . ?
O7 Ta1 O10 85.9(5) . 2_655 ?
O7 Ta1 O11 45.6(5) . . ?
O7 Ta1 O12 123.9(6) . 2_655 ?
O7 Ta1 O17 158.7(5) . 2_655 ?
O10 Ta1 Ta2 80.8(3) 2_655 2_655 ?
O10 Ta1 Cs1 120.2(3) 2_655 . ?
O10 Ta1 K1 47.3(3) 2_655 . ?
O10 Ta1 O12 90.6(5) 2_655 2_655 ?
O10 Ta1 O17 79.3(5) 2_655 2_655 ?
O11 Ta1 Ta2 112.3(4) . 2_655 ?
O11 Ta1 Cs1 88.5(4) . . ?
O11 Ta1 K1 44.8(4) . . ?
O11 Ta1 O2 124.3(5) . . ?
O11 Ta1 O10 89.5(5) . 2_655 ?
O11 Ta1 O12 78.4(5) . 2_655 ?
O11 Ta1 O17 147.9(5) . 2_655 ?
O12 Ta1 Ta2 35.5(4) 2_655 2_655 ?
O12 Ta1 Cs1 146.6(3) 2_655 . ?
O12 Ta1 K1 94.2(4) 2_655 . ?
O15 Ta1 Ta2 95.9(4) . 2_655 ?
O15 Ta1 Cs1 60.8(4) . . ?
O15 Ta1 K1 140.0(4) . . ?
O15 Ta1 O2 87.6(5) . . ?
O15 Ta1 O7 99.6(5) . . ?
O15 Ta1 O10 172.4(5) . 2_655 ?
O15 Ta1 O11 98.0(6) . . ?
O15 Ta1 O12 90.5(5) . 2_655 ?
O15 Ta1 O17 94.0(5) . 2_655 ?
O17 Ta1 Ta2 36.5(3) 2_655 2_655 ?
O17 Ta1 Cs1 123.1(3) 2_655 . ?
O17 Ta1 K1 125.2(3) 2_655 . ?
O17 Ta1 O12 71.8(5) 2_655 2_655 ?
Ta1 Ta2 Ta3 72.82(3) 2_655 . ?
Ta1 Ta2 Cs1 116.94(4) 2_655 3_455 ?
Ta3 Ta2 Cs1 122.43(3) . 3_455 ?
O1 Ta2 Ta1 119.4(5) . 2_655 ?
O1 Ta2 Ta3 161.5(4) . . ?
O1 Ta2 Cs1 40.9(4) . 3_455 ?
O1 Ta2 O4 45.7(6) . . ?
O1 Ta2 O8 128.6(6) . . ?
O1 Ta2 O9 89.0(6) . . ?
O1 Ta2 O12 83.3(6) . . ?
O1 Ta2 O17 156.2(6) . . ?
O4 Ta2 Ta1 162.0(4) . 2_655 ?
O4 Ta2 Ta3 119.0(4) . . ?
O4 Ta2 Cs1 45.8(4) . 3_455 ?
O4 Ta2 O8 83.0(6) . . ?
O4 Ta2 O9 88.7(5) . . ?
O4 Ta2 O12 128.8(6) . . ?
O4 Ta2 O17 155.8(5) . . ?
O6 Ta2 Ta1 96.7(4) . 2_655 ?
O6 Ta2 Ta3 96.0(4) . . ?
O6 Ta2 Cs1 134.0(5) . 3_455 ?
O6 Ta2 O1 96.1(6) . . ?
O6 Ta2 O4 95.5(6) . . ?
O6 Ta2 O8 91.9(4) . . ?
O6 Ta2 O9 174.8(7) . . ?
O6 Ta2 O12 94.4(4) . . ?
O6 Ta2 O17 91.2(6) . . ?
O8 Ta2 Ta1 109.8(4) . 2_655 ?
O8 Ta2 Ta3 36.9(4) . . ?
O8 Ta2 Cs1 103.9(4) . 3_455 ?
O8 Ta2 O9 85.5(5) . . ?
O8 Ta2 O17 73.5(5) . . ?
O9 Ta2 Ta1 79.9(4) . 2_655 ?
O9 Ta2 Ta3 79.2(4) . . ?
O9 Ta2 Cs1 51.2(4) . 3_455 ?
O12 Ta2 Ta1 36.8(4) . 2_655 ?
O12 Ta2 Ta3 109.6(4) . . ?
O12 Ta2 Cs1 95.1(4) . 3_455 ?
O12 Ta2 O8 146.5(5) . . ?
O12 Ta2 O9 85.3(5) . . ?
O12 Ta2 O17 73.5(5) . . ?
O17 Ta2 Ta1 36.9(3) . 2_655 ?
O17 Ta2 Ta3 37.0(3) . . ?
O17 Ta2 Cs1 134.6(3) . 3_455 ?
O17 Ta2 O9 83.8(5) . . ?
Ta2 Ta3 Cs1 123.62(4) . 5_666 ?
Ta2 Ta3 Cs1 149.18(3) . . ?
Cs1 Ta3 Cs1 83.18(4) . 5_666 ?
O5 Ta3 Ta2 124.3(4) 2_655 . ?
O5 Ta3 Cs1 70.9(4) 2_655 5_666 ?
O5 Ta3 Cs1 45.0(4) 2_655 . ?
O5 Ta3 O8 160.2(6) 2_655 . ?
O5 Ta3 O16 87.2(5) 2_655 . ?
O5 Ta3 O17 88.2(5) 2_655 . ?
O8 Ta3 Ta2 36.1(4) . . ?
O8 Ta3 Cs1 147.0(4) . . ?
O8 Ta3 Cs1 119.1(4) . 5_666 ?
O13 Ta3 Ta2 154.5(4) . . ?
O13 Ta3 Cs1 45.6(4) . 5_666 ?
O13 Ta3 Cs1 55.1(4) . . ?
O13 Ta3 O5 77.4(6) . 2_655 ?
O13 Ta3 O8 122.0(6) . . ?
O13 Ta3 O16 89.5(5) . . ?
O13 Ta3 O17 162.4(5) . . ?
O14 Ta3 Ta2 113.2(4) . . ?
O14 Ta3 Cs1 68.6(4) . 5_666 ?
O14 Ta3 Cs1 89.5(4) . . ?
O14 Ta3 O5 121.3(6) . 2_655 ?
O14 Ta3 O8 78.3(6) . . ?
O14 Ta3 O13 43.9(5) . . ?
O14 Ta3 O16 92.7(5) . . ?
O14 Ta3 O17 149.3(5) . . ?
O15 Ta3 Ta2 96.2(4) . . ?
O15 Ta3 Cs1 140.1(4) . 5_666 ?
O15 Ta3 Cs1 59.2(4) . . ?
O15 Ta3 O5 88.8(5) . 2_655 ?
O15 Ta3 O8 91.5(5) . . ?
O15 Ta3 O13 97.6(5) . . ?
O15 Ta3 O14 96.4(6) . . ?
O15 Ta3 O16 170.9(5) . . ?
O15 Ta3 O17 92.1(5) . . ?
O16 Ta3 Ta2 79.4(4) . . ?
O16 Ta3 Cs1 45.2(4) . 5_666 ?
O16 Ta3 Cs1 121.9(4) . . ?
O16 Ta3 O8 89.5(5) . . ?
O16 Ta3 O17 79.6(5) . . ?
O17 Ta3 Ta2 36.3(3) . . ?
O17 Ta3 Cs1 120.0(3) . 5_666 ?
O17 Ta3 Cs1 119.9(3) . . ?
O17 Ta3 O8 72.1(5) . . ?
O9 Se1 Cs1 130.8(5) . 5_666 ?
O9 Se1 O10 103.1(6) . . ?
O9 Se1 O16 99.6(7) . . ?
O10 Se1 Cs1 110.4(4) . 5_666 ?
O16 Se1 Cs1 39.4(4) . 5_666 ?
O16 Se1 O10 102.5(6) . . ?
Cs1 Se2 Cs1 110.61(6) 2_655 . ?
O2 Se2 Cs1 42.2(5) . . ?
O2 Se2 Cs1 117.6(5) . 2_655 ?
O2 Se2 O5 99.8(7) . . ?
O3 Se2 Cs1 59.5(6) . 2_655 ?
O3 Se2 Cs1 64.3(5) . . ?
O3 Se2 O2 100.9(7) . . ?
O3 Se2 O5 101.4(7) . . ?
O5 Se2 Cs1 125.6(5) . . ?
O5 Se2 Cs1 43.8(5) . 2_655 ?
O1 Cs1 O2 65.5(4) 3_545 . ?
O1 Cs1 O3 98.9(4) 3_545 2_655 ?
O1 Cs1 O4 27.3(4) 3_545 3_545 ?
O1 Cs1 O5 127.2(4) 3_545 2_655 ?
O1 Cs1 O7 61.3(4) 3_545 . ?
O1 Cs1 O9 50.6(4) 3_545 3_545 ?
O1 Cs1 O13 140.3(4) 3_545 5_666 ?
O1 Cs1 O13 151.4(4) 3_545 . ?
O1 Cs1 O15 104.4(3) 3_545 . ?
O1 Cs1 O16 110.2(4) 3_545 5_666 ?
O1 Cs1 O5W 82.8(5) 3_545 . ?
O2 Cs1 O3 66.6(3) . 2_655 ?
O2 Cs1 O4 85.7(3) . 3_545 ?
O2 Cs1 O7 45.3(3) . . ?
O2 Cs1 O9 109.6(3) . 3_545 ?
O2 Cs1 O13 91.5(3) . . ?
O2 Cs1 O13 122.6(4) . 5_666 ?
O2 Cs1 O15 46.5(3) . . ?
O2 Cs1 O5W 117.6(5) . . ?
O3 Cs1 O15 83.1(3) 2_655 . ?
O4 Cs1 O3 125.2(4) 3_545 2_655 ?
O4 Cs1 O7 62.0(3) 3_545 . ?
O4 Cs1 O9 49.8(3) 3_545 3_545 ?
O4 Cs1 O13 143.4(3) 3_545 . ?
O4 Cs1 O15 111.3(3) 3_545 . ?
O5 Cs1 O2 64.8(4) 2_655 . ?
O5 Cs1 O3 44.8(4) 2_655 2_655 ?
O5 Cs1 O4 150.4(4) 2_655 3_545 ?
O5 Cs1 O7 94.0(4) 2_655 . ?
O5 Cs1 O9 139.5(4) 2_655 3_545 ?
O5 Cs1 O13 63.1(4) 2_655 5_666 ?
O5 Cs1 O13 43.6(3) 2_655 . ?
O5 Cs1 O15 47.3(3) 2_655 . ?
O5 Cs1 O16 115.2(4) 2_655 5_666 ?
O5 Cs1 O5W 136.7(5) 2_655 . ?
O7 Cs1 O3 111.7(3) . 2_655 ?
O7 Cs1 O9 109.5(3) . 3_545 ?
O7 Cs1 O13 90.7(3) . . ?
O7 Cs1 O15 49.3(3) . . ?
O9 Cs1 O3 95.1(3) 3_545 2_655 ?
O9 Cs1 O13 157.5(3) 3_545 . ?
O9 Cs1 O15 154.5(3) 3_545 . ?
O13 Cs1 O3 86.0(3) . 2_655 ?
O13 Cs1 O3 60.1(3) 5_666 2_655 ?
O13 Cs1 O4 143.0(4) 5_666 3_545 ?
O13 Cs1 O7 154.9(4) 5_666 . ?
O13 Cs1 O9 95.2(3) 5_666 3_545 ?
O13 Cs1 O13 65.9(4) 5_666 . ?
O13 Cs1 O15 48.0(3) . . ?
O13 Cs1 O15 105.7(3) 5_666 . ?
O16 Cs1 O2 168.6(4) 5_666 . ?
O16 Cs1 O3 104.9(3) 5_666 2_655 ?
O16 Cs1 O4 94.0(3) 5_666 3_545 ?
O16 Cs1 O7 143.2(3) 5_666 . ?
O16 Cs1 O9 62.5(3) 5_666 3_545 ?
O16 Cs1 O13 95.5(3) 5_666 . ?
O16 Cs1 O13 53.4(4) 5_666 5_666 ?
O16 Cs1 O15 142.6(3) 5_666 . ?
O16 Cs1 O5W 70.9(5) 5_666 . ?
O5W Cs1 O3 175.7(5) . 2_655 ?
O5W Cs1 O4 56.0(5) . 3_545 ?
O5W Cs1 O7 72.5(5) . . ?
O5W Cs1 O9 82.9(5) . 3_545 ?
O5W Cs1 O13 116.2(5) . 5_666 ?
O5W Cs1 O13 94.4(5) . . ?
O5W Cs1 O15 100.3(5) . . ?
Ta1 K1 Ta1 168.6(2) 2_755 . ?
O7 K1 Ta1 28.7(3) 2_755 2_755 ?
O7 K1 Ta1 157.9(3) 2_755 . ?
O7 K1 Ta1 157.9(3) . 2_755 ?
O7 K1 Ta1 28.7(3) . . ?
O7 K1 O7 151.6(6) 2_755 . ?
O7 K1 O10 55.6(4) 2_755 1_655 ?
O7 K1 O10 128.2(4) 2_755 2_655 ?
O7 K1 O10 128.2(4) . 1_655 ?
O7 K1 O10 55.6(4) . 2_655 ?
O10 K1 Ta1 146.5(3) 1_655 . ?
O10 K1 Ta1 146.5(3) 2_655 2_755 ?
O10 K1 Ta1 31.2(2) 2_655 . ?
O10 K1 Ta1 31.2(2) 1_655 2_755 ?
O10 K1 O10 167.7(6) 1_655 2_655 ?
O11 K1 Ta1 28.8(3) 2_755 2_755 ?
O11 K1 Ta1 145.5(3) . 2_755 ?
O11 K1 Ta1 145.5(3) 2_755 . ?
O11 K1 Ta1 28.8(3) . . ?
O11 K1 O7 30.3(4) 2_755 2_755 ?
O11 K1 O7 173.3(4) 2_755 . ?
O11 K1 O7 30.3(4) . . ?
O11 K1 O7 173.3(4) . 2_755 ?
O11 K1 O10 58.5(4) . 2_655 ?
O11 K1 O10 117.8(4) 2_755 2_655 ?
O11 K1 O10 117.8(4) . 1_655 ?
O11 K1 O10 58.5(4) 2_755 1_655 ?
O11 K1 O11 149.4(6) 2_755 . ?
O11 K1 O4W 66.4(5) . . ?
O11 K1 O4W 87.1(5) 2_755 . ?
O11 K1 O4W 66.4(5) 2_755 2_755 ?
O11 K1 O4W 87.1(5) . 2_755 ?
O3W K1 Ta1 108.0(4) . 2_755 ?
O3W K1 Ta1 108.0(4) 2_755 . ?
O3W K1 Ta1 81.7(4) 2_755 2_755 ?
O3W K1 Ta1 81.7(4) . . ?
O3W K1 O7 76.2(5) 2_755 2_755 ?
O3W K1 O7 76.2(5) . . ?
O3W K1 O7 80.2(5) . 2_755 ?
O3W K1 O7 80.2(5) 2_755 . ?
O3W K1 O10 122.8(5) 2_755 2_655 ?
O3W K1 O10 68.7(5) . 2_655 ?
O3W K1 O10 122.8(5) . 1_655 ?
O3W K1 O10 68.7(5) 2_755 1_655 ?
O3W K1 O11 104.5(5) . . ?
O3W K1 O11 101.0(5) . 2_755 ?
O3W K1 O11 104.5(5) 2_755 2_755 ?
O3W K1 O11 101.0(5) 2_755 . ?
O3W K1 O3W 66.7(8) 2_755 . ?
O3W K1 O4W 115.8(6) 2_755 . ?
O3W K1 O4W 170.7(5) . . ?
O3W K1 O4W 170.7(5) 2_755 2_755 ?
O3W K1 O4W 115.8(6) . 2_755 ?
O4W K1 Ta1 89.0(4) . . ?
O4W K1 Ta1 89.0(4) 2_755 2_755 ?
O4W K1 Ta1 81.3(4) 2_755 . ?
O4W K1 Ta1 81.3(4) . 2_755 ?
O4W K1 O7 95.2(5) 2_755 2_755 ?
O4W K1 O7 95.2(5) . . ?
O4W K1 O7 109.1(5) . 2_755 ?
O4W K1 O7 109.0(5) 2_755 . ?
O4W K1 O10 103.6(5) . 2_655 ?
O4W K1 O10 65.3(5) . 1_655 ?
O4W K1 O10 103.6(5) 2_755 1_655 ?
O4W K1 O10 65.3(5) 2_755 2_655 ?
O4W K1 O4W 63.2(8) 2_755 . ?
Ta2 O1 Cs1 115.2(6) . 3_455 ?
O4 O1 Ta2 68.1(8) . . ?
O4 O1 Cs1 81.7(8) . 3_455 ?
Ta1 O2 Cs1 105.1(5) . . ?
Se2 O2 Ta1 136.0(8) . . ?
Se2 O2 Cs1 116.9(6) . . ?
Se2 O3 Cs1 97.1(6) . 2_655 ?
Se2 O3 Cs1 92.3(6) . . ?
Cs1 O3 Cs1 136.5(4) 2_655 . ?
Ta2 O4 Cs1 108.7(5) . 3_455 ?
O1 O4 Ta2 66.2(8) . . ?
O1 O4 Cs1 71.0(8) . 3_455 ?
Ta3 O5 Cs1 107.8(6) 2_655 2_655 ?
Se2 O5 Ta3 137.7(8) . 2_655 ?
Se2 O5 Cs1 114.2(6) . 2_655 ?
Ta2 O6 Ta2 164.1(11) . 2_655 ?
Ta1 O7 Cs1 99.4(5) . . ?
Ta1 O7 K1 105.1(5) . . ?
K1 O7 Cs1 150.0(5) . . ?
O11 O7 Ta1 67.8(7) . . ?
O11 O7 Cs1 133.6(8) . . ?
O11 O7 K1 73.0(7) . . ?
Ta2 O8 Ta3 107.0(6) . . ?
Ta2 O9 Cs1 100.7(5) . 3_455 ?
Se1 O9 Ta2 128.3(7) . . ?
Se1 O9 Cs1 130.5(6) . 3_455 ?
Ta1 O10 K1 101.5(5) 2_655 1_455 ?
Se1 O10 Ta1 131.6(7) . 2_655 ?
Se1 O10 K1 117.6(6) . 1_455 ?
Ta1 O11 K1 106.4(5) . . ?
O7 O11 Ta1 66.5(7) . . ?
O7 O11 K1 76.8(7) . . ?
Ta2 O12 Ta1 107.7(6) . 2_655 ?
Ta3 O13 Cs1 97.7(5) . . ?
Ta3 O13 Cs1 108.6(5) . 5_666 ?
Cs1 O13 Cs1 114.1(4) 5_666 . ?
O14 O13 Ta3 67.9(8) . . ?
O14 O13 Cs1 111.5(8) . 5_666 ?
O14 O13 Cs1 134.4(9) . . ?
O13 O14 Ta3 68.2(8) . . ?
Ta1 O15 Ta3 159.7(8) . . ?
Ta1 O15 Cs1 92.2(4) . . ?
Ta3 O15 Cs1 94.0(4) . . ?
Ta3 O16 Cs1 106.6(5) . 5_666 ?
Se1 O16 Ta3 131.9(7) . . ?
Se1 O16 Cs1 120.7(6) . 5_666 ?
Ta1 O17 Ta3 142.3(6) 2_655 . ?
Ta2 O17 Ta1 106.5(5) . 2_655 ?
Ta2 O17 Ta3 106.7(5) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy5_a
_database_code_depnum_ccdc_archive 'CCDC 1893230'
loop_
_audit_author_name
_audit_author_address
ddzhang
;Henan University
China
;
_audit_update_record             
;
2019-01-24 deposited with the CCDC.	2020-02-27 downloaded from the CCDC.
;
_audit_creation_date             2018-02-09
_audit_creation_method           
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs Er K O46 Se4 Ta6, 4(O)'
_chemical_formula_sum            'Cs Er K O50 Se4 Ta6'
_chemical_formula_weight         2540.81
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -0.2586 4.9576 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.2890(5)
_cell_length_b                   27.3478(11)
_cell_length_c                   13.9854(6)
_cell_angle_alpha                90
_cell_angle_beta                 114.0310(10)
_cell_angle_gamma                90
_cell_volume                     4292.8(3)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    8557
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.29
_cell_measurement_theta_min      2.39
_shelx_estimated_absorpt_T_max   0.181
_shelx_estimated_absorpt_T_min   0.087
_exptl_absorpt_coefficient_mu    21.617
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.2992
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1303 before and 0.0512 after correction.
The Ratio of minimum to maximum transmission is 0.4012.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.931
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4464
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.12
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0405
_diffrn_reflns_av_unetI/netI     0.0455
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            22080
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.814
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                6674
_reflns_number_total             7625
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         1.999
_refine_diff_density_min         -4.532
_refine_diff_density_rms         0.338
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.038
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7625
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0468
_refine_ls_R_factor_gt           0.0394
_refine_ls_restrained_S_all      1.038
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0427P)²+108.9842P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0954
_refine_ls_wR_factor_ref         0.0994
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28594(4) 0.54917(2) 0.55589(4) 0.01005(12) Uani 1 1 d . . . . .
Ta2 Ta 0.43746(4) 0.65816(2) 0.47009(4) 0.01014(12) Uani 1 1 d . . . . .
Ta3 Ta 0.17177(4) 0.60799(2) 0.32797(4) 0.01037(12) Uani 1 1 d . . . . .
Ta4 Ta 0.13666(4) 0.64101(2) 0.66476(4) 0.01048(12) Uani 1 1 d . . . . .
Ta5 Ta 0.28238(4) 0.75190(2) 0.57490(4) 0.01091(12) Uani 1 1 d . . . . .
Ta6 Ta 0.03104(4) 0.70139(2) 0.43795(4) 0.01284(12) Uani 1 1 d . . . . .
Er1 Er 0.68424(5) 0.64983(2) 0.98531(4) 0.01475(13) Uani 1 1 d . . . . .
Se1 Se 0.41777(11) 0.53776(5) 0.38144(9) 0.0150(3) Uani 1 1 d . . . . .
Se2 Se 0.04913(11) 0.76035(5) 0.65930(9) 0.0146(3) Uani 1 1 d . . . . .
Se3 Se 0.37747(10) 0.71176(4) 0.82835(9) 0.0126(2) Uani 1 1 d . . . . .
Se4 Se 0.49209(11) 0.62457(5) 0.71390(9) 0.0155(3) Uani 1 1 d . . . . .
Cs1 Cs -0.18182(11) 0.66399(5) 0.72007(11) 0.0578(3) Uani 1 1 d . . . . .
K1 K 0.2245(4) 0.57325(17) 0.0688(3) 0.0538(11) Uani 1 1 d . . . . .
O1 O 0.6182(8) 0.6147(4) 0.8167(7) 0.023(2) Uiso 1 1 d . . . . .
O2 O 0.3888(10) 0.8000(4) 0.5498(8) 0.038(3) Uiso 1 1 d . . . . .
O3 O -0.1390(8) 0.6931(4) 0.3423(7) 0.024(2) Uiso 1 1 d . . . . .
O4 O 0.5083(8) 0.6879(3) 0.8976(7) 0.0189(19) Uiso 1 1 d . . . . .
O5 O 0.5024(8) 0.6937(4) 0.3816(7) 0.023(2) Uiso 1 1 d . . . . .
O6 O 0.5956(8) 0.6848(3) 0.4888(7) 0.0194(19) Uiso 1 1 d . . . . .
O7 O -0.0812(8) 0.7370(4) 0.3151(7) 0.026(2) Uiso 1 1 d . . . . .
O8 O 0.0946(8) 0.6204(3) 0.1761(7) 0.021(2) Uiso 1 1 d . . . . .
O9 O 0.5437(8) 0.6373(3) 0.6205(7) 0.021(2) Uiso 1 1 d . . . . .
O10 O 0.1254(8) 0.6051(3) 0.7847(7) 0.022(2) Uiso 1 1 d . . . . .
O11 O 0.3181(10) 0.8213(5) 0.6021(9) 0.045(3) Uiso 1 1 d . . . . .
O12 O 0.0305(8) 0.5805(4) 0.2118(7) 0.023(2) Uiso 1 1 d . . . . .
O13 O 0.0703(7) 0.7030(3) 0.7107(7) 0.0179(19) Uiso 1 1 d . . . . .
O14 O 0.0165(8) 0.5998(3) 0.6867(7) 0.022(2) Uiso 1 1 d . . . . .
O15 O 0.2962(8) 0.6598(3) 0.7838(7) 0.0189(19) Uiso 1 1 d . . . . .
O16 O 0.2026(8) 0.4868(3) 0.5510(7) 0.023(2) Uiso 1 1 d . . . . .
O17 O 0.3989(7) 0.7285(3) 0.7186(6) 0.0155(18) Uiso 1 1 d . . . . .
O18 O 0.3181(8) 0.4895(3) 0.6459(7) 0.020(2) Uiso 1 1 d . . . . .
O19 O 0.0881(7) 0.6576(3) 0.3630(6) 0.0158(18) Uiso 1 1 d . . . . .
O20 O 0.2816(8) 0.5583(3) 0.2968(7) 0.0185(19) Uiso 1 1 d . . . . .
O21 O -0.0278(7) 0.7486(3) 0.5294(6) 0.0157(18) Uiso 1 1 d . . . . .
O22 O 0.2103(7) 0.5882(3) 0.6233(6) 0.0156(18) Uiso 1 1 d . . . . .
O23 O 0.1874(7) 0.7756(3) 0.6667(7) 0.0185(19) Uiso 1 1 d . . . . .
O24 O 0.4482(7) 0.5651(3) 0.6761(6) 0.0158(18) Uiso 1 1 d . . . . .
O25 O 0.3832(7) 0.5176(3) 0.4821(6) 0.0150(18) Uiso 1 1 d . . . . .
O26 O 0.3717(7) 0.7086(3) 0.5170(6) 0.0168(18) Uiso 1 1 d . . . . .
O27 O 0.4934(7) 0.5903(3) 0.4274(6) 0.0171(19) Uiso 1 1 d . . . . .
O28 O 0.1434(7) 0.7564(3) 0.4467(6) 0.0159(18) Uiso 1 1 d . . . . .
O29 O -0.0069(7) 0.6458(3) 0.5205(6) 0.0167(19) Uiso 1 1 d . . . . .
O30 O 0.1399(7) 0.5547(3) 0.4142(6) 0.0170(19) Uiso 1 1 d . . . . .
O31 O 0.1808(7) 0.6899(3) 0.5758(6) 0.0095(16) Uiso 1 1 d . . . . .
O32 O 0.2940(7) 0.6580(3) 0.3240(6) 0.0163(18) Uiso 1 1 d . . . . .
O33 O 0.3090(7) 0.6095(3) 0.4776(6) 0.0117(17) Uiso 1 1 d . . . . .
O1W O 0.5633(9) 0.6382(4) 1.0799(8) 0.033(2) Uiso 1 1 d . . . . .
O2W O 0.7005(9) 0.7262(4) 1.0803(8) 0.036(3) Uiso 1 1 d . . . . .
O3W O 0.8270(9) 0.6385(4) 1.1580(8) 0.036(3) Uiso 1 1 d . . . . .
O4W O 0.7575(10) 0.7100(4) 0.9090(8) 0.038(3) Uiso 1 1 d . . . . .
O5W O -0.0450(10) 0.4993(4) 0.3469(9) 0.041(3) Uiso 1 1 d . . . . .
O6W O 0.6300(10) 0.7676(5) 0.7522(9) 0.045(3) Uiso 1 1 d . . . . .
O7W O -0.2180(13) 0.6129(6) 0.4956(12) 0.071(4) Uiso 1 1 d . . . . .
O8W O 0.0503(12) 0.6463(5) 0.9281(11) 0.058(4) Uiso 1 1 d . . . . .
O9W O 0.8587(10) 0.6165(4) 0.9757(9) 0.043(3) Uiso 1 1 d . . . . .
O10W O 0.6730(10) 0.5662(4) 1.0055(9) 0.042(3) Uiso 1 1 d . . . . .
O11W O 0.5840(11) 0.4980(5) 0.8456(10) 0.053(3) Uiso 1 1 d . . . . .
O12W O 0.3628(12) 0.5805(5) -0.0558(11) 0.059(4) Uiso 1 1 d . . . . .
O13W O 0.0940(14) 0.5160(6) -0.1027(12) 0.071(4) Uiso 1 1 d . . . . .
O14W O 0.3550(13) 0.4916(6) 0.8544(11) 0.065(4) Uiso 1 1 d . . . . .
O15W O 0.6009(18) 0.6152(8) 1.2767(16) 0.109(7) Uiso 1 1 d . . . . .
O16W O 0.276(2) 0.4420(9) 0.3327(18) 0.123(7) Uiso 1 1 d . . . . .
O17W O 0.1404(19) 0.4700(8) 0.1273(17) 0.113(7) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3278(7) . ?
Ta1 O16 1.975(9) . ?
Ta1 O18 2.000(9) . ?
Ta1 O22 1.899(8) . ?
Ta1 O24 2.065(8) . ?
Ta1 O25 2.060(8) . ?
Ta1 O30 2.067(8) . ?
Ta1 O33 2.062(8) . ?
Ta2 Ta3 3.3479(7) . ?
Ta2 Cs1 4.5624(14) 1_655 ?
Ta2 O5 1.980(9) . ?
Ta2 O6 1.990(9) . ?
Ta2 O9 2.054(9) . ?
Ta2 O26 1.848(9) . ?
Ta2 O27 2.147(9) . ?
Ta2 O32 2.085(8) . ?
Ta2 O33 2.100(8) . ?
Ta3 K1 4.046(4) . ?
Ta3 O8 1.971(9) . ?
Ta3 O12 1.981(9) . ?
Ta3 O19 1.883(8) . ?
Ta3 O20 2.082(9) . ?
Ta3 O30 2.029(9) . ?
Ta3 O32 2.049(9) . ?
Ta3 O33 2.086(8) . ?
Ta4 Ta6 3.3346(7) . ?
Ta4 Cs1 4.3333(13) . ?
Ta4 O10 1.997(9) . ?
Ta4 O13 2.092(9) . ?
Ta4 O14 1.978(9) . ?
Ta4 O15 2.055(9) . ?
Ta4 O22 1.915(9) . ?
Ta4 O29 2.074(8) . ?
Ta4 O31 2.044(8) . ?
Ta5 Ta6 3.2091(7) . ?
Ta5 O2 1.984(11) . ?
Ta5 O11 1.951(13) . ?
Ta5 O17 2.038(8) . ?
Ta5 O23 2.156(9) . ?
Ta5 O26 1.997(9) . ?
Ta5 O28 1.912(8) . ?
Ta5 O31 2.109(8) . ?
Ta6 O3 1.983(9) . ?
Ta6 O7 1.968(9) . ?
Ta6 O19 1.905(8) . ?
Ta6 O21 2.139(8) . ?
Ta6 O28 2.012(9) . ?
Ta6 O29 2.073(9) . ?
Ta6 O31 2.077(8) . ?
Er1 Cs1 4.6466(15) 1_655 ?
Er1 O1 2.364(9) . ?
Er1 O4 2.259(9) . ?
Er1 O1W 2.379(10) . ?
Er1 O2W 2.440(11) . ?
Er1 O3W 2.357(11) . ?
Er1 O4W 2.331(11) . ?
Er1 O9W 2.383(12) . ?
Er1 O10W 2.316(12) . ?
Se1 O20 1.704(9) . ?
Se1 O25 1.719(8) . ?
Se1 O27 1.689(9) . ?
Se2 Cs1 4.2055(18) . ?
Se2 O13 1.701(9) . ?
Se2 O21 1.703(8) . ?
Se2 O23 1.712(9) . ?
Se3 O4 1.637(9) . ?
Se3 O15 1.702(9) . ?
Se3 O17 1.722(8) . ?
Se4 Cs1 4.1166(17) 1_655 ?
Se4 O1 1.651(9) . ?
Se4 O9 1.705(9) . ?
Se4 O24 1.726(9) . ?
Cs1 O1 3.520(9) 1_455 ?
Cs1 O6 3.326(9) 1_455 ?
Cs1 O7 3.048(10) 4_576 ?
Cs1 O9 3.165(9) 1_455 ?
Cs1 O13 3.329(9) . ?
Cs1 O14 3.188(9) . ?
Cs1 O2W 3.553(11) 4_475 ?
Cs1 O4W 3.275(11) 1_455 ?
Cs1 O7W 3.297(15) . ?
Cs1 O8W 3.174(14) . ?
Cs1 O9W 3.642(12) 1_455 ?
Cs1 O16W 3.10(2) 3_566 ?
K1 O8 2.900(10) . ?
K1 O11 3.068(14) 4_575 ?
K1 O20 3.000(9) . ?
K1 O8W 3.002(14) 1_554 ?
K1 O11W 2.912(14) 3_666 ?
K1 O12W 2.895(14) . ?
K1 O13W 2.765(16) . ?
K1 O17W 3.22(2) . ?
O2 O11 1.466(16) . ?
O3 O7 1.520(13) . ?
O5 O6 1.490(12) . ?
O8 O12 1.543(13) . ?
O10 O14 1.482(12) . ?
O16 O18 1.499(12) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Ta1 Ta3 111.9(3) . . ?
O16 Ta1 O18 44.3(4) . . ?
O16 Ta1 O24 121.7(4) . . ?
O16 Ta1 O25 91.1(4) . . ?
O16 Ta1 O30 78.1(4) . . ?
O16 Ta1 O33 148.6(3) . . ?
O18 Ta1 Ta3 153.6(3) . . ?
O18 Ta1 O24 77.4(3) . . ?
O18 Ta1 O25 88.1(3) . . ?
O18 Ta1 O30 122.3(4) . . ?
O18 Ta1 O33 162.3(3) . . ?
O22 Ta1 Ta3 95.9(3) . . ?
O22 Ta1 O16 98.7(4) . . ?
O22 Ta1 O18 99.0(4) . . ?
O22 Ta1 O24 89.0(3) . . ?
O22 Ta1 O25 170.2(4) . . ?
O22 Ta1 O30 91.4(3) . . ?
O22 Ta1 O33 90.8(3) . . ?
O24 Ta1 Ta3 124.6(2) . . ?
O24 Ta1 O30 159.8(3) . . ?
O25 Ta1 Ta3 80.0(2) . . ?
O25 Ta1 O24 86.1(3) . . ?
O25 Ta1 O30 90.3(3) . . ?
O25 Ta1 O33 80.6(3) . . ?
O30 Ta1 Ta3 35.3(2) . . ?
O33 Ta1 Ta3 36.9(2) . . ?
O33 Ta1 O24 88.1(3) . . ?
O33 Ta1 O30 71.7(3) . . ?
Ta3 Ta2 Cs1 156.50(2) . 1_655 ?
O5 Ta2 Ta3 112.0(3) . . ?
O5 Ta2 Cs1 85.0(3) . 1_655 ?
O5 Ta2 O6 44.1(4) . . ?
O5 Ta2 O9 121.8(4) . . ?
O5 Ta2 O27 89.7(4) . . ?
O5 Ta2 O32 77.5(3) . . ?
O5 Ta2 O33 147.7(3) . . ?
O6 Ta2 Ta3 153.1(2) . . ?
O6 Ta2 Cs1 41.0(2) . 1_655 ?
O6 Ta2 O9 77.7(4) . . ?
O6 Ta2 O27 87.0(3) . . ?
O6 Ta2 O32 121.3(3) . . ?
O6 Ta2 O33 159.9(3) . . ?
O9 Ta2 Ta3 123.7(3) . . ?
O9 Ta2 Cs1 36.8(3) . 1_655 ?
O9 Ta2 O27 84.4(3) . . ?
O9 Ta2 O32 159.1(4) . . ?
O9 Ta2 O33 87.2(3) . . ?
O26 Ta2 Ta3 93.1(3) . . ?
O26 Ta2 Cs1 99.3(3) . 1_655 ?
O26 Ta2 O5 101.6(4) . . ?
O26 Ta2 O6 103.0(4) . . ?
O26 Ta2 O9 91.8(4) . . ?
O26 Ta2 O27 168.3(4) . . ?
O26 Ta2 O32 91.8(4) . . ?
O26 Ta2 O33 90.5(3) . . ?
O27 Ta2 Ta3 80.0(2) . . ?
O27 Ta2 Cs1 84.2(2) . 1_655 ?
O32 Ta2 Ta3 35.6(2) . . ?
O32 Ta2 Cs1 160.9(2) . 1_655 ?
O32 Ta2 O27 88.0(3) . . ?
O32 Ta2 O33 72.2(3) . . ?
O33 Ta2 Ta3 36.7(2) . . ?
O33 Ta2 Cs1 122.7(2) . 1_655 ?
O33 Ta2 O27 78.4(3) . . ?
Ta1 Ta3 Ta2 72.580(15) . . ?
Ta1 Ta3 K1 125.85(6) . . ?
Ta2 Ta3 K1 98.91(7) . . ?
O8 Ta3 Ta1 161.0(3) . . ?
O8 Ta3 Ta2 119.6(3) . . ?
O8 Ta3 K1 42.0(3) . . ?
O8 Ta3 O12 46.0(4) . . ?
O8 Ta3 O20 87.4(4) . . ?
O8 Ta3 O30 129.7(4) . . ?
O8 Ta3 O32 83.8(4) . . ?
O8 Ta3 O33 156.3(3) . . ?
O12 Ta3 Ta1 119.3(3) . . ?
O12 Ta3 Ta2 163.7(3) . . ?
O12 Ta3 K1 65.3(3) . . ?
O12 Ta3 O20 90.4(4) . . ?
O12 Ta3 O30 84.1(4) . . ?
O12 Ta3 O32 129.7(4) . . ?
O12 Ta3 O33 155.6(4) . . ?
O19 Ta3 Ta1 99.3(3) . . ?
O19 Ta3 Ta2 93.1(3) . . ?
O19 Ta3 K1 134.9(3) . . ?
O19 Ta3 O8 94.7(4) . . ?
O19 Ta3 O12 95.6(4) . . ?
O19 Ta3 O20 173.3(4) . . ?
O19 Ta3 O30 96.0(4) . . ?
O19 Ta3 O32 90.6(4) . . ?
O19 Ta3 O33 91.6(3) . . ?
O20 Ta3 Ta1 80.2(2) . . ?
O20 Ta3 Ta2 80.4(2) . . ?
O20 Ta3 K1 46.0(2) . . ?
O20 Ta3 O33 84.0(3) . . ?
O30 Ta3 Ta1 36.1(2) . . ?
O30 Ta3 Ta2 108.6(2) . . ?
O30 Ta3 K1 120.3(3) . . ?
O30 Ta3 O20 87.4(3) . . ?
O30 Ta3 O32 144.8(3) . . ?
O30 Ta3 O33 72.0(3) . . ?
O32 Ta3 Ta1 108.7(2) . . ?
O32 Ta3 Ta2 36.3(2) . . ?
O32 Ta3 K1 75.3(2) . . ?
O32 Ta3 O20 83.4(3) . . ?
O32 Ta3 O33 73.3(3) . . ?
O33 Ta3 Ta1 36.4(2) . . ?
O33 Ta3 Ta2 37.0(2) . . ?
O33 Ta3 K1 123.0(2) . . ?
Ta6 Ta4 Cs1 93.90(2) . . ?
O10 Ta4 Ta6 155.4(3) . . ?
O10 Ta4 Cs1 62.9(3) . . ?
O10 Ta4 O13 88.4(4) . . ?
O10 Ta4 O15 79.2(4) . . ?
O10 Ta4 O29 121.7(3) . . ?
O10 Ta4 O31 163.6(3) . . ?
O13 Ta4 Ta6 80.9(2) . . ?
O13 Ta4 Cs1 48.3(2) . . ?
O14 Ta4 Ta6 113.8(3) . . ?
O14 Ta4 Cs1 43.1(3) . . ?
O14 Ta4 O10 43.8(4) . . ?
O14 Ta4 O13 90.3(4) . . ?
O14 Ta4 O15 122.9(4) . . ?
O14 Ta4 O29 78.1(3) . . ?
O14 Ta4 O31 150.1(3) . . ?
O15 Ta4 Ta6 121.4(2) . . ?
O15 Ta4 Cs1 116.9(2) . . ?
O15 Ta4 O13 84.9(3) . . ?
O15 Ta4 O29 157.7(3) . . ?
O22 Ta4 Ta6 97.7(2) . . ?
O22 Ta4 Cs1 137.4(3) . . ?
O22 Ta4 O10 95.0(4) . . ?
O22 Ta4 O13 174.3(3) . . ?
O22 Ta4 O14 95.3(4) . . ?
O22 Ta4 O15 91.2(3) . . ?
O22 Ta4 O29 94.2(3) . . ?
O22 Ta4 O31 91.9(3) . . ?
O29 Ta4 Ta6 36.5(2) . . ?
O29 Ta4 Cs1 72.1(2) . . ?
O29 Ta4 O13 87.9(3) . . ?
O31 Ta4 Ta6 36.3(2) . . ?
O31 Ta4 Cs1 119.8(2) . . ?
O31 Ta4 O13 83.7(3) . . ?
O31 Ta4 O15 85.8(3) . . ?
O31 Ta4 O29 72.4(3) . . ?
O2 Ta5 Ta6 136.3(3) . . ?
O2 Ta5 O17 97.7(4) . . ?
O2 Ta5 O23 117.5(4) . . ?
O2 Ta5 O26 79.1(4) . . ?
O2 Ta5 O31 165.6(4) . . ?
O11 Ta5 Ta6 128.4(3) . . ?
O11 Ta5 O2 43.7(5) . . ?
O11 Ta5 O17 95.8(4) . . ?
O11 Ta5 O23 74.0(4) . . ?
O11 Ta5 O26 122.6(4) . . ?
O11 Ta5 O31 150.2(4) . . ?
O17 Ta5 Ta6 124.9(2) . . ?
O17 Ta5 O23 80.8(3) . . ?
O17 Ta5 O31 85.5(3) . . ?
O23 Ta5 Ta6 82.1(2) . . ?
O26 Ta5 Ta6 93.3(2) . . ?
O26 Ta5 O17 86.1(3) . . ?
O26 Ta5 O23 160.0(3) . . ?
O26 Ta5 O31 87.1(3) . . ?
O28 Ta5 Ta6 36.2(3) . . ?
O28 Ta5 O2 101.1(4) . . ?
O28 Ta5 O11 99.4(4) . . ?
O28 Ta5 O17 161.1(4) . . ?
O28 Ta5 O23 92.6(3) . . ?
O28 Ta5 O26 95.0(3) . . ?
O28 Ta5 O31 75.7(3) . . ?
O31 Ta5 Ta6 39.6(2) . . ?
O31 Ta5 O23 76.9(3) . . ?
Ta5 Ta6 Ta4 74.827(15) . . ?
O3 Ta6 Ta4 118.7(3) . . ?
O3 Ta6 Ta5 161.0(3) . . ?
O3 Ta6 O21 87.3(4) . . ?
O3 Ta6 O28 129.4(4) . . ?
O3 Ta6 O29 83.0(4) . . ?
O3 Ta6 O31 154.3(3) . . ?
O7 Ta6 Ta4 159.8(3) . . ?
O7 Ta6 Ta5 118.0(3) . . ?
O7 Ta6 O3 45.2(4) . . ?
O7 Ta6 O21 86.3(4) . . ?
O7 Ta6 O28 84.4(4) . . ?
O7 Ta6 O29 127.7(4) . . ?
O7 Ta6 O31 157.9(4) . . ?
O19 Ta6 Ta4 97.1(3) . . ?
O19 Ta6 Ta5 96.8(3) . . ?
O19 Ta6 O3 94.6(4) . . ?
O19 Ta6 O7 96.6(4) . . ?
O19 Ta6 O21 177.0(3) . . ?
O19 Ta6 O28 96.1(3) . . ?
O19 Ta6 O29 93.6(3) . . ?
O19 Ta6 O31 91.7(3) . . ?
O21 Ta6 Ta4 79.9(2) . . ?
O21 Ta6 Ta5 82.0(2) . . ?
O28 Ta6 Ta4 108.7(2) . . ?
O28 Ta6 Ta5 34.1(2) . . ?
O28 Ta6 O21 84.5(3) . . ?
O28 Ta6 O29 145.0(3) . . ?
O28 Ta6 O31 74.4(3) . . ?
O29 Ta6 Ta4 36.5(2) . . ?
O29 Ta6 Ta5 111.3(2) . . ?
O29 Ta6 O21 84.4(3) . . ?
O29 Ta6 O31 71.8(3) . . ?
O31 Ta6 Ta4 35.7(2) . . ?
O31 Ta6 Ta5 40.3(2) . . ?
O31 Ta6 O21 85.6(3) . . ?
O1 Er1 Cs1 47.7(2) . 1_655 ?
O1 Er1 O1W 117.5(3) . . ?
O1 Er1 O2W 144.1(3) . . ?
O1 Er1 O9W 74.9(4) . . ?
O4 Er1 Cs1 95.7(2) . 1_655 ?
O4 Er1 O1 77.4(3) . . ?
O4 Er1 O1W 71.7(3) . . ?
O4 Er1 O2W 75.5(3) . . ?
O4 Er1 O3W 139.9(3) . . ?
O4 Er1 O4W 83.6(4) . . ?
O4 Er1 O9W 146.1(4) . . ?
O4 Er1 O10W 115.5(4) . . ?
O1W Er1 Cs1 163.6(3) . 1_655 ?
O1W Er1 O2W 75.1(4) . . ?
O1W Er1 O9W 139.5(4) . . ?
O2W Er1 Cs1 112.7(3) . 1_655 ?
O3W Er1 Cs1 118.1(3) . 1_655 ?
O3W Er1 O1 141.2(4) . . ?
O3W Er1 O1W 77.6(4) . . ?
O3W Er1 O2W 72.1(4) . . ?
O3W Er1 O9W 72.3(4) . . ?
O4W Er1 Cs1 41.2(3) . 1_655 ?
O4W Er1 O1 82.6(4) . . ?
O4W Er1 O1W 142.5(4) . . ?
O4W Er1 O2W 71.6(4) . . ?
O4W Er1 O3W 107.2(4) . . ?
O4W Er1 O9W 73.8(4) . . ?
O9W Er1 Cs1 50.8(3) . 1_655 ?
O9W Er1 O2W 118.8(4) . . ?
O10W Er1 Cs1 103.7(3) . 1_655 ?
O10W Er1 O1 72.9(4) . . ?
O10W Er1 O1W 73.6(4) . . ?
O10W Er1 O2W 140.8(4) . . ?
O10W Er1 O3W 78.6(4) . . ?
O10W Er1 O4W 143.7(4) . . ?
O10W Er1 O9W 74.3(4) . . ?
O20 Se1 O25 100.1(4) . . ?
O27 Se1 O20 102.5(4) . . ?
O27 Se1 O25 104.0(4) . . ?
O13 Se2 Cs1 48.4(3) . . ?
O13 Se2 O21 101.5(4) . . ?
O13 Se2 O23 102.8(4) . . ?
O21 Se2 Cs1 88.3(3) . . ?
O21 Se2 O23 102.5(4) . . ?
O23 Se2 Cs1 151.1(3) . . ?
O4 Se3 O15 99.9(4) . . ?
O4 Se3 O17 99.4(4) . . ?
O15 Se3 O17 100.2(4) . . ?
O1 Se4 Cs1 57.6(3) . 1_655 ?
O1 Se4 O9 101.0(4) . . ?
O1 Se4 O24 100.2(4) . . ?
O9 Se4 Cs1 45.5(3) . 1_655 ?
O9 Se4 O24 97.2(4) . . ?
O24 Se4 Cs1 115.7(3) . 1_655 ?
O1 Cs1 O2W 110.1(2) 1_455 4_475 ?
O1 Cs1 O9W 47.5(2) 1_455 1_455 ?
O6 Cs1 O1 90.7(2) 1_455 1_455 ?
O6 Cs1 O13 108.5(2) 1_455 . ?
O6 Cs1 O2W 48.0(2) 1_455 4_475 ?
O6 Cs1 O9W 138.2(2) 1_455 1_455 ?
O7 Cs1 O1 113.3(2) 4_576 1_455 ?
O7 Cs1 O6 107.4(2) 4_576 1_455 ?
O7 Cs1 O9 124.5(2) 4_576 1_455 ?
O7 Cs1 O13 60.9(2) 4_576 . ?
O7 Cs1 O14 110.8(2) 4_576 . ?
O7 Cs1 O2W 59.4(2) 4_576 4_475 ?
O7 Cs1 O4W 59.5(3) 4_576 1_455 ?
O7 Cs1 O7W 131.7(3) 4_576 . ?
O7 Cs1 O8W 71.5(3) 4_576 . ?
O7 Cs1 O9W 91.1(3) 4_576 1_455 ?
O7 Cs1 O16W 168.9(5) 4_576 3_566 ?
O9 Cs1 O1 45.2(2) 1_455 1_455 ?
O9 Cs1 O6 45.9(2) 1_455 1_455 ?
O9 Cs1 O13 153.9(2) 1_455 . ?
O9 Cs1 O14 123.4(2) 1_455 . ?
O9 Cs1 O2W 80.2(2) 1_455 4_475 ?
O9 Cs1 O4W 83.8(3) 1_455 1_455 ?
O9 Cs1 O7W 77.1(3) 1_455 . ?
O9 Cs1 O8W 140.1(3) 1_455 . ?
O9 Cs1 O9W 92.6(2) 1_455 1_455 ?
O13 Cs1 O1 160.8(2) . 1_455 ?
O13 Cs1 O2W 83.4(2) . 4_475 ?
O13 Cs1 O9W 113.3(2) . 1_455 ?
O14 Cs1 O1 122.7(2) . 1_455 ?
O14 Cs1 O6 109.1(2) . 1_455 ?
O14 Cs1 O13 52.5(2) . . ?
O14 Cs1 O2W 123.3(2) . 4_475 ?
O14 Cs1 O4W 140.2(3) . 1_455 ?
O14 Cs1 O7W 56.1(3) . . ?
O14 Cs1 O9W 98.1(2) . 1_455 ?
O2W Cs1 O9W 134.7(3) 4_475 1_455 ?
O4W Cs1 O1 54.1(3) 1_455 1_455 ?
O4W Cs1 O6 110.6(2) 1_455 1_455 ?
O4W Cs1 O13 115.5(2) 1_455 . ?
O4W Cs1 O2W 86.8(3) 1_455 4_475 ?
O4W Cs1 O7W 160.8(3) 1_455 . ?
O4W Cs1 O9W 47.9(3) 1_455 1_455 ?
O7W Cs1 O1 111.0(3) . 1_455 ?
O7W Cs1 O6 53.7(3) . 1_455 ?
O7W Cs1 O13 82.2(3) . . ?
O7W Cs1 O2W 88.1(3) . 4_475 ?
O7W Cs1 O9W 134.0(3) . 1_455 ?
O8W Cs1 O1 95.6(3) . 1_455 ?
O8W Cs1 O6 173.5(3) . 1_455 ?
O8W Cs1 O13 65.3(3) . . ?
O8W Cs1 O14 66.1(3) . . ?
O8W Cs1 O2W 130.2(3) . 4_475 ?
O8W Cs1 O4W 74.6(3) . 1_455 ?
O8W Cs1 O7W 122.0(4) . . ?
O8W Cs1 O9W 48.2(3) . 1_455 ?
O16W Cs1 O1 58.7(4) 3_566 1_455 ?
O16W Cs1 O6 81.3(5) 3_566 1_455 ?
O16W Cs1 O9 56.7(5) 3_566 1_455 ?
O16W Cs1 O13 123.7(5) 3_566 . ?
O16W Cs1 O14 71.6(5) 3_566 . ?
O16W Cs1 O2W 129.1(5) 3_566 4_475 ?
O16W Cs1 O4W 111.4(5) 3_566 1_455 ?
O16W Cs1 O7W 59.0(5) 3_566 . ?
O16W Cs1 O8W 100.7(5) 3_566 . ?
O16W Cs1 O9W 77.8(5) 3_566 1_455 ?
O8 K1 Ta3 27.08(18) . . ?
O8 K1 O11 75.9(3) . 4_575 ?
O8 K1 O20 56.7(3) . . ?
O8 K1 O8W 69.4(3) . 1_554 ?
O8 K1 O11W 127.4(3) . 3_666 ?
O8 K1 O17W 87.5(5) . . ?
O11 K1 Ta3 80.2(2) 4_575 . ?
O11 K1 O17W 157.4(5) 4_575 . ?
O20 K1 Ta3 29.95(17) . . ?
O20 K1 O11 93.2(3) . 4_575 ?
O20 K1 O8W 125.7(3) . 1_554 ?
O20 K1 O17W 64.6(4) . . ?
O8W K1 Ta3 95.7(3) 1_554 . ?
O8W K1 O11 66.3(4) 1_554 4_575 ?
O8W K1 O17W 122.2(5) 1_554 . ?
O11W K1 Ta3 100.8(3) 3_666 . ?
O11W K1 O11 112.1(4) 3_666 4_575 ?
O11W K1 O20 70.9(3) 3_666 . ?
O11W K1 O8W 162.9(4) 3_666 1_554 ?
O11W K1 O17W 66.3(5) 3_666 . ?
O12W K1 Ta3 150.5(3) . . ?
O12W K1 O8 149.6(4) . . ?
O12W K1 O11 75.6(4) . 4_575 ?
O12W K1 O20 135.1(4) . . ?
O12W K1 O8W 89.8(4) . 1_554 ?
O12W K1 O11W 73.7(4) . 3_666 ?
O12W K1 O17W 122.7(5) . . ?
O13W K1 Ta3 131.5(4) . . ?
O13W K1 O8 117.0(4) . . ?
O13W K1 O11 135.4(4) . 4_575 ?
O13W K1 O20 130.3(4) . . ?
O13W K1 O8W 78.5(4) . 1_554 ?
O13W K1 O11W 93.7(4) . 3_666 ?
O13W K1 O12W 78.0(4) . . ?
O13W K1 O17W 65.9(5) . . ?
O17W K1 Ta3 78.1(4) . . ?
Er1 O1 Cs1 102.5(3) . 1_655 ?
Se4 O1 Er1 128.4(5) . . ?
Se4 O1 Cs1 99.0(4) . 1_655 ?
O11 O2 Ta5 67.0(6) . . ?
O7 O3 Ta6 66.9(5) . . ?
Se3 O4 Er1 175.6(5) . . ?
O6 O5 Ta2 68.3(5) . . ?
Ta2 O6 Cs1 116.0(3) . 1_655 ?
O5 O6 Ta2 67.6(5) . . ?
O5 O6 Cs1 175.7(6) . 1_655 ?
Ta6 O7 Cs1 146.7(4) . 4_575 ?
O3 O7 Ta6 67.9(5) . . ?
O3 O7 Cs1 131.5(6) . 4_575 ?
Ta3 O8 K1 110.9(4) . . ?
O12 O8 Ta3 67.3(5) . . ?
O12 O8 K1 108.3(6) . . ?
Ta2 O9 Cs1 120.4(4) . 1_655 ?
Se4 O9 Ta2 124.2(5) . . ?
Se4 O9 Cs1 111.9(4) . 1_655 ?
O14 O10 Ta4 67.5(5) . . ?
Ta5 O11 K1 147.6(5) . 4_576 ?
O2 O11 Ta5 69.3(7) . . ?
O2 O11 K1 124.1(8) . 4_576 ?
O8 O12 Ta3 66.7(5) . . ?
Ta4 O13 Cs1 103.8(3) . . ?
Se2 O13 Ta4 129.0(5) . . ?
Se2 O13 Cs1 109.1(4) . . ?
Ta4 O14 Cs1 111.9(4) . . ?
O10 O14 Ta4 68.8(5) . . ?
O10 O14 Cs1 105.5(5) . . ?
Se3 O15 Ta4 136.8(5) . . ?
O18 O16 Ta1 68.7(5) . . ?
Se3 O17 Ta5 131.4(5) . . ?
O16 O18 Ta1 67.0(5) . . ?
Ta3 O19 Ta6 163.5(5) . . ?
Ta3 O20 K1 104.1(3) . . ?
Se1 O20 Ta3 127.3(5) . . ?
Se1 O20 K1 121.5(4) . . ?
Se2 O21 Ta6 125.2(4) . . ?
Ta1 O22 Ta4 164.0(5) . . ?
Se2 O23 Ta5 131.0(5) . . ?
Se4 O24 Ta1 121.7(5) . . ?
Se1 O25 Ta1 131.5(5) . . ?
Ta2 O26 Ta5 168.1(5) . . ?
Se1 O27 Ta2 130.7(5) . . ?
Ta5 O28 Ta6 109.7(4) . . ?
Ta6 O29 Ta4 107.0(4) . . ?
Ta3 O30 Ta1 108.7(4) . . ?
Ta4 O31 Ta5 146.5(4) . . ?
Ta4 O31 Ta6 108.0(3) . . ?
Ta6 O31 Ta5 100.1(3) . . ?
Ta3 O32 Ta2 108.1(4) . . ?
Ta1 O33 Ta2 143.3(4) . . ?
Ta1 O33 Ta3 106.7(4) . . ?
Ta3 O33 Ta2 106.2(3) . . ?
Er1 O2W Cs1 161.4(4) . 4_676 ?
Er1 O4W Cs1 110.8(4) . 1_655 ?
K1 O8W Cs1 146.8(5) 1_556 . ?
Er1 O9W Cs1 98.8(4) . 1_655 ?

_shelx_SHELXL_version_number     2018/1
_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy2_a
_database_code_depnum_ccdc_archive 'CCDC 1893227'
loop_
_audit_author_name
_audit_author_address
ddzhang
;Henan University
China
;
_audit_update_record             
;
2019-01-24 deposited with the CCDC.	2020-02-27 downloaded from the CCDC.
;
_audit_creation_date             2018-02-09
_audit_creation_method           
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs K O46 Se4 Ta6 Tb, 4(O)'
_chemical_formula_sum            'Cs K O50 Se4 Ta6 Tb'
_chemical_formula_weight         2532.47
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tb Tb -0.1723 4.1537 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.3034(7)
_cell_length_b                   27.2518(15)
_cell_length_c                   14.0071(8)
_cell_angle_alpha                90
_cell_angle_beta                 113.9280(10)
_cell_angle_gamma                90
_cell_volume                     4292.8(4)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    9449
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.33
_cell_measurement_theta_min      2.35
_shelx_estimated_absorpt_T_max   0.203
_shelx_estimated_absorpt_T_min   0.048
_exptl_absorpt_coefficient_mu    21.310
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.2655
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1309 before and 0.0484 after correction.
The Ratio of minimum to maximum transmission is 0.3560.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.918
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4452
_exptl_crystal_size_max          0.36
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.11
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0368
_diffrn_reflns_av_unetI/netI     0.0424
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            22120
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.098
_diffrn_reflns_theta_max         25.098
_diffrn_reflns_theta_min         1.494
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                6742
_reflns_number_total             7631
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         1.486
_refine_diff_density_min         -4.754
_refine_diff_density_rms         0.313
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.012
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7631
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0435
_refine_ls_R_factor_gt           0.0370
_refine_ls_restrained_S_all      1.012
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0409P)²+110.7533P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0908
_refine_ls_wR_factor_ref         0.0941
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28594(4) 0.54873(2) 0.55534(3) 0.01095(11) Uani 1 1 d . . . . .
Ta2 Ta 0.43795(4) 0.65822(2) 0.47102(3) 0.01115(11) Uani 1 1 d . . . . .
Ta3 Ta 0.17296(4) 0.60805(2) 0.32860(3) 0.01133(11) Uani 1 1 d . . . . .
Ta4 Ta 0.13699(4) 0.64078(2) 0.66428(3) 0.01133(11) Uani 1 1 d . . . . .
Ta5 Ta 0.28288(4) 0.75232(2) 0.57593(3) 0.01158(11) Uani 1 1 d . . . . .
Ta6 Ta 0.03340(4) 0.70202(2) 0.43881(3) 0.01277(11) Uani 1 1 d . . . . .
Tb1 Tb 0.68549(5) 0.64924(2) 0.98603(4) 0.01523(13) Uani 1 1 d . . . . .
Se1 Se 0.41826(10) 0.53752(4) 0.38164(8) 0.0148(2) Uani 1 1 d . . . . .
Se2 Se 0.04987(10) 0.76029(4) 0.66025(9) 0.0151(2) Uani 1 1 d . . . . .
Se3 Se 0.37728(10) 0.71183(4) 0.82830(8) 0.0135(2) Uani 1 1 d . . . . .
Se4 Se 0.49220(10) 0.62399(4) 0.71373(9) 0.0167(2) Uani 1 1 d . . . . .
Cs1 Cs -0.18025(11) 0.66379(5) 0.72155(11) 0.0609(3) Uani 1 1 d . . . . .
K1 K 0.2251(4) 0.57350(16) 0.0739(3) 0.0552(10) Uani 1 1 d . . . . .
O1 O 0.6196(7) 0.6138(3) 0.8164(6) 0.0208(19) Uiso 1 1 d . . . . .
O2 O 0.3883(8) 0.8010(4) 0.5497(7) 0.030(2) Uiso 1 1 d . . . . .
O3 O -0.1352(8) 0.6946(3) 0.3440(7) 0.0234(19) Uiso 1 1 d . . . . .
O4 O 0.5072(7) 0.6873(3) 0.8973(6) 0.0202(18) Uiso 1 1 d . . . . .
O5 O 0.5034(7) 0.6931(3) 0.3828(7) 0.0222(19) Uiso 1 1 d . . . . .
O6 O 0.5966(7) 0.6850(3) 0.4898(6) 0.0196(18) Uiso 1 1 d . . . . .
O7 O -0.0779(8) 0.7380(3) 0.3173(7) 0.025(2) Uiso 1 1 d . . . . .
O8 O 0.0971(7) 0.6192(3) 0.1772(6) 0.0208(18) Uiso 1 1 d . . . . .
O9 O 0.5453(7) 0.6375(3) 0.6204(6) 0.0203(18) Uiso 1 1 d . . . . .
O10 O 0.1248(8) 0.6041(3) 0.7830(7) 0.0237(19) Uiso 1 1 d . . . . .
O11 O 0.3169(9) 0.8224(4) 0.6024(8) 0.034(2) Uiso 1 1 d . . . . .
O12 O 0.0342(8) 0.5802(3) 0.2127(7) 0.025(2) Uiso 1 1 d . . . . .
O13 O 0.0703(7) 0.7027(3) 0.7103(6) 0.0183(18) Uiso 1 1 d . . . . .
O14 O 0.0162(7) 0.5999(3) 0.6860(7) 0.0209(18) Uiso 1 1 d . . . . .
O15 O 0.2961(7) 0.6593(3) 0.7832(6) 0.0201(18) Uiso 1 1 d . . . . .
O16 O 0.2018(8) 0.4864(3) 0.5504(7) 0.0237(19) Uiso 1 1 d . . . . .
O17 O 0.3997(7) 0.7291(3) 0.7194(6) 0.0181(18) Uiso 1 1 d . . . . .
O18 O 0.3179(8) 0.4887(3) 0.6436(7) 0.0234(19) Uiso 1 1 d . . . . .
O19 O 0.0886(7) 0.6587(3) 0.3637(6) 0.0165(17) Uiso 1 1 d . . . . .
O20 O 0.2820(7) 0.5580(3) 0.2969(6) 0.0167(17) Uiso 1 1 d . . . . .
O21 O -0.0249(7) 0.7489(3) 0.5306(6) 0.0188(18) Uiso 1 1 d . . . . .
O22 O 0.2102(7) 0.5872(3) 0.6229(6) 0.0183(18) Uiso 1 1 d . . . . .
O23 O 0.1878(7) 0.7756(3) 0.6683(6) 0.0185(18) Uiso 1 1 d . . . . .
O24 O 0.4473(7) 0.5646(3) 0.6758(6) 0.0206(18) Uiso 1 1 d . . . . .
O25 O 0.3830(7) 0.5168(3) 0.4823(6) 0.0158(17) Uiso 1 1 d . . . . .
O26 O 0.3733(7) 0.7089(3) 0.5180(6) 0.0170(17) Uiso 1 1 d . . . . .
O27 O 0.4934(7) 0.5902(3) 0.4278(6) 0.0189(18) Uiso 1 1 d . . . . .
O28 O 0.1447(7) 0.7567(3) 0.4475(6) 0.0180(18) Uiso 1 1 d . . . . .
O29 O -0.0051(7) 0.6454(3) 0.5193(6) 0.0203(18) Uiso 1 1 d . . . . .
O30 O 0.1398(7) 0.5544(3) 0.4140(6) 0.0170(17) Uiso 1 1 d . . . . .
O31 O 0.1813(7) 0.6899(3) 0.5757(6) 0.0130(16) Uiso 1 1 d . . . . .
O32 O 0.2948(7) 0.6581(3) 0.3250(6) 0.0168(17) Uiso 1 1 d . . . . .
O33 O 0.3104(6) 0.6094(3) 0.4785(6) 0.0104(15) Uiso 1 1 d . . . . .
O1W O 0.5642(8) 0.6363(4) 1.0823(7) 0.031(2) Uiso 1 1 d . . . . .
O2W O 0.7011(9) 0.7276(4) 1.0826(8) 0.035(2) Uiso 1 1 d . . . . .
O3W O 0.8307(9) 0.6386(4) 1.1613(8) 0.036(2) Uiso 1 1 d . . . . .
O4W O 0.7600(9) 0.7104(4) 0.9087(8) 0.036(2) Uiso 1 1 d . . . . .
O5W O -0.0458(9) 0.5001(4) 0.3459(8) 0.038(2) Uiso 1 1 d . . . . .
O6W O 0.6270(9) 0.7691(4) 0.7521(8) 0.041(3) Uiso 1 1 d . . . . .
O7W O -0.2169(12) 0.6148(5) 0.4978(11) 0.065(4) Uiso 1 1 d . . . . .
O8W O 0.0525(11) 0.6443(5) 0.9268(10) 0.053(3) Uiso 1 1 d . . . . .
O9W O 0.8622(10) 0.6153(4) 0.9752(9) 0.045(3) Uiso 1 1 d . . . . .
O10W O 0.6780(10) 0.5638(4) 1.0091(9) 0.045(3) Uiso 1 1 d . . . . .
O11W O 0.5827(10) 0.4968(4) 0.8450(9) 0.050(3) Uiso 1 1 d . . . . .
O12W O 0.3619(11) 0.5816(5) -0.0540(9) 0.053(3) Uiso 1 1 d . . . . .
O13W O 0.0950(12) 0.5158(5) -0.1037(11) 0.064(4) Uiso 1 1 d . . . . .
O14W O 0.3564(12) 0.4922(5) 0.8521(10) 0.061(3) Uiso 1 1 d . . . . .
O15W O 0.6010(16) 0.6133(7) 1.2777(14) 0.094(5) Uiso 1 1 d . . . . .
O16W O 0.2751(19) 0.4413(8) 0.3356(17) 0.122(7) Uiso 1 1 d . . . . .
O17W O 0.1396(17) 0.4712(7) 0.1269(15) 0.106(6) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3243(6) . ?
Ta1 O16 1.975(9) . ?
Ta1 O18 1.991(9) . ?
Ta1 O22 1.892(8) . ?
Ta1 O24 2.064(8) . ?
Ta1 O25 2.054(8) . ?
Ta1 O30 2.070(8) . ?
Ta1 O33 2.061(7) . ?
Ta2 Ta3 3.3471(6) . ?
Ta2 O5 1.972(8) . ?
Ta2 O6 2.000(8) . ?
Ta2 O9 2.049(8) . ?
Ta2 O26 1.843(8) . ?
Ta2 O27 2.145(8) . ?
Ta2 O32 2.088(8) . ?
Ta2 O33 2.092(7) . ?
Ta3 K1 3.985(4) . ?
Ta3 O8 1.964(8) . ?
Ta3 O12 1.969(9) . ?
Ta3 O19 1.908(8) . ?
Ta3 O20 2.083(8) . ?
Ta3 O30 2.032(8) . ?
Ta3 O32 2.043(8) . ?
Ta3 O33 2.095(7) . ?
Ta4 Ta6 3.3343(6) . ?
Ta4 Cs1 4.3373(13) . ?
Ta4 O10 1.997(9) . ?
Ta4 O13 2.090(8) . ?
Ta4 O14 1.976(8) . ?
Ta4 O15 2.053(8) . ?
Ta4 O22 1.924(8) . ?
Ta4 O29 2.077(8) . ?
Ta4 O31 2.045(8) . ?
Ta5 Ta6 3.1949(7) . ?
Ta5 O2 1.990(9) . ?
Ta5 O11 1.958(10) . ?
Ta5 O17 2.040(8) . ?
Ta5 O23 2.162(8) . ?
Ta5 O26 2.007(8) . ?
Ta5 O28 1.913(8) . ?
Ta5 O31 2.109(8) . ?
Ta6 O3 1.969(9) . ?
Ta6 O7 1.961(9) . ?
Ta6 O19 1.881(8) . ?
Ta6 O21 2.132(8) . ?
Ta6 O28 1.995(8) . ?
Ta6 O29 2.077(8) . ?
Ta6 O31 2.066(8) . ?
Tb1 Cs1 4.6448(14) 1_655 ?
Tb1 O1 2.382(8) . ?
Tb1 O4 2.285(8) . ?
Tb1 O1W 2.409(10) . ?
Tb1 O2W 2.493(10) . ?
Tb1 O3W 2.397(10) . ?
Tb1 O4W 2.365(10) . ?
Tb1 O9W 2.423(11) . ?
Tb1 O10W 2.358(12) . ?
Se1 O20 1.709(8) . ?
Se1 O25 1.729(8) . ?
Se1 O27 1.688(8) . ?
Se2 Cs1 4.2002(17) . ?
Se2 O13 1.695(8) . ?
Se2 O21 1.699(8) . ?
Se2 O23 1.706(8) . ?
Se3 O4 1.638(8) . ?
Se3 O15 1.714(8) . ?
Se3 O17 1.722(8) . ?
Se4 Cs1 4.1317(17) 1_655 ?
Se4 O1 1.665(8) . ?
Se4 O9 1.722(8) . ?
Se4 O24 1.722(9) . ?
Cs1 O1 3.513(8) 1_455 ?
Cs1 O6 3.344(8) 1_455 ?
Cs1 O7 3.029(9) 4_576 ?
Cs1 O9 3.169(8) 1_455 ?
Cs1 O13 3.324(8) . ?
Cs1 O14 3.177(8) . ?
Cs1 O2W 3.518(10) 4_475 ?
Cs1 O4W 3.254(10) 1_455 ?
Cs1 O7W 3.265(14) . ?
Cs1 O8W 3.173(12) . ?
Cs1 O9W 3.624(11) 1_455 ?
Cs1 O16W 3.07(2) 3_566 ?
K1 O8 2.824(9) . ?
K1 O11 3.019(11) 4_575 ?
K1 O20 2.941(9) . ?
K1 O8W 2.988(13) 1_554 ?
K1 O11W 2.895(13) 3_666 ?
K1 O12W 2.922(13) . ?
K1 O13W 2.828(15) . ?
K1 O17W 3.17(2) . ?
O2 O11 1.479(13) . ?
O3 O7 1.501(12) . ?
O5 O6 1.488(12) . ?
O8 O12 1.511(12) . ?
O10 O14 1.473(12) . ?
O16 O18 1.495(12) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Ta1 Ta3 112.0(3) . . ?
O16 Ta1 O18 44.3(3) . . ?
O16 Ta1 O24 121.7(3) . . ?
O16 Ta1 O25 91.2(3) . . ?
O16 Ta1 O30 78.0(3) . . ?
O16 Ta1 O33 149.0(3) . . ?
O18 Ta1 Ta3 153.3(3) . . ?
O18 Ta1 O24 77.4(3) . . ?
O18 Ta1 O25 87.4(3) . . ?
O18 Ta1 O30 122.1(3) . . ?
O18 Ta1 O33 161.8(3) . . ?
O22 Ta1 Ta3 96.2(2) . . ?
O22 Ta1 O16 97.8(4) . . ?
O22 Ta1 O18 99.1(4) . . ?
O22 Ta1 O24 88.9(3) . . ?
O22 Ta1 O25 171.0(3) . . ?
O22 Ta1 O30 91.4(3) . . ?
O22 Ta1 O33 91.3(3) . . ?
O24 Ta1 Ta3 124.7(2) . . ?
O24 Ta1 O30 160.1(3) . . ?
O25 Ta1 Ta3 80.3(2) . . ?
O25 Ta1 O24 86.3(3) . . ?
O25 Ta1 O30 90.6(3) . . ?
O25 Ta1 O33 80.9(3) . . ?
O30 Ta1 Ta3 35.5(2) . . ?
O33 Ta1 Ta3 37.2(2) . . ?
O33 Ta1 O24 87.8(3) . . ?
O33 Ta1 O30 72.2(3) . . ?
O5 Ta2 Ta3 111.7(2) . . ?
O5 Ta2 O6 44.0(3) . . ?
O5 Ta2 O9 121.0(3) . . ?
O5 Ta2 O27 89.0(3) . . ?
O5 Ta2 O32 77.5(3) . . ?
O5 Ta2 O33 147.5(3) . . ?
O6 Ta2 Ta3 153.0(2) . . ?
O6 Ta2 O9 77.1(3) . . ?
O6 Ta2 O27 87.0(3) . . ?
O6 Ta2 O32 121.3(3) . . ?
O6 Ta2 O33 159.7(3) . . ?
O9 Ta2 Ta3 124.4(2) . . ?
O9 Ta2 O27 84.4(3) . . ?
O9 Ta2 O32 159.7(3) . . ?
O9 Ta2 O33 87.7(3) . . ?
O26 Ta2 Ta3 93.5(2) . . ?
O26 Ta2 O5 102.0(4) . . ?
O26 Ta2 O6 102.7(3) . . ?
O26 Ta2 O9 92.0(3) . . ?
O26 Ta2 O27 168.7(3) . . ?
O26 Ta2 O32 92.1(3) . . ?
O26 Ta2 O33 91.0(3) . . ?
O27 Ta2 Ta3 79.8(2) . . ?
O32 Ta2 Ta3 35.4(2) . . ?
O32 Ta2 O27 87.8(3) . . ?
O32 Ta2 O33 72.3(3) . . ?
O33 Ta2 Ta3 37.0(2) . . ?
O33 Ta2 O27 78.2(3) . . ?
Ta1 Ta3 Ta2 72.569(14) . . ?
Ta1 Ta3 K1 125.71(6) . . ?
Ta2 Ta3 K1 99.12(7) . . ?
O8 Ta3 Ta1 159.8(3) . . ?
O8 Ta3 Ta2 120.1(2) . . ?
O8 Ta3 K1 41.3(2) . . ?
O8 Ta3 O12 45.2(3) . . ?
O8 Ta3 O20 86.3(3) . . ?
O8 Ta3 O30 128.8(3) . . ?
O8 Ta3 O32 84.4(3) . . ?
O8 Ta3 O33 156.4(3) . . ?
O12 Ta3 Ta1 119.2(3) . . ?
O12 Ta3 Ta2 163.3(3) . . ?
O12 Ta3 K1 64.6(3) . . ?
O12 Ta3 O20 89.4(3) . . ?
O12 Ta3 O30 84.0(3) . . ?
O12 Ta3 O32 129.5(3) . . ?
O12 Ta3 O33 155.6(3) . . ?
O19 Ta3 Ta1 99.6(2) . . ?
O19 Ta3 Ta2 92.9(2) . . ?
O19 Ta3 K1 134.7(2) . . ?
O19 Ta3 O8 95.5(3) . . ?
O19 Ta3 O12 96.4(3) . . ?
O19 Ta3 O20 173.4(3) . . ?
O19 Ta3 O30 96.3(3) . . ?
O19 Ta3 O32 90.2(3) . . ?
O19 Ta3 O33 91.8(3) . . ?
O20 Ta3 Ta1 80.2(2) . . ?
O20 Ta3 Ta2 80.7(2) . . ?
O20 Ta3 K1 45.8(2) . . ?
O20 Ta3 O33 84.2(3) . . ?
O30 Ta3 Ta1 36.3(2) . . ?
O30 Ta3 Ta2 108.8(2) . . ?
O30 Ta3 K1 120.0(2) . . ?
O30 Ta3 O20 87.4(3) . . ?
O30 Ta3 O32 145.0(3) . . ?
O30 Ta3 O33 72.3(3) . . ?
O32 Ta3 Ta1 108.8(2) . . ?
O32 Ta3 Ta2 36.3(2) . . ?
O32 Ta3 K1 75.5(2) . . ?
O32 Ta3 O20 83.6(3) . . ?
O32 Ta3 O33 73.2(3) . . ?
O33 Ta3 Ta1 36.5(2) . . ?
O33 Ta3 Ta2 36.9(2) . . ?
O33 Ta3 K1 123.0(2) . . ?
Ta6 Ta4 Cs1 94.35(2) . . ?
O10 Ta4 Ta6 155.5(2) . . ?
O10 Ta4 Cs1 62.7(2) . . ?
O10 Ta4 O13 88.6(3) . . ?
O10 Ta4 O15 79.4(3) . . ?
O10 Ta4 O29 121.7(3) . . ?
O10 Ta4 O31 164.1(3) . . ?
O13 Ta4 Ta6 80.8(2) . . ?
O13 Ta4 Cs1 48.0(2) . . ?
O14 Ta4 Ta6 113.9(2) . . ?
O14 Ta4 Cs1 42.6(2) . . ?
O14 Ta4 O10 43.5(3) . . ?
O14 Ta4 O13 89.6(3) . . ?
O14 Ta4 O15 122.8(3) . . ?
O14 Ta4 O29 78.3(3) . . ?
O14 Ta4 O31 149.8(3) . . ?
O15 Ta4 Ta6 121.2(2) . . ?
O15 Ta4 Cs1 116.6(2) . . ?
O15 Ta4 O13 85.2(3) . . ?
O15 Ta4 O29 157.8(3) . . ?
O22 Ta4 Ta6 98.1(2) . . ?
O22 Ta4 Cs1 137.0(2) . . ?
O22 Ta4 O10 94.2(3) . . ?
O22 Ta4 O13 175.0(3) . . ?
O22 Ta4 O14 95.3(3) . . ?
O22 Ta4 O15 91.3(3) . . ?
O22 Ta4 O29 93.6(3) . . ?
O22 Ta4 O31 92.4(3) . . ?
O29 Ta4 Ta6 36.6(2) . . ?
O29 Ta4 Cs1 73.0(2) . . ?
O29 Ta4 O13 88.5(3) . . ?
O31 Ta4 Ta6 36.0(2) . . ?
O31 Ta4 Cs1 119.9(2) . . ?
O31 Ta4 O13 83.8(3) . . ?
O31 Ta4 O15 86.0(3) . . ?
O31 Ta4 O29 72.1(3) . . ?
O2 Ta5 Ta6 135.6(3) . . ?
O2 Ta5 O17 97.9(4) . . ?
O2 Ta5 O23 117.8(4) . . ?
O2 Ta5 O26 79.0(4) . . ?
O2 Ta5 O31 165.2(3) . . ?
O11 Ta5 Ta6 127.7(3) . . ?
O11 Ta5 O2 44.0(4) . . ?
O11 Ta5 O17 96.0(4) . . ?
O11 Ta5 O23 74.1(4) . . ?
O11 Ta5 O26 122.8(4) . . ?
O11 Ta5 O31 150.2(3) . . ?
O17 Ta5 Ta6 125.5(2) . . ?
O17 Ta5 O23 80.7(3) . . ?
O17 Ta5 O31 86.1(3) . . ?
O23 Ta5 Ta6 82.2(2) . . ?
O26 Ta5 Ta6 93.4(2) . . ?
O26 Ta5 O17 86.0(3) . . ?
O26 Ta5 O23 159.7(3) . . ?
O26 Ta5 O31 87.1(3) . . ?
O28 Ta5 Ta6 36.0(2) . . ?
O28 Ta5 O2 100.5(4) . . ?
O28 Ta5 O11 99.0(4) . . ?
O28 Ta5 O17 161.5(3) . . ?
O28 Ta5 O23 93.1(3) . . ?
O28 Ta5 O26 94.8(3) . . ?
O28 Ta5 O31 75.5(3) . . ?
O31 Ta5 Ta6 39.6(2) . . ?
O31 Ta5 O23 76.9(3) . . ?
Ta5 Ta6 Ta4 74.954(15) . . ?
O3 Ta6 Ta4 118.7(3) . . ?
O3 Ta6 Ta5 160.5(3) . . ?
O3 Ta6 O21 87.0(3) . . ?
O3 Ta6 O28 128.9(3) . . ?
O3 Ta6 O29 83.1(3) . . ?
O3 Ta6 O31 154.3(3) . . ?
O7 Ta6 Ta4 159.5(3) . . ?
O7 Ta6 Ta5 118.0(3) . . ?
O7 Ta6 O3 44.9(4) . . ?
O7 Ta6 O21 86.4(3) . . ?
O7 Ta6 O28 84.2(3) . . ?
O7 Ta6 O29 127.6(3) . . ?
O7 Ta6 O31 158.1(3) . . ?
O19 Ta6 Ta4 97.5(2) . . ?
O19 Ta6 Ta5 97.4(2) . . ?
O19 Ta6 O3 94.5(3) . . ?
O19 Ta6 O7 96.4(4) . . ?
O19 Ta6 O21 177.2(3) . . ?
O19 Ta6 O28 96.2(3) . . ?
O19 Ta6 O29 92.9(3) . . ?
O19 Ta6 O31 92.1(3) . . ?
O21 Ta6 Ta4 79.7(2) . . ?
O21 Ta6 Ta5 81.8(2) . . ?
O28 Ta6 Ta4 109.1(2) . . ?
O28 Ta6 Ta5 34.3(2) . . ?
O28 Ta6 O21 84.6(3) . . ?
O28 Ta6 O29 145.6(3) . . ?
O28 Ta6 O31 74.8(3) . . ?
O29 Ta6 Ta4 36.6(2) . . ?
O29 Ta6 Ta5 111.6(2) . . ?
O29 Ta6 O21 84.9(3) . . ?
O31 Ta6 Ta4 35.6(2) . . ?
O31 Ta6 Ta5 40.6(2) . . ?
O31 Ta6 O21 85.5(3) . . ?
O31 Ta6 O29 71.7(3) . . ?
O1 Tb1 Cs1 47.6(2) . 1_655 ?
O1 Tb1 O1W 117.5(3) . . ?
O1 Tb1 O2W 144.0(3) . . ?
O1 Tb1 O3W 141.6(3) . . ?
O1 Tb1 O9W 74.6(3) . . ?
O4 Tb1 Cs1 95.8(2) . 1_655 ?
O4 Tb1 O1 77.2(3) . . ?
O4 Tb1 O1W 72.2(3) . . ?
O4 Tb1 O2W 75.7(3) . . ?
O4 Tb1 O3W 139.8(3) . . ?
O4 Tb1 O4W 84.0(3) . . ?
O4 Tb1 O9W 145.8(3) . . ?
O4 Tb1 O10W 116.1(3) . . ?
O1W Tb1 Cs1 163.8(2) . 1_655 ?
O1W Tb1 O2W 75.6(3) . . ?
O1W Tb1 O9W 139.0(4) . . ?
O2W Tb1 Cs1 112.7(2) . 1_655 ?
O3W Tb1 Cs1 118.0(2) . 1_655 ?
O3W Tb1 O1W 77.4(3) . . ?
O3W Tb1 O2W 71.7(3) . . ?
O3W Tb1 O9W 72.7(4) . . ?
O4W Tb1 Cs1 41.0(2) . 1_655 ?
O4W Tb1 O1 82.4(3) . . ?
O4W Tb1 O1W 143.4(3) . . ?
O4W Tb1 O2W 71.7(3) . . ?
O4W Tb1 O3W 106.7(4) . . ?
O4W Tb1 O9W 73.5(4) . . ?
O9W Tb1 Cs1 50.5(3) . 1_655 ?
O9W Tb1 O2W 119.1(4) . . ?
O10W Tb1 Cs1 103.9(3) . 1_655 ?
O10W Tb1 O1 73.7(3) . . ?
O10W Tb1 O1W 73.2(4) . . ?
O10W Tb1 O2W 140.4(4) . . ?
O10W Tb1 O3W 78.2(4) . . ?
O10W Tb1 O4W 143.4(4) . . ?
O10W Tb1 O9W 73.6(4) . . ?
O20 Se1 O25 100.0(4) . . ?
O27 Se1 O20 102.6(4) . . ?
O27 Se1 O25 104.1(4) . . ?
O13 Se2 Cs1 48.3(3) . . ?
O13 Se2 O21 101.4(4) . . ?
O13 Se2 O23 102.9(4) . . ?
O21 Se2 Cs1 89.2(3) . . ?
O21 Se2 O23 102.0(4) . . ?
O23 Se2 Cs1 151.0(3) . . ?
O4 Se3 O15 99.2(4) . . ?
O4 Se3 O17 99.5(4) . . ?
O15 Se3 O17 100.4(4) . . ?
O1 Se4 Cs1 57.0(3) . 1_655 ?
O1 Se4 O9 100.2(4) . . ?
O1 Se4 O24 100.4(4) . . ?
O9 Se4 Cs1 45.4(3) . 1_655 ?
O9 Se4 O24 98.0(4) . . ?
O24 Se4 Cs1 116.2(3) . 1_655 ?
O1 Cs1 O2W 109.8(2) 1_455 4_475 ?
O1 Cs1 O9W 48.1(2) 1_455 1_455 ?
O6 Cs1 O1 90.5(2) 1_455 1_455 ?
O6 Cs1 O2W 47.5(2) 1_455 4_475 ?
O6 Cs1 O9W 138.6(2) 1_455 1_455 ?
O7 Cs1 O1 113.9(2) 4_576 1_455 ?
O7 Cs1 O6 107.9(2) 4_576 1_455 ?
O7 Cs1 O9 125.0(2) 4_576 1_455 ?
O7 Cs1 O13 60.8(2) 4_576 . ?
O7 Cs1 O14 110.3(2) 4_576 . ?
O7 Cs1 O2W 60.4(2) 4_576 4_475 ?
O7 Cs1 O4W 59.2(2) 4_576 1_455 ?
O7 Cs1 O7W 131.1(3) 4_576 . ?
O7 Cs1 O8W 71.7(3) 4_576 . ?
O7 Cs1 O9W 91.1(2) 4_576 1_455 ?
O7 Cs1 O16W 169.8(4) 4_576 3_566 ?
O9 Cs1 O1 45.4(2) 1_455 1_455 ?
O9 Cs1 O6 45.5(2) 1_455 1_455 ?
O9 Cs1 O13 153.1(2) 1_455 . ?
O9 Cs1 O14 123.1(2) 1_455 . ?
O9 Cs1 O2W 79.3(2) 1_455 4_475 ?
O9 Cs1 O4W 84.3(2) 1_455 1_455 ?
O9 Cs1 O7W 76.8(3) 1_455 . ?
O9 Cs1 O8W 140.7(3) 1_455 . ?
O9 Cs1 O9W 93.4(2) 1_455 1_455 ?
O13 Cs1 O1 161.4(2) . 1_455 ?
O13 Cs1 O6 108.1(2) . 1_455 ?
O13 Cs1 O2W 83.7(2) . 4_475 ?
O13 Cs1 O9W 113.3(2) . 1_455 ?
O14 Cs1 O1 122.8(2) . 1_455 ?
O14 Cs1 O6 108.6(2) . 1_455 ?
O14 Cs1 O13 52.3(2) . . ?
O14 Cs1 O2W 123.0(2) . 4_475 ?
O14 Cs1 O4W 140.8(2) . 1_455 ?
O14 Cs1 O7W 56.2(3) . . ?
O14 Cs1 O9W 97.9(2) . 1_455 ?
O2W Cs1 O9W 135.3(2) 4_475 1_455 ?
O4W Cs1 O1 54.9(2) 1_455 1_455 ?
O4W Cs1 O6 110.5(2) 1_455 1_455 ?
O4W Cs1 O13 115.5(2) 1_455 . ?
O4W Cs1 O2W 86.5(2) 1_455 4_475 ?
O4W Cs1 O7W 160.8(3) 1_455 . ?
O4W Cs1 O9W 48.9(3) 1_455 1_455 ?
O7W Cs1 O1 111.0(3) . 1_455 ?
O7W Cs1 O6 53.1(3) . 1_455 ?
O7W Cs1 O13 81.7(3) . . ?
O7W Cs1 O2W 87.0(3) . 4_475 ?
O7W Cs1 O9W 134.5(3) . 1_455 ?
O8W Cs1 O1 96.1(3) . 1_455 ?
O8W Cs1 O6 173.0(3) . 1_455 ?
O8W Cs1 O13 65.4(3) . . ?
O8W Cs1 O14 65.6(3) . . ?
O8W Cs1 O2W 131.4(3) . 4_475 ?
O8W Cs1 O4W 75.6(3) . 1_455 ?
O8W Cs1 O7W 121.6(3) . . ?
O8W Cs1 O9W 48.1(3) . 1_455 ?
O16W Cs1 O1 59.1(4) 3_566 1_455 ?
O16W Cs1 O6 80.4(4) 3_566 1_455 ?
O16W Cs1 O9 56.6(4) 3_566 1_455 ?
O16W Cs1 O13 123.1(4) 3_566 . ?
O16W Cs1 O14 71.4(4) 3_566 . ?
O16W Cs1 O2W 127.7(4) 3_566 4_475 ?
O16W Cs1 O4W 112.8(4) 3_566 1_455 ?
O16W Cs1 O7W 58.6(5) 3_566 . ?
O16W Cs1 O8W 100.8(5) 3_566 . ?
O16W Cs1 O9W 78.7(4) 3_566 1_455 ?
O8 K1 Ta3 27.30(17) . . ?
O8 K1 O11 77.0(3) . 4_575 ?
O8 K1 O20 57.4(2) . . ?
O8 K1 O8W 71.3(3) . 1_554 ?
O8 K1 O11W 128.9(3) . 3_666 ?
O8 K1 O12W 149.4(3) . . ?
O8 K1 O13W 117.5(4) . . ?
O8 K1 O17W 87.8(4) . . ?
O11 K1 Ta3 81.2(2) 4_575 . ?
O11 K1 O17W 159.5(4) 4_575 . ?
O20 K1 Ta3 30.52(16) . . ?
O20 K1 O11 94.5(3) . 4_575 ?
O20 K1 O8W 128.4(3) . 1_554 ?
O20 K1 O17W 65.4(4) . . ?
O8W K1 Ta3 97.9(3) 1_554 . ?
O8W K1 O11 66.9(3) 1_554 4_575 ?
O8W K1 O17W 121.2(4) 1_554 . ?
O11W K1 Ta3 102.0(3) 3_666 . ?
O11W K1 O11 111.6(3) 3_666 4_575 ?
O11W K1 O20 71.6(3) 3_666 . ?
O11W K1 O8W 159.6(4) 3_666 1_554 ?
O11W K1 O12W 73.1(3) 3_666 . ?
O11W K1 O17W 67.8(4) 3_666 . ?
O12W K1 Ta3 150.8(3) . . ?
O12W K1 O11 74.5(3) . 4_575 ?
O12W K1 O20 135.6(3) . . ?
O12W K1 O8W 87.3(4) . 1_554 ?
O12W K1 O17W 122.5(4) . . ?
O13W K1 Ta3 132.8(3) . . ?
O13W K1 O11 133.4(4) . 4_575 ?
O13W K1 O20 131.3(4) . . ?
O13W K1 O8W 76.3(4) . 1_554 ?
O13W K1 O11W 93.3(4) . 3_666 ?
O13W K1 O12W 76.3(4) . . ?
O13W K1 O17W 66.0(5) . . ?
O17W K1 Ta3 79.0(4) . . ?
Tb1 O1 Cs1 102.3(3) . 1_655 ?
Se4 O1 Tb1 127.9(4) . . ?
Se4 O1 Cs1 99.6(3) . 1_655 ?
O11 O2 Ta5 66.9(5) . . ?
O7 O3 Ta6 67.3(5) . . ?
Se3 O4 Tb1 176.5(5) . . ?
O6 O5 Ta2 69.0(5) . . ?
Ta2 O6 Cs1 115.9(3) . 1_655 ?
O5 O6 Ta2 67.0(4) . . ?
O5 O6 Cs1 175.6(6) . 1_655 ?
Ta6 O7 Cs1 147.7(4) . 4_575 ?
O3 O7 Ta6 67.8(5) . . ?
O3 O7 Cs1 130.9(6) . 4_575 ?
Ta3 O8 K1 111.4(4) . . ?
O12 O8 Ta3 67.6(5) . . ?
O12 O8 K1 109.0(5) . . ?
Ta2 O9 Cs1 121.5(3) . 1_655 ?
Se4 O9 Ta2 123.3(4) . . ?
Se4 O9 Cs1 111.9(4) . 1_655 ?
O14 O10 Ta4 67.5(5) . . ?
Ta5 O11 K1 148.4(5) . 4_576 ?
O2 O11 Ta5 69.2(5) . . ?
O2 O11 K1 124.9(6) . 4_576 ?
O8 O12 Ta3 67.2(5) . . ?
Ta4 O13 Cs1 104.1(3) . . ?
Se2 O13 Ta4 129.1(4) . . ?
Se2 O13 Cs1 109.3(3) . . ?
Ta4 O14 Cs1 112.5(3) . . ?
O10 O14 Ta4 69.0(5) . . ?
O10 O14 Cs1 106.0(5) . . ?
Se3 O15 Ta4 136.5(5) . . ?
O18 O16 Ta1 68.4(5) . . ?
Se3 O17 Ta5 130.9(4) . . ?
O16 O18 Ta1 67.3(5) . . ?
Ta6 O19 Ta3 162.8(5) . . ?
Ta3 O20 K1 103.7(3) . . ?
Se1 O20 Ta3 126.9(4) . . ?
Se1 O20 K1 121.9(4) . . ?
Se2 O21 Ta6 125.8(4) . . ?
Ta1 O22 Ta4 163.1(5) . . ?
Se2 O23 Ta5 130.8(4) . . ?
Se4 O24 Ta1 122.1(4) . . ?
Se1 O25 Ta1 131.1(4) . . ?
Ta2 O26 Ta5 167.5(5) . . ?
Se1 O27 Ta2 131.0(4) . . ?
Ta5 O28 Ta6 109.7(4) . . ?
Ta6 O29 Ta4 106.8(4) . . ?
Ta3 O30 Ta1 108.2(4) . . ?
Ta4 O31 Ta5 146.2(4) . . ?
Ta4 O31 Ta6 108.4(3) . . ?
Ta6 O31 Ta5 99.9(3) . . ?
Ta3 O32 Ta2 108.2(4) . . ?
Ta1 O33 Ta2 143.9(4) . . ?
Ta1 O33 Ta3 106.2(3) . . ?
Ta2 O33 Ta3 106.1(3) . . ?
Tb1 O2W Cs1 160.8(4) . 4_676 ?
Tb1 O4W Cs1 110.5(4) . 1_655 ?
K1 O8W Cs1 149.4(5) 1_556 . ?
Tb1 O9W Cs1 98.4(3) . 1_655 ?

_shelx_SHELXL_version_number     2018/1
_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy3_a
_database_code_depnum_ccdc_archive 'CCDC 1893228'
loop_
_audit_author_name
_audit_author_address
ddzhang
;Henan University
China
;
_audit_update_record             
;
2019-01-24 deposited with the CCDC.	2020-02-27 downloaded from the CCDC.
;
_audit_creation_date             2018-02-09
_audit_creation_method           
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs Dy K O46 Se4 Ta6, 4(O)'
_chemical_formula_sum            'Cs Dy K O50 Se4 Ta6'
_chemical_formula_weight         2536.05
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.2606(5)
_cell_length_b                   27.0796(12)
_cell_length_c                   13.9404(6)
_cell_angle_alpha                90
_cell_angle_beta                 114.0920(10)
_cell_angle_gamma                90
_cell_volume                     4225.2(3)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    5259
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.19
_cell_measurement_theta_min      2.40
_shelx_estimated_absorpt_T_max   0.129
_shelx_estimated_absorpt_T_min   0.074
_exptl_absorpt_coefficient_mu    21.745
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.3312
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1323 before and 0.0524 after correction.
The Ratio of minimum to maximum transmission is 0.4441.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.987
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4456
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.16
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0478
_diffrn_reflns_av_unetI/netI     0.0553
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            21760
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        25.098
_diffrn_reflns_theta_max         25.098
_diffrn_reflns_theta_min         1.819
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                6067
_reflns_number_total             7483
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         2.692
_refine_diff_density_min         -5.387
_refine_diff_density_rms         0.390
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.008
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7483
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0603
_refine_ls_R_factor_gt           0.0466
_refine_ls_restrained_S_all      1.008
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0543P)²+166.7232P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1143
_refine_ls_wR_factor_ref         0.1233
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28340(5) 0.54700(2) 0.55220(5) 0.01343(15) Uani 1 1 d . . . . .
Ta2 Ta 0.43579(5) 0.65678(2) 0.46499(5) 0.01278(15) Uani 1 1 d . . . . .
Ta3 Ta 0.16896(5) 0.60609(2) 0.32376(5) 0.01401(15) Uani 1 1 d . . . . .
Ta4 Ta 0.13506(5) 0.64038(2) 0.66150(5) 0.01390(15) Uani 1 1 d . . . . .
Ta5 Ta 0.27994(5) 0.75181(2) 0.56892(5) 0.01409(15) Uani 1 1 d . . . . .
Ta6 Ta 0.02746(6) 0.70074(2) 0.43289(5) 0.01589(16) Uani 1 1 d . . . . .
Dy1 Dy 0.68409(7) 0.64901(3) 0.98163(6) 0.02113(19) Uani 1 1 d . . . . .
Se1 Se 0.41517(14) 0.53475(6) 0.37776(12) 0.0176(3) Uani 1 1 d . . . . .
Se2 Se 0.04662(14) 0.76090(6) 0.65439(13) 0.0197(4) Uani 1 1 d . . . . .
Se3 Se 0.37651(13) 0.71236(6) 0.82353(12) 0.0156(3) Uani 1 1 d . . . . .
Se4 Se 0.49182(14) 0.62303(6) 0.70934(12) 0.0191(3) Uani 1 1 d . . . . .
Cs1 Cs -0.1868(2) 0.65962(11) 0.7158(2) 0.1024(8) Uani 1 1 d . . . . .
K1 K 0.2263(6) 0.5753(2) 0.0595(5) 0.0692(18) Uani 1 1 d . . . . .
O1 O 0.6197(10) 0.6129(5) 0.8144(9) 0.027(3) Uiso 1 1 d . . . . .
O2 O 0.3828(12) 0.8002(5) 0.5413(11) 0.039(3) Uiso 1 1 d . . . . .
O3 O -0.1423(10) 0.6935(5) 0.3372(9) 0.028(3) Uiso 1 1 d . . . . .
O4 O 0.5080(10) 0.6877(4) 0.8930(9) 0.023(3) Uiso 1 1 d . . . . .
O5 O 0.5001(10) 0.6915(4) 0.3756(9) 0.024(3) Uiso 1 1 d . . . . .
O6 O 0.5949(10) 0.6839(4) 0.4836(9) 0.022(3) Uiso 1 1 d . . . . .
O7 O -0.0848(10) 0.7369(5) 0.3108(9) 0.027(3) Uiso 1 1 d . . . . .
O8 O 0.0918(10) 0.6168(4) 0.1699(9) 0.024(3) Uiso 1 1 d . . . . .
O9 O 0.5433(10) 0.6363(4) 0.6154(9) 0.023(3) Uiso 1 1 d . . . . .
O10 O 0.1260(10) 0.6046(5) 0.7822(9) 0.026(3) Uiso 1 1 d . . . . .
O11 O 0.3133(13) 0.8230(6) 0.5925(11) 0.045(4) Uiso 1 1 d . . . . .
O12 O 0.0290(11) 0.5779(5) 0.2065(10) 0.033(3) Uiso 1 1 d . . . . .
O13 O 0.0692(10) 0.7031(4) 0.7046(9) 0.023(3) Uiso 1 1 d . . . . .
O14 O 0.0140(11) 0.5987(5) 0.6844(9) 0.028(3) Uiso 1 1 d . . . . .
O15 O 0.2970(10) 0.6601(4) 0.7792(8) 0.020(2) Uiso 1 1 d . . . . .
O16 O 0.1993(10) 0.4846(4) 0.5493(9) 0.024(3) Uiso 1 1 d . . . . .
O17 O 0.3969(10) 0.7284(4) 0.7127(9) 0.022(3) Uiso 1 1 d . . . . .
O18 O 0.3140(10) 0.4873(5) 0.6408(9) 0.026(3) Uiso 1 1 d . . . . .
O19 O 0.0838(10) 0.6558(4) 0.3578(9) 0.023(3) Uiso 1 1 d . . . . .
O20 O 0.2765(9) 0.5539(4) 0.2913(8) 0.018(2) Uiso 1 1 d . . . . .
O21 O -0.0292(9) 0.7482(4) 0.5239(8) 0.020(2) Uiso 1 1 d . . . . .
O22 O 0.2072(9) 0.5872(4) 0.6197(8) 0.020(2) Uiso 1 1 d . . . . .
O23 O 0.1836(10) 0.7773(5) 0.6595(9) 0.027(3) Uiso 1 1 d . . . . .
O24 O 0.4472(10) 0.5632(4) 0.6726(8) 0.021(2) Uiso 1 1 d . . . . .
O25 O 0.3790(10) 0.5149(4) 0.4779(9) 0.024(3) Uiso 1 1 d . . . . .
O26 O 0.3683(9) 0.7079(4) 0.5109(8) 0.019(2) Uiso 1 1 d . . . . .
O27 O 0.4888(10) 0.5882(4) 0.4206(9) 0.022(2) Uiso 1 1 d . . . . .
O28 O 0.1387(10) 0.7558(4) 0.4399(9) 0.024(3) Uiso 1 1 d . . . . .
O29 O -0.0092(10) 0.6451(4) 0.5165(9) 0.021(2) Uiso 1 1 d . . . . .
O30 O 0.1350(9) 0.5533(4) 0.4097(8) 0.020(2) Uiso 1 1 d . . . . .
O31 O 0.1788(9) 0.6893(4) 0.5702(8) 0.016(2) Uiso 1 1 d . . . . .
O32 O 0.2902(10) 0.6568(4) 0.3189(8) 0.020(2) Uiso 1 1 d . . . . .
O33 O 0.3066(9) 0.6079(4) 0.4730(8) 0.015(2) Uiso 1 1 d . . . . .
O1W O 0.5637(12) 0.6379(5) 1.0778(11) 0.042(3) Uiso 1 1 d . . . . .
O2W O 0.7050(12) 0.7271(5) 1.0785(11) 0.041(3) Uiso 1 1 d . . . . .
O3W O 0.8238(13) 0.6371(6) 1.1578(12) 0.046(4) Uiso 1 1 d . . . . .
O4W O 0.7556(14) 0.7086(6) 0.9001(12) 0.054(4) Uiso 1 1 d . . . . .
O5W O -0.0524(12) 0.5004(5) 0.3415(11) 0.042(3) Uiso 1 1 d . . . . .
O6W O 0.6282(14) 0.7682(6) 0.7452(13) 0.056(4) Uiso 1 1 d . . . . .
O7W O -0.2192(14) 0.6146(6) 0.5036(12) 0.055(4) Uiso 1 1 d . . . . .
O8W O 0.0390(17) 0.6474(7) 0.9174(15) 0.076(6) Uiso 1 1 d . . . . .
O9W O 0.8652(18) 0.6190(8) 0.9763(16) 0.082(6) Uiso 1 1 d . . . . .
O10W O 0.6797(16) 0.5636(7) 1.0040(14) 0.066(5) Uiso 1 1 d . . . . .
O11W O 0.5735(17) 0.4952(7) 0.8420(15) 0.073(5) Uiso 1 1 d . . . . .
O12W O 0.3628(18) 0.5810(8) -0.0599(16) 0.085(6) Uiso 1 1 d . . . . .
O13W O 0.099(2) 0.5163(11) -0.090(2) 0.121(9) Uiso 1 1 d . . . . .
O14W O 0.346(2) 0.4939(10) 0.8480(19) 0.107(8) Uiso 1 1 d . . . . .
O15W O 0.5983(19) 0.6123(8) 1.2728(17) 0.089(6) Uiso 1 1 d . . . . .
O16W O 0.138(5) 0.463(2) 0.174(4) 0.23(2) Uiso 1 1 d . . . . .
O17W O 0.063(8) 0.487(4) 0.081(7) 0.41(5) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3200(9) . ?
Ta1 O16 1.971(12) . ?
Ta1 O18 1.975(12) . ?
Ta1 O22 1.914(11) . ?
Ta1 O24 2.072(11) . ?
Ta1 O25 2.048(11) . ?
Ta1 O30 2.082(11) . ?
Ta1 O33 2.068(10) . ?
Ta2 Ta3 3.3473(9) . ?
Ta2 Cs1 4.520(2) 1_655 ?
Ta2 O5 1.965(11) . ?
Ta2 O6 1.999(11) . ?
Ta2 O9 2.046(11) . ?
Ta2 O26 1.856(11) . ?
Ta2 O27 2.142(12) . ?
Ta2 O32 2.089(11) . ?
Ta2 O33 2.102(10) . ?
Ta3 K1 4.109(6) . ?
Ta3 O8 1.981(11) . ?
Ta3 O12 1.976(13) . ?
Ta3 O19 1.879(11) . ?
Ta3 O20 2.103(11) . ?
Ta3 O30 2.014(11) . ?
Ta3 O32 2.045(11) . ?
Ta3 O33 2.077(10) . ?
Ta4 Ta6 3.3371(9) . ?
Ta4 Cs1 4.343(2) . ?
Ta4 O10 1.983(12) . ?
Ta4 O13 2.072(12) . ?
Ta4 O14 1.992(12) . ?
Ta4 O15 2.064(11) . ?
Ta4 O22 1.901(11) . ?
Ta4 O29 2.077(11) . ?
Ta4 O31 2.053(10) . ?
Ta5 Ta6 3.2091(9) . ?
Ta5 O2 1.963(14) . ?
Ta5 O11 1.970(16) . ?
Ta5 O17 2.032(11) . ?
Ta5 O23 2.165(12) . ?
Ta5 O26 1.989(11) . ?
Ta5 O28 1.924(11) . ?
Ta5 O31 2.104(10) . ?
Ta6 O3 1.971(12) . ?
Ta6 O7 1.959(12) . ?
Ta6 O19 1.909(11) . ?
Ta6 O21 2.113(11) . ?
Ta6 O28 1.996(12) . ?
Ta6 O29 2.063(11) . ?
Ta6 O31 2.075(10) . ?
Dy1 Cs1 4.594(3) 1_655 ?
Dy1 O1 2.348(12) . ?
Dy1 O4 2.260(11) . ?
Dy1 O1W 2.384(14) . ?
Dy1 O2W 2.465(15) . ?
Dy1 O3W 2.374(15) . ?
Dy1 O4W 2.341(16) . ?
Dy1 O9W 2.39(2) . ?
Dy1 O10W 2.337(19) . ?
Se1 O20 1.715(11) . ?
Se1 O25 1.715(11) . ?
Se1 O27 1.680(12) . ?
Se2 Cs1 4.295(3) . ?
Se2 O13 1.690(12) . ?
Se2 O21 1.706(11) . ?
Se2 O23 1.710(12) . ?
Se3 O4 1.646(11) . ?
Se3 O15 1.686(11) . ?
Se3 O17 1.718(11) . ?
Se4 Cs1 4.028(3) 1_655 ?
Se4 O1 1.674(12) . ?
Se4 O9 1.708(11) . ?
Se4 O24 1.720(11) . ?
Cs1 O1 3.432(12) 1_455 ?
Cs1 O6 3.317(11) 1_455 ?
Cs1 O7 3.133(13) 4_576 ?
Cs1 O9 3.086(11) 1_455 ?
Cs1 O13 3.415(11) . ?
Cs1 O14 3.140(12) . ?
Cs1 O2W 3.572(15) 4_475 ?
Cs1 O4W 3.216(16) 1_455 ?
Cs1 O7W 3.072(16) . ?
Cs1 O8W 3.05(2) . ?
Cs1 O9W 3.59(2) 1_455 ?
Cs1 O16W 3.60(6) 3_566 ?
K1 O8 2.902(13) . ?
K1 O11 2.923(17) 4_575 ?
K1 O20 3.088(12) . ?
K1 O8W 3.05(2) 1_554 ?
K1 O11W 2.97(2) 3_666 ?
K1 O12W 2.80(2) . ?
K1 O13W 2.58(3) . ?
K1 O17W 3.20(10) . ?
O2 O11 1.454(19) . ?
O3 O7 1.492(17) . ?
O5 O6 1.494(15) . ?
O8 O12 1.510(17) . ?
O10 O14 1.497(16) . ?
O16 O18 1.465(15) . ?
O16W O17W 1.42(8) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Ta1 Ta3 112.4(3) . . ?
O16 Ta1 O18 43.6(5) . . ?
O16 Ta1 O24 121.6(5) . . ?
O16 Ta1 O25 91.6(5) . . ?
O16 Ta1 O30 78.8(5) . . ?
O16 Ta1 O33 149.0(4) . . ?
O18 Ta1 Ta3 153.2(3) . . ?
O18 Ta1 O24 78.0(5) . . ?
O18 Ta1 O25 88.1(5) . . ?
O18 Ta1 O30 122.2(5) . . ?
O18 Ta1 O33 162.6(4) . . ?
O22 Ta1 Ta3 95.6(3) . . ?
O22 Ta1 O16 98.1(5) . . ?
O22 Ta1 O18 99.4(5) . . ?
O22 Ta1 O24 89.3(4) . . ?
O22 Ta1 O25 170.2(5) . . ?
O22 Ta1 O30 90.6(4) . . ?
O22 Ta1 O33 90.6(4) . . ?
O24 Ta1 Ta3 124.4(3) . . ?
O24 Ta1 O30 159.4(4) . . ?
O25 Ta1 Ta3 79.9(3) . . ?
O25 Ta1 O24 86.2(4) . . ?
O25 Ta1 O30 90.6(4) . . ?
O25 Ta1 O33 80.6(4) . . ?
O30 Ta1 Ta3 35.2(3) . . ?
O33 Ta1 Ta3 36.9(3) . . ?
O33 Ta1 O24 88.0(4) . . ?
O33 Ta1 O30 71.4(4) . . ?
Ta3 Ta2 Cs1 155.23(4) . 1_655 ?
O5 Ta2 Ta3 111.8(3) . . ?
O5 Ta2 Cs1 86.2(3) . 1_655 ?
O5 Ta2 O6 44.3(5) . . ?
O5 Ta2 O9 121.5(5) . . ?
O5 Ta2 O27 89.1(5) . . ?
O5 Ta2 O32 77.7(4) . . ?
O5 Ta2 O33 147.3(4) . . ?
O6 Ta2 Ta3 153.4(3) . . ?
O6 Ta2 Cs1 42.0(3) . 1_655 ?
O6 Ta2 O9 77.3(4) . . ?
O6 Ta2 O27 87.8(4) . . ?
O6 Ta2 O32 121.8(4) . . ?
O6 Ta2 O33 160.2(4) . . ?
O9 Ta2 Ta3 123.9(3) . . ?
O9 Ta2 Cs1 35.3(3) . 1_655 ?
O9 Ta2 O27 85.2(4) . . ?
O9 Ta2 O32 159.4(4) . . ?
O9 Ta2 O33 87.7(4) . . ?
O26 Ta2 Ta3 92.4(3) . . ?
O26 Ta2 Cs1 100.4(3) . 1_655 ?
O26 Ta2 O5 102.3(5) . . ?
O26 Ta2 O6 103.3(5) . . ?
O26 Ta2 O9 92.3(5) . . ?
O26 Ta2 O27 167.9(5) . . ?
O26 Ta2 O32 90.7(4) . . ?
O26 Ta2 O33 90.0(4) . . ?
O27 Ta2 Ta3 79.2(3) . . ?
O27 Ta2 Cs1 84.4(3) . 1_655 ?
O32 Ta2 Ta3 35.5(3) . . ?
O32 Ta2 Cs1 162.1(3) . 1_655 ?
O32 Ta2 O27 87.6(4) . . ?
O32 Ta2 O33 71.9(4) . . ?
O33 Ta2 Ta3 36.5(3) . . ?
O33 Ta2 Cs1 121.7(3) . 1_655 ?
O33 Ta2 O27 78.1(4) . . ?
Ta1 Ta3 Ta2 72.817(19) . . ?
Ta1 Ta3 K1 127.03(8) . . ?
Ta2 Ta3 K1 97.29(10) . . ?
O8 Ta3 Ta1 159.6(3) . . ?
O8 Ta3 Ta2 119.8(3) . . ?
O8 Ta3 K1 40.5(3) . . ?
O8 Ta3 O20 85.9(4) . . ?
O8 Ta3 O30 128.6(5) . . ?
O8 Ta3 O32 84.2(5) . . ?
O8 Ta3 O33 156.2(4) . . ?
O12 Ta3 Ta1 119.4(4) . . ?
O12 Ta3 Ta2 162.7(4) . . ?
O12 Ta3 K1 65.7(4) . . ?
O12 Ta3 O8 44.9(5) . . ?
O12 Ta3 O20 88.4(5) . . ?
O12 Ta3 O30 84.1(5) . . ?
O12 Ta3 O32 129.0(5) . . ?
O12 Ta3 O33 156.0(5) . . ?
O19 Ta3 Ta1 99.4(3) . . ?
O19 Ta3 Ta2 93.9(3) . . ?
O19 Ta3 K1 133.5(4) . . ?
O19 Ta3 O8 95.7(5) . . ?
O19 Ta3 O12 95.8(5) . . ?
O19 Ta3 O20 175.4(5) . . ?
O19 Ta3 O30 95.0(5) . . ?
O19 Ta3 O32 90.7(5) . . ?
O19 Ta3 O33 92.2(4) . . ?
O20 Ta3 Ta1 80.0(3) . . ?
O20 Ta3 Ta2 81.6(3) . . ?
O20 Ta3 K1 47.1(3) . . ?
O30 Ta3 Ta1 36.5(3) . . ?
O30 Ta3 Ta2 109.3(3) . . ?
O30 Ta3 K1 122.8(3) . . ?
O30 Ta3 O20 87.2(4) . . ?
O30 Ta3 O32 145.6(4) . . ?
O30 Ta3 O33 72.6(4) . . ?
O32 Ta3 Ta1 109.1(3) . . ?
O32 Ta3 Ta2 36.4(3) . . ?
O32 Ta3 K1 73.4(3) . . ?
O32 Ta3 O20 85.2(4) . . ?
O32 Ta3 O33 73.3(4) . . ?
O33 Ta3 Ta1 36.7(3) . . ?
O33 Ta3 Ta2 37.0(3) . . ?
O33 Ta3 K1 122.5(3) . . ?
O33 Ta3 O20 84.7(4) . . ?
Ta6 Ta4 Cs1 94.28(4) . . ?
O10 Ta4 Ta6 155.8(3) . . ?
O10 Ta4 Cs1 62.7(3) . . ?
O10 Ta4 O13 89.5(5) . . ?
O10 Ta4 O14 44.2(5) . . ?
O10 Ta4 O15 79.7(5) . . ?
O10 Ta4 O29 122.4(5) . . ?
O10 Ta4 O31 163.7(5) . . ?
O13 Ta4 Ta6 80.0(3) . . ?
O13 Ta4 Cs1 50.3(3) . . ?
O13 Ta4 O29 87.3(4) . . ?
O14 Ta4 Ta6 113.6(3) . . ?
O14 Ta4 Cs1 41.4(4) . . ?
O14 Ta4 O13 90.8(5) . . ?
O14 Ta4 O15 123.9(5) . . ?
O14 Ta4 O29 78.3(5) . . ?
O14 Ta4 O31 149.9(4) . . ?
O15 Ta4 Ta6 120.6(3) . . ?
O15 Ta4 Cs1 118.6(3) . . ?
O15 Ta4 O13 85.4(4) . . ?
O15 Ta4 O29 156.7(4) . . ?
O22 Ta4 Ta6 97.5(3) . . ?
O22 Ta4 Cs1 135.5(3) . . ?
O22 Ta4 O10 94.8(5) . . ?
O22 Ta4 O13 174.0(5) . . ?
O22 Ta4 O14 95.2(5) . . ?
O22 Ta4 O15 91.3(4) . . ?
O22 Ta4 O29 93.8(4) . . ?
O22 Ta4 O31 91.5(4) . . ?
O29 Ta4 Ta6 36.1(3) . . ?
O29 Ta4 Cs1 71.9(3) . . ?
O31 Ta4 Ta6 36.3(3) . . ?
O31 Ta4 Cs1 121.1(3) . . ?
O31 Ta4 O13 83.2(4) . . ?
O31 Ta4 O15 85.2(4) . . ?
O31 Ta4 O29 72.0(4) . . ?
O2 Ta5 Ta6 135.5(4) . . ?
O2 Ta5 O11 43.4(6) . . ?
O2 Ta5 O17 98.7(5) . . ?
O2 Ta5 O23 116.7(5) . . ?
O2 Ta5 O26 79.6(5) . . ?
O2 Ta5 O31 165.3(5) . . ?
O11 Ta5 Ta6 127.2(4) . . ?
O11 Ta5 O17 97.3(5) . . ?
O11 Ta5 O23 73.5(5) . . ?
O11 Ta5 O26 122.8(5) . . ?
O11 Ta5 O31 150.4(5) . . ?
O17 Ta5 Ta6 124.8(3) . . ?
O17 Ta5 O23 81.8(4) . . ?
O17 Ta5 O31 85.5(4) . . ?
O23 Ta5 Ta6 81.8(3) . . ?
O26 Ta5 Ta6 93.2(3) . . ?
O26 Ta5 O17 86.1(4) . . ?
O26 Ta5 O23 161.0(5) . . ?
O26 Ta5 O31 86.7(4) . . ?
O28 Ta5 Ta6 35.8(3) . . ?
O28 Ta5 O2 100.6(5) . . ?
O28 Ta5 O11 98.5(5) . . ?
O28 Ta5 O17 160.5(5) . . ?
O28 Ta5 O23 91.8(5) . . ?
O28 Ta5 O26 94.8(5) . . ?
O28 Ta5 O31 75.2(4) . . ?
O31 Ta5 Ta6 39.5(3) . . ?
O31 Ta5 O23 77.8(4) . . ?
Ta5 Ta6 Ta4 74.74(2) . . ?
O3 Ta6 Ta4 119.6(4) . . ?
O3 Ta6 Ta5 160.2(4) . . ?
O3 Ta6 O21 87.2(5) . . ?
O3 Ta6 O28 128.3(5) . . ?
O3 Ta6 O29 84.0(5) . . ?
O3 Ta6 O31 155.4(5) . . ?
O7 Ta6 Ta4 159.7(3) . . ?
O7 Ta6 Ta5 117.7(4) . . ?
O7 Ta6 O3 44.6(5) . . ?
O7 Ta6 O21 86.0(5) . . ?
O7 Ta6 O28 83.9(5) . . ?
O7 Ta6 O29 128.2(5) . . ?
O7 Ta6 O31 157.4(5) . . ?
O19 Ta6 Ta4 97.0(3) . . ?
O19 Ta6 Ta5 96.9(3) . . ?
O19 Ta6 O3 94.8(5) . . ?
O19 Ta6 O7 97.2(5) . . ?
O19 Ta6 O21 176.7(5) . . ?
O19 Ta6 O28 96.3(5) . . ?
O19 Ta6 O29 93.2(5) . . ?
O19 Ta6 O31 91.3(4) . . ?
O21 Ta6 Ta4 79.8(3) . . ?
O21 Ta6 Ta5 81.8(3) . . ?
O28 Ta6 Ta4 108.9(3) . . ?
O28 Ta6 Ta5 34.3(3) . . ?
O28 Ta6 O21 84.4(4) . . ?
O28 Ta6 O29 145.1(5) . . ?
O28 Ta6 O31 74.4(4) . . ?
O29 Ta6 Ta4 36.4(3) . . ?
O29 Ta6 Ta5 111.1(3) . . ?
O29 Ta6 O21 84.5(4) . . ?
O29 Ta6 O31 71.8(4) . . ?
O31 Ta6 Ta4 35.8(3) . . ?
O31 Ta6 Ta5 40.2(3) . . ?
O31 Ta6 O21 85.8(4) . . ?
O1 Dy1 Cs1 46.6(3) . 1_655 ?
O1 Dy1 O1W 118.1(5) . . ?
O1 Dy1 O2W 145.0(4) . . ?
O1 Dy1 O3W 141.1(5) . . ?
O1 Dy1 O9W 76.6(6) . . ?
O4 Dy1 Cs1 95.6(3) . 1_655 ?
O4 Dy1 O1 78.0(4) . . ?
O4 Dy1 O1W 72.1(4) . . ?
O4 Dy1 O2W 76.4(4) . . ?
O4 Dy1 O3W 138.9(5) . . ?
O4 Dy1 O4W 83.0(5) . . ?
O4 Dy1 O9W 146.3(6) . . ?
O4 Dy1 O10W 117.6(5) . . ?
O1W Dy1 Cs1 163.3(3) . 1_655 ?
O1W Dy1 O2W 75.5(5) . . ?
O1W Dy1 O9W 140.3(6) . . ?
O2W Dy1 Cs1 113.3(3) . 1_655 ?
O3W Dy1 Cs1 120.2(4) . 1_655 ?
O3W Dy1 O1W 75.6(5) . . ?
O3W Dy1 O2W 71.4(5) . . ?
O3W Dy1 O9W 72.5(6) . . ?
O4W Dy1 Cs1 41.0(4) . 1_655 ?
O4W Dy1 O1 81.2(5) . . ?
O4W Dy1 O1W 143.2(5) . . ?
O4W Dy1 O2W 72.4(5) . . ?
O4W Dy1 O3W 109.9(5) . . ?
O4W Dy1 O9W 71.5(7) . . ?
O9W Dy1 Cs1 50.7(5) . 1_655 ?
O9W Dy1 O2W 114.7(6) . . ?
O10W Dy1 Cs1 101.8(4) . 1_655 ?
O10W Dy1 O1 72.7(5) . . ?
O10W Dy1 O1W 75.3(6) . . ?
O10W Dy1 O2W 141.1(5) . . ?
O10W Dy1 O3W 76.9(6) . . ?
O10W Dy1 O4W 141.3(6) . . ?
O10W Dy1 O9W 75.0(7) . . ?
O20 Se1 O25 98.9(5) . . ?
O27 Se1 O20 102.9(5) . . ?
O27 Se1 O25 105.1(5) . . ?
O13 Se2 Cs1 48.4(4) . . ?
O13 Se2 O21 100.4(5) . . ?
O13 Se2 O23 103.4(6) . . ?
O21 Se2 Cs1 88.1(4) . . ?
O21 Se2 O23 101.3(5) . . ?
O23 Se2 Cs1 151.7(4) . . ?
O4 Se3 O15 99.0(6) . . ?
O4 Se3 O17 99.5(5) . . ?
O15 Se3 O17 99.0(5) . . ?
O1 Se4 Cs1 57.5(4) . 1_655 ?
O1 Se4 O9 101.4(6) . . ?
O1 Se4 O24 100.1(6) . . ?
O9 Se4 Cs1 45.7(4) . 1_655 ?
O9 Se4 O24 98.2(5) . . ?
O24 Se4 Cs1 115.3(4) . 1_655 ?
O1 Cs1 O2W 111.4(3) 1_455 4_475 ?
O1 Cs1 O9W 49.4(4) 1_455 1_455 ?
O1 Cs1 O16W 60.7(8) 1_455 3_566 ?
O6 Cs1 O1 92.8(3) 1_455 1_455 ?
O6 Cs1 O13 106.1(3) 1_455 . ?
O6 Cs1 O2W 48.1(3) 1_455 4_475 ?
O6 Cs1 O9W 141.9(4) 1_455 1_455 ?
O6 Cs1 O16W 121.8(9) 1_455 3_566 ?
O7 Cs1 O1 112.5(3) 4_576 1_455 ?
O7 Cs1 O6 105.0(3) 4_576 1_455 ?
O7 Cs1 O13 59.7(3) 4_576 . ?
O7 Cs1 O14 109.2(3) 4_576 . ?
O7 Cs1 O2W 57.0(3) 4_576 4_475 ?
O7 Cs1 O4W 58.2(4) 4_576 1_455 ?
O7 Cs1 O9W 88.4(4) 4_576 1_455 ?
O7 Cs1 O16W 132.4(9) 4_576 3_566 ?
O9 Cs1 O1 47.0(3) 1_455 1_455 ?
O9 Cs1 O6 46.3(3) 1_455 1_455 ?
O9 Cs1 O7 122.9(3) 1_455 4_576 ?
O9 Cs1 O13 152.2(3) 1_455 . ?
O9 Cs1 O14 125.9(3) 1_455 . ?
O9 Cs1 O2W 80.7(3) 1_455 4_475 ?
O9 Cs1 O4W 84.4(4) 1_455 1_455 ?
O9 Cs1 O9W 96.4(4) 1_455 1_455 ?
O9 Cs1 O16W 88.1(8) 1_455 3_566 ?
O13 Cs1 O1 160.7(3) . 1_455 ?
O13 Cs1 O2W 80.0(3) . 4_475 ?
O13 Cs1 O9W 111.4(4) . 1_455 ?
O13 Cs1 O16W 110.0(8) . 3_566 ?
O14 Cs1 O1 124.9(3) . 1_455 ?
O14 Cs1 O6 109.5(3) . 1_455 ?
O14 Cs1 O13 52.2(3) . . ?
O14 Cs1 O2W 121.2(3) . 4_475 ?
O14 Cs1 O4W 140.2(4) . 1_455 ?
O14 Cs1 O9W 98.9(4) . 1_455 ?
O14 Cs1 O16W 64.7(8) . 3_566 ?
O2W Cs1 O9W 132.7(4) 4_475 1_455 ?
O2W Cs1 O16W 168.6(9) 4_475 3_566 ?
O4W Cs1 O1 54.5(4) 1_455 1_455 ?
O4W Cs1 O6 110.2(4) 1_455 1_455 ?
O4W Cs1 O13 113.6(4) 1_455 . ?
O4W Cs1 O2W 85.4(4) 1_455 4_475 ?
O4W Cs1 O9W 47.6(5) 1_455 1_455 ?
O4W Cs1 O16W 95.2(9) 1_455 3_566 ?
O7W Cs1 O1 113.6(4) . 1_455 ?
O7W Cs1 O6 53.4(4) . 1_455 ?
O7W Cs1 O7 129.3(4) . 4_576 ?
O7W Cs1 O9 77.8(4) . 1_455 ?
O7W Cs1 O13 81.5(4) . . ?
O7W Cs1 O14 57.1(4) . . ?
O7W Cs1 O2W 87.2(4) . 4_475 ?
O7W Cs1 O4W 161.6(4) . 1_455 ?
O7W Cs1 O9W 138.7(5) . 1_455 ?
O7W Cs1 O16W 88.9(9) . 3_566 ?
O8W Cs1 O1 96.1(4) . 1_455 ?
O8W Cs1 O6 170.8(4) . 1_455 ?
O8W Cs1 O7 69.6(4) . 4_576 ?
O8W Cs1 O9 142.9(4) . 1_455 ?
O8W Cs1 O13 64.8(4) . . ?
O8W Cs1 O14 66.6(4) . . ?
O8W Cs1 O2W 125.8(5) . 4_475 ?
O8W Cs1 O4W 73.8(5) . 1_455 ?
O8W Cs1 O7W 123.7(5) . . ?
O8W Cs1 O9W 46.9(5) . 1_455 ?
O8W Cs1 O16W 65.0(9) . 3_566 ?
O9W Cs1 O16W 49.9(9) 1_455 3_566 ?
O8 K1 Ta3 26.3(2) . . ?
O8 K1 O11 78.5(4) . 4_575 ?
O8 K1 O20 55.3(3) . . ?
O8 K1 O8W 69.9(5) . 1_554 ?
O8 K1 O11W 123.0(5) . 3_666 ?
O8 K1 O17W 74.1(18) . . ?
O11 K1 Ta3 81.5(3) 4_575 . ?
O11 K1 O20 96.2(4) 4_575 . ?
O11 K1 O8W 68.1(5) 4_575 1_554 ?
O11 K1 O11W 110.7(5) 4_575 3_666 ?
O11 K1 O17W 152.6(18) 4_575 . ?
O20 K1 Ta3 29.9(2) . . ?
O20 K1 O17W 68.2(15) . . ?
O8W K1 Ta3 95.3(4) 1_554 . ?
O8W K1 O20 125.1(5) 1_554 . ?
O8W K1 O17W 101.7(16) 1_554 . ?
O11W K1 Ta3 97.3(4) 3_666 . ?
O11W K1 O20 67.8(4) 3_666 . ?
O11W K1 O8W 167.0(6) 3_666 1_554 ?
O11W K1 O17W 84.8(17) 3_666 . ?
O12W K1 Ta3 152.0(5) . . ?
O12W K1 O8 154.0(6) . . ?
O12W K1 O11 76.9(6) . 4_575 ?
O12W K1 O20 136.0(5) . . ?
O12W K1 O8W 93.1(6) . 1_554 ?
O12W K1 O11W 74.3(6) . 3_666 ?
O12W K1 O17W 130.1(18) . . ?
O13W K1 Ta3 125.4(6) . . ?
O13W K1 O8 112.2(7) . . ?
O13W K1 O11 140.6(7) . 4_575 ?
O13W K1 O20 121.6(7) . . ?
O13W K1 O8W 79.9(8) . 1_554 ?
O13W K1 O11W 95.2(7) . 3_666 ?
O13W K1 O12W 82.5(8) . . ?
O13W K1 O17W 54.5(17) . . ?
O17W K1 Ta3 74.0(17) . . ?
Dy1 O1 Cs1 103.7(4) . 1_655 ?
Se4 O1 Dy1 128.0(6) . . ?
Se4 O1 Cs1 98.2(5) . 1_655 ?
O11 O2 Ta5 68.5(8) . . ?
O7 O3 Ta6 67.3(6) . . ?
Se3 O4 Dy1 176.0(7) . . ?
O6 O5 Ta2 69.1(6) . . ?
Ta2 O6 Cs1 114.2(4) . 1_655 ?
O5 O6 Ta2 66.6(6) . . ?
O5 O6 Cs1 175.5(8) . 1_655 ?
Ta6 O7 Cs1 146.3(6) . 4_575 ?
O3 O7 Ta6 68.1(6) . . ?
O3 O7 Cs1 131.4(8) . 4_575 ?
Ta3 O8 K1 113.2(5) . . ?
O12 O8 Ta3 67.4(6) . . ?
O12 O8 K1 112.9(8) . . ?
Ta2 O9 Cs1 122.2(5) . 1_655 ?
Se4 O9 Ta2 123.9(6) . . ?
Se4 O9 Cs1 111.0(5) . 1_655 ?
O14 O10 Ta4 68.2(6) . . ?
Ta5 O11 K1 149.2(7) . 4_576 ?
O2 O11 Ta5 68.1(8) . . ?
O2 O11 K1 124.9(10) . 4_576 ?
O8 O12 Ta3 67.7(6) . . ?
Ta4 O13 Cs1 101.8(4) . . ?
Se2 O13 Ta4 131.0(6) . . ?
Se2 O13 Cs1 109.9(5) . . ?
Ta4 O14 Cs1 113.7(5) . . ?
O10 O14 Ta4 67.6(6) . . ?
O10 O14 Cs1 107.3(7) . . ?
Se3 O15 Ta4 137.2(6) . . ?
O18 O16 Ta1 68.3(7) . . ?
Se3 O17 Ta5 131.5(6) . . ?
O16 O18 Ta1 68.1(6) . . ?
Ta3 O19 Ta6 163.3(7) . . ?
Ta3 O20 K1 103.0(4) . . ?
Se1 O20 Ta3 125.5(6) . . ?
Se1 O20 K1 120.6(5) . . ?
Se2 O21 Ta6 126.4(6) . . ?
Ta4 O22 Ta1 164.4(7) . . ?
Se2 O23 Ta5 130.8(7) . . ?
Se4 O24 Ta1 121.7(6) . . ?
Se1 O25 Ta1 132.1(7) . . ?
Ta2 O26 Ta5 168.4(6) . . ?
Se1 O27 Ta2 131.9(6) . . ?
Ta5 O28 Ta6 109.9(5) . . ?
Ta6 O29 Ta4 107.5(5) . . ?
Ta3 O30 Ta1 108.3(5) . . ?
Ta4 O31 Ta5 145.9(5) . . ?
Ta4 O31 Ta6 107.9(5) . . ?
Ta6 O31 Ta5 100.4(4) . . ?
Ta3 O32 Ta2 108.1(5) . . ?
Ta1 O33 Ta2 143.3(5) . . ?
Ta1 O33 Ta3 106.5(5) . . ?
Ta3 O33 Ta2 106.4(4) . . ?
Dy1 O2W Cs1 164.4(5) . 4_676 ?
Dy1 O4W Cs1 110.5(6) . 1_655 ?
K1 O8W Cs1 145.7(7) 1_556 . ?
Dy1 O9W Cs1 98.2(6) . 1_655 ?
O17W O16W Cs1 140(5) . 3_566 ?
O16W O17W K1 104(5) . . ?

_shelx_SHELXL_version_number     2018/1
_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy4_a
_database_code_depnum_ccdc_archive 'CCDC 1893229'
loop_
_audit_author_name
_audit_author_address
ddzhang
;Henan University
China
;
_audit_update_record             
;
2019-01-24 deposited with the CCDC.	2020-02-27 downloaded from the CCDC.
;
_audit_creation_date             2018-02-09
_audit_creation_method           
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs Ho K O46 Se4 Ta6, 4(O)'
_chemical_formula_sum            'Cs Ho K O50 Se4 Ta6'
_chemical_formula_weight         2538.48
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ho Ho -0.2175 4.6783 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.3009(7)
_cell_length_b                   27.3358(17)
_cell_length_c                   14.0022(8)
_cell_angle_alpha                90
_cell_angle_beta                 114.0180(10)
_cell_angle_gamma                90
_cell_volume                     4300.7(4)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    2698
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.64
_cell_measurement_theta_min      2.18
_shelx_estimated_absorpt_T_max   0.279
_shelx_estimated_absorpt_T_min   0.141
_exptl_absorpt_coefficient_mu    21.466
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.3957
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1379 before and 0.0614 after correction.
The Ratio of minimum to maximum transmission is 0.5306.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.921
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4460
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.08
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0730
_diffrn_reflns_av_unetI/netI     0.0824
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            22334
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.758
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                5593
_reflns_number_total             7653
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         2.059
_refine_diff_density_min         -3.168
_refine_diff_density_rms         0.380
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.027
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7653
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0693
_refine_ls_R_factor_gt           0.0433
_refine_ls_restrained_S_all      1.027
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0273P)²+41.4008P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0911
_refine_ls_wR_factor_ref         0.1032
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28621(5) 0.54904(2) 0.55603(5) 0.01234(15) Uani 1 1 d . . . . .
Ta2 Ta 0.43785(5) 0.65825(2) 0.47101(5) 0.01254(15) Uani 1 1 d . . . . .
Ta3 Ta 0.17245(5) 0.60814(2) 0.32858(5) 0.01291(15) Uani 1 1 d . . . . .
Ta4 Ta 0.13701(5) 0.64091(2) 0.66468(5) 0.01266(15) Uani 1 1 d . . . . .
Ta5 Ta 0.28270(5) 0.75226(2) 0.57590(5) 0.01286(15) Uani 1 1 d . . . . .
Ta6 Ta 0.03301(5) 0.70193(2) 0.43890(5) 0.01374(16) Uani 1 1 d . . . . .
Ho1 Ho 0.68513(6) 0.64960(3) 0.98583(5) 0.01630(18) Uani 1 1 d . . . . .
Se1 Se 0.41805(14) 0.53768(6) 0.38182(12) 0.0172(4) Uani 1 1 d . . . . .
Se2 Se 0.04951(14) 0.76020(6) 0.66036(12) 0.0171(4) Uani 1 1 d . . . . .
Se3 Se 0.37802(14) 0.71178(6) 0.82857(12) 0.0159(4) Uani 1 1 d . . . . .
Se4 Se 0.49254(14) 0.62434(6) 0.71413(12) 0.0190(4) Uani 1 1 d . . . . .
Cs1 Cs -0.18079(13) 0.66411(6) 0.72058(13) 0.0574(4) Uani 1 1 d . . . . .
K1 K 0.2244(4) 0.57279(19) 0.0712(4) 0.0508(13) Uani 1 1 d . . . . .
O1 O 0.6207(9) 0.6145(4) 0.8172(8) 0.021(3) Uiso 1 1 d . . . . .
O2 O 0.3869(10) 0.7998(4) 0.5498(9) 0.030(3) Uiso 1 1 d . . . . .
O3 O -0.1367(10) 0.6941(4) 0.3432(9) 0.026(3) Uiso 1 1 d . . . . .
O4 O 0.5095(10) 0.6874(4) 0.8980(9) 0.027(3) Uiso 1 1 d . . . . .
O5 O 0.5032(9) 0.6928(4) 0.3827(8) 0.023(3) Uiso 1 1 d . . . . .
O6 O 0.5961(9) 0.6850(4) 0.4905(8) 0.021(3) Uiso 1 1 d . . . . .
O7 O -0.0771(9) 0.7378(4) 0.3177(8) 0.023(3) Uiso 1 1 d . . . . .
O8 O 0.0954(9) 0.6192(4) 0.1761(8) 0.019(2) Uiso 1 1 d . . . . .
O9 O 0.5447(9) 0.6371(4) 0.6211(8) 0.020(3) Uiso 1 1 d . . . . .
O10 O 0.1263(10) 0.6046(4) 0.7827(9) 0.025(3) Uiso 1 1 d . . . . .
O11 O 0.3173(10) 0.8217(5) 0.6012(9) 0.032(3) Uiso 1 1 d . . . . .
O12 O 0.0332(9) 0.5805(4) 0.2132(8) 0.023(3) Uiso 1 1 d . . . . .
O13 O 0.0701(9) 0.7022(4) 0.7099(8) 0.024(3) Uiso 1 1 d . . . . .
O14 O 0.0165(10) 0.5990(4) 0.6858(9) 0.027(3) Uiso 1 1 d . . . . .
O15 O 0.2975(9) 0.6593(4) 0.7832(8) 0.020(3) Uiso 1 1 d . . . . .
O16 O 0.2021(10) 0.4860(4) 0.5502(8) 0.024(3) Uiso 1 1 d . . . . .
O17 O 0.3987(9) 0.7287(4) 0.7194(8) 0.016(2) Uiso 1 1 d . . . . .
O18 O 0.3190(9) 0.4897(4) 0.6445(8) 0.024(3) Uiso 1 1 d . . . . .
O19 O 0.0883(9) 0.6581(4) 0.3630(8) 0.016(2) Uiso 1 1 d . . . . .
O20 O 0.2827(8) 0.5578(4) 0.2972(7) 0.015(2) Uiso 1 1 d . . . . .
O21 O -0.0249(9) 0.7485(4) 0.5306(8) 0.022(3) Uiso 1 1 d . . . . .
O22 O 0.2106(9) 0.5881(4) 0.6240(8) 0.016(2) Uiso 1 1 d . . . . .
O23 O 0.1866(10) 0.7758(4) 0.6684(8) 0.024(3) Uiso 1 1 d . . . . .
O24 O 0.4488(9) 0.5654(4) 0.6763(8) 0.023(3) Uiso 1 1 d . . . . .
O25 O 0.3831(9) 0.5169(4) 0.4827(8) 0.018(2) Uiso 1 1 d . . . . .
O26 O 0.3716(9) 0.7079(4) 0.5177(8) 0.018(2) Uiso 1 1 d . . . . .
O27 O 0.4953(9) 0.5903(4) 0.4278(8) 0.020(3) Uiso 1 1 d . . . . .
O28 O 0.1449(9) 0.7564(4) 0.4490(8) 0.019(2) Uiso 1 1 d . . . . .
O29 O -0.0043(9) 0.6457(4) 0.5199(8) 0.020(3) Uiso 1 1 d . . . . .
O30 O 0.1395(9) 0.5547(4) 0.4136(8) 0.017(2) Uiso 1 1 d . . . . .
O31 O 0.1837(8) 0.6899(4) 0.5775(7) 0.014(2) Uiso 1 1 d . . . . .
O32 O 0.2944(8) 0.6583(4) 0.3250(7) 0.014(2) Uiso 1 1 d . . . . .
O33 O 0.3120(8) 0.6091(4) 0.4790(7) 0.012(2) Uiso 1 1 d . . . . .
O1W O 0.5635(10) 0.6370(5) 1.0808(9) 0.031(3) Uiso 1 1 d . . . . .
O2W O 0.6974(10) 0.7262(5) 1.0805(9) 0.034(3) Uiso 1 1 d . . . . .
O3W O 0.8314(10) 0.6401(5) 1.1598(9) 0.033(3) Uiso 1 1 d . . . . .
O4W O 0.7560(10) 0.7103(5) 0.9063(9) 0.033(3) Uiso 1 1 d . . . . .
O5W O -0.0445(11) 0.4986(5) 0.3459(10) 0.043(3) Uiso 1 1 d . . . . .
O6W O 0.6277(11) 0.7689(5) 0.7511(10) 0.042(3) Uiso 1 1 d . . . . .
O7W O -0.2188(13) 0.6148(6) 0.4957(12) 0.061(4) Uiso 1 1 d . . . . .
O8W O 0.0534(12) 0.6444(5) 0.9278(11) 0.051(4) Uiso 1 1 d . . . . .
O9W O 0.8628(11) 0.6165(5) 0.9765(10) 0.043(4) Uiso 1 1 d . . . . .
O10W O 0.6741(11) 0.5655(5) 1.0062(10) 0.038(3) Uiso 1 1 d . . . . .
O11W O 0.5829(13) 0.4979(6) 0.8455(11) 0.056(4) Uiso 1 1 d . . . . .
O12W O 0.3615(13) 0.5812(6) -0.0574(11) 0.056(4) Uiso 1 1 d . . . . .
O13W O 0.0940(14) 0.5151(6) -0.1069(12) 0.068(5) Uiso 1 1 d . . . . .
O14W O 0.3547(13) 0.4920(6) 0.8538(12) 0.063(4) Uiso 1 1 d . . . . .
O15W O 0.5963(19) 0.6137(8) 1.2745(17) 0.111(7) Uiso 1 1 d . . . . .
O16W O 0.276(2) 0.4411(10) 0.3386(19) 0.133(9) Uiso 1 1 d . . . . .
O17W O 0.137(2) 0.4687(9) 0.1291(18) 0.121(8) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3292(9) . ?
Ta1 O16 1.993(11) . ?
Ta1 O18 1.979(11) . ?
Ta1 O22 1.906(10) . ?
Ta1 O24 2.072(11) . ?
Ta1 O25 2.061(10) . ?
Ta1 O30 2.080(10) . ?
Ta1 O33 2.058(10) . ?
Ta2 Ta3 3.3485(9) . ?
Ta2 Cs1 4.5715(17) 1_655 ?
Ta2 O5 1.969(11) . ?
Ta2 O6 1.991(10) . ?
Ta2 O9 2.056(10) . ?
Ta2 O26 1.835(10) . ?
Ta2 O27 2.160(11) . ?
Ta2 O32 2.087(10) . ?
Ta2 O33 2.088(10) . ?
Ta3 K1 4.025(5) . ?
Ta3 O8 1.976(10) . ?
Ta3 O12 1.966(11) . ?
Ta3 O19 1.890(10) . ?
Ta3 O20 2.100(10) . ?
Ta3 O30 2.027(10) . ?
Ta3 O32 2.048(10) . ?
Ta3 O33 2.107(9) . ?
Ta4 Ta6 3.3349(9) . ?
Ta4 Cs1 4.3346(16) . ?
Ta4 O10 1.978(11) . ?
Ta4 O13 2.077(11) . ?
Ta4 O14 1.988(11) . ?
Ta4 O15 2.059(10) . ?
Ta4 O22 1.909(10) . ?
Ta4 O29 2.068(10) . ?
Ta4 O31 2.046(10) . ?
Ta5 Ta6 3.1952(9) . ?
Ta5 O2 1.961(12) . ?
Ta5 O11 1.946(13) . ?
Ta5 O17 2.039(10) . ?
Ta5 O23 2.177(11) . ?
Ta5 O26 2.014(10) . ?
Ta5 O28 1.895(10) . ?
Ta5 O31 2.100(10) . ?
Ta6 O3 1.981(11) . ?
Ta6 O7 1.950(11) . ?
Ta6 O19 1.902(10) . ?
Ta6 O21 2.127(11) . ?
Ta6 O28 1.994(10) . ?
Ta6 O29 2.071(11) . ?
Ta6 O31 2.093(10) . ?
Ho1 Cs1 4.6538(17) 1_655 ?
Ho1 O1 2.366(10) . ?
Ho1 O4 2.254(11) . ?
Ho1 O1W 2.397(12) . ?
Ho1 O2W 2.449(13) . ?
Ho1 O3W 2.381(12) . ?
Ho1 O4W 2.354(12) . ?
Ho1 O9W 2.419(13) . ?
Ho1 O10W 2.328(13) . ?
Se1 O20 1.695(10) . ?
Se1 O25 1.731(10) . ?
Se1 O27 1.699(11) . ?
Se2 Cs1 4.193(2) . ?
Se2 O13 1.707(11) . ?
Se2 O21 1.699(11) . ?
Se2 O23 1.698(11) . ?
Se3 O4 1.651(11) . ?
Se3 O15 1.711(11) . ?
Se3 O17 1.712(10) . ?
Se4 Cs1 4.128(2) 1_655 ?
Se4 O1 1.670(11) . ?
Se4 O9 1.707(10) . ?
Se4 O24 1.713(11) . ?
Cs1 O1 3.510(11) 1_455 ?
Cs1 O6 3.322(10) 1_455 ?
Cs1 O7 3.043(11) 4_576 ?
Cs1 O9 3.171(10) 1_455 ?
Cs1 O13 3.318(11) . ?
Cs1 O14 3.201(11) . ?
Cs1 O2W 3.563(13) 4_475 ?
Cs1 O4W 3.257(12) 1_455 ?
Cs1 O7W 3.279(15) . ?
Cs1 O8W 3.194(14) . ?
Cs1 O9W 3.641(13) 1_455 ?
Cs1 O16W 3.09(3) 3_566 ?
K1 O8 2.860(11) . ?
K1 O11 3.068(14) 4_575 ?
K1 O20 2.975(11) . ?
K1 O8W 2.975(15) 1_554 ?
K1 O11W 2.910(16) 3_666 ?
K1 O12W 2.936(15) . ?
K1 O13W 2.832(17) . ?
K1 O17W 3.26(2) . ?
O2 O11 1.453(15) . ?
O3 O7 1.519(15) . ?
O5 O6 1.492(14) . ?
O8 O12 1.517(14) . ?
O10 O14 1.482(15) . ?
O16 O18 1.508(14) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Ta1 Ta3 111.8(3) . . ?
O16 Ta1 O24 122.2(4) . . ?
O16 Ta1 O25 90.4(4) . . ?
O16 Ta1 O30 78.0(4) . . ?
O16 Ta1 O33 148.8(4) . . ?
O18 Ta1 Ta3 153.5(3) . . ?
O18 Ta1 O16 44.6(4) . . ?
O18 Ta1 O24 77.6(4) . . ?
O18 Ta1 O25 87.2(4) . . ?
O18 Ta1 O30 122.5(4) . . ?
O18 Ta1 O33 161.0(4) . . ?
O22 Ta1 Ta3 96.0(3) . . ?
O22 Ta1 O16 98.9(4) . . ?
O22 Ta1 O18 99.4(4) . . ?
O22 Ta1 O24 88.8(4) . . ?
O22 Ta1 O25 170.7(4) . . ?
O22 Ta1 O30 91.6(4) . . ?
O22 Ta1 O33 91.5(4) . . ?
O24 Ta1 Ta3 124.3(3) . . ?
O24 Ta1 O30 159.5(4) . . ?
O25 Ta1 Ta3 80.4(3) . . ?
O25 Ta1 O24 86.2(4) . . ?
O25 Ta1 O30 90.4(4) . . ?
O30 Ta1 Ta3 35.3(3) . . ?
O33 Ta1 Ta3 37.5(3) . . ?
O33 Ta1 O24 87.1(4) . . ?
O33 Ta1 O25 80.5(4) . . ?
O33 Ta1 O30 72.4(4) . . ?
Ta3 Ta2 Cs1 156.63(3) . 1_655 ?
O5 Ta2 Ta3 111.8(3) . . ?
O5 Ta2 Cs1 84.8(3) . 1_655 ?
O5 Ta2 O6 44.2(4) . . ?
O5 Ta2 O9 121.4(4) . . ?
O5 Ta2 O27 88.5(4) . . ?
O5 Ta2 O32 77.5(4) . . ?
O5 Ta2 O33 147.6(4) . . ?
O6 Ta2 Ta3 153.3(3) . . ?
O6 Ta2 Cs1 40.6(3) . 1_655 ?
O6 Ta2 O9 77.3(4) . . ?
O6 Ta2 O27 86.7(4) . . ?
O6 Ta2 O32 121.6(4) . . ?
O6 Ta2 O33 159.1(4) . . ?
O9 Ta2 Ta3 123.8(3) . . ?
O9 Ta2 Cs1 36.7(3) . 1_655 ?
O9 Ta2 O27 84.2(4) . . ?
O9 Ta2 O32 159.2(4) . . ?
O9 Ta2 O33 86.8(4) . . ?
O26 Ta2 Ta3 92.7(3) . . ?
O26 Ta2 Cs1 99.7(3) . 1_655 ?
O26 Ta2 O5 102.9(5) . . ?
O26 Ta2 O6 103.3(4) . . ?
O26 Ta2 O9 92.1(4) . . ?
O26 Ta2 O27 168.3(4) . . ?
O26 Ta2 O32 91.6(4) . . ?
O26 Ta2 O33 90.6(4) . . ?
O27 Ta2 Ta3 80.3(3) . . ?
O27 Ta2 Cs1 83.9(3) . 1_655 ?
O32 Ta2 Ta3 35.5(3) . . ?
O32 Ta2 Cs1 160.7(3) . 1_655 ?
O32 Ta2 O27 88.2(4) . . ?
O32 Ta2 O33 72.7(4) . . ?
O33 Ta2 Ta3 37.2(3) . . ?
O33 Ta2 Cs1 122.3(3) . 1_655 ?
O33 Ta2 O27 78.2(4) . . ?
Ta1 Ta3 Ta2 72.57(2) . . ?
Ta1 Ta3 K1 125.59(7) . . ?
Ta2 Ta3 K1 99.20(8) . . ?
O8 Ta3 Ta1 159.8(3) . . ?
O8 Ta3 Ta2 120.2(3) . . ?
O8 Ta3 K1 41.4(3) . . ?
O8 Ta3 O20 86.6(4) . . ?
O8 Ta3 O30 128.5(4) . . ?
O8 Ta3 O32 84.6(4) . . ?
O8 Ta3 O33 156.3(4) . . ?
O12 Ta3 Ta1 119.1(3) . . ?
O12 Ta3 Ta2 163.6(3) . . ?
O12 Ta3 K1 64.8(3) . . ?
O12 Ta3 O8 45.3(4) . . ?
O12 Ta3 O20 89.8(4) . . ?
O12 Ta3 O30 83.7(4) . . ?
O12 Ta3 O32 129.8(4) . . ?
O12 Ta3 O33 155.4(4) . . ?
O19 Ta3 Ta1 99.6(3) . . ?
O19 Ta3 Ta2 93.1(3) . . ?
O19 Ta3 K1 134.8(3) . . ?
O19 Ta3 O8 95.4(4) . . ?
O19 Ta3 O12 95.9(4) . . ?
O19 Ta3 O20 173.6(4) . . ?
O19 Ta3 O30 96.3(4) . . ?
O19 Ta3 O32 90.3(4) . . ?
O19 Ta3 O33 92.5(4) . . ?
O20 Ta3 Ta1 80.0(3) . . ?
O20 Ta3 Ta2 80.6(3) . . ?
O20 Ta3 K1 45.9(3) . . ?
O20 Ta3 O33 83.3(4) . . ?
O30 Ta3 Ta1 36.4(3) . . ?
O30 Ta3 Ta2 108.9(3) . . ?
O30 Ta3 K1 119.7(3) . . ?
O30 Ta3 O20 87.2(4) . . ?
O30 Ta3 O32 145.1(4) . . ?
O30 Ta3 O33 72.4(4) . . ?
O32 Ta3 Ta1 108.7(3) . . ?
O32 Ta3 Ta2 36.3(3) . . ?
O32 Ta3 K1 75.8(3) . . ?
O32 Ta3 O20 83.8(4) . . ?
O32 Ta3 O33 73.1(4) . . ?
O33 Ta3 Ta1 36.4(3) . . ?
O33 Ta3 Ta2 36.8(3) . . ?
O33 Ta3 K1 122.4(3) . . ?
Ta6 Ta4 Cs1 94.12(3) . . ?
O10 Ta4 Ta6 155.9(3) . . ?
O10 Ta4 Cs1 63.3(3) . . ?
O10 Ta4 O13 88.9(4) . . ?
O10 Ta4 O14 43.9(4) . . ?
O10 Ta4 O15 79.5(4) . . ?
O10 Ta4 O29 122.4(4) . . ?
O10 Ta4 O31 163.3(4) . . ?
O13 Ta4 Ta6 80.7(3) . . ?
O13 Ta4 Cs1 47.8(3) . . ?
O14 Ta4 Ta6 114.0(3) . . ?
O14 Ta4 Cs1 43.6(3) . . ?
O14 Ta4 O13 90.4(5) . . ?
O14 Ta4 O15 123.3(4) . . ?
O14 Ta4 O29 78.6(4) . . ?
O14 Ta4 O31 150.8(4) . . ?
O15 Ta4 Ta6 120.9(3) . . ?
O15 Ta4 Cs1 117.2(3) . . ?
O15 Ta4 O13 85.7(4) . . ?
O15 Ta4 O29 157.2(4) . . ?
O22 Ta4 Ta6 98.1(3) . . ?
O22 Ta4 Cs1 137.4(3) . . ?
O22 Ta4 O10 94.1(4) . . ?
O22 Ta4 O13 174.8(4) . . ?
O22 Ta4 O14 94.7(5) . . ?
O22 Ta4 O15 90.6(4) . . ?
O22 Ta4 O29 93.8(4) . . ?
O22 Ta4 O31 92.0(4) . . ?
O29 Ta4 Ta6 36.3(3) . . ?
O29 Ta4 Cs1 73.0(3) . . ?
O29 Ta4 O13 88.2(4) . . ?
O31 Ta4 Ta6 36.8(3) . . ?
O31 Ta4 Cs1 120.3(3) . . ?
O31 Ta4 O13 84.0(4) . . ?
O31 Ta4 O15 84.9(4) . . ?
O31 Ta4 O29 72.7(4) . . ?
O2 Ta5 Ta6 135.6(3) . . ?
O2 Ta5 O17 98.3(4) . . ?
O2 Ta5 O23 118.0(5) . . ?
O2 Ta5 O26 79.6(5) . . ?
O2 Ta5 O31 164.9(4) . . ?
O11 Ta5 Ta6 127.9(3) . . ?
O11 Ta5 O2 43.7(5) . . ?
O11 Ta5 O17 96.6(5) . . ?
O11 Ta5 O23 74.6(5) . . ?
O11 Ta5 O26 123.1(5) . . ?
O11 Ta5 O31 151.0(4) . . ?
O17 Ta5 Ta6 124.9(3) . . ?
O17 Ta5 O23 80.7(4) . . ?
O17 Ta5 O31 84.8(4) . . ?
O23 Ta5 Ta6 82.1(3) . . ?
O26 Ta5 Ta6 92.6(3) . . ?
O26 Ta5 O17 86.0(4) . . ?
O26 Ta5 O23 159.2(4) . . ?
O26 Ta5 O31 85.9(4) . . ?
O28 Ta5 Ta6 35.8(3) . . ?
O28 Ta5 O2 100.9(5) . . ?
O28 Ta5 O11 99.1(5) . . ?
O28 Ta5 O17 160.6(4) . . ?
O28 Ta5 O23 92.6(4) . . ?
O28 Ta5 O26 94.7(4) . . ?
O28 Ta5 O31 76.0(4) . . ?
O31 Ta5 Ta6 40.3(3) . . ?
O31 Ta5 O23 77.1(4) . . ?
Ta5 Ta6 Ta4 75.06(2) . . ?
O3 Ta6 Ta4 118.6(3) . . ?
O3 Ta6 Ta5 160.7(3) . . ?
O3 Ta6 O21 87.3(4) . . ?
O3 Ta6 O28 129.5(4) . . ?
O3 Ta6 O29 83.2(4) . . ?
O3 Ta6 O31 154.4(4) . . ?
O7 Ta6 Ta4 159.8(3) . . ?
O7 Ta6 Ta5 117.6(3) . . ?
O7 Ta6 O3 45.5(4) . . ?
O7 Ta6 O21 86.5(4) . . ?
O7 Ta6 O28 84.4(4) . . ?
O7 Ta6 O29 128.3(4) . . ?
O7 Ta6 O31 157.7(4) . . ?
O19 Ta6 Ta4 97.3(3) . . ?
O19 Ta6 Ta5 97.6(3) . . ?
O19 Ta6 O3 94.1(4) . . ?
O19 Ta6 O7 96.3(4) . . ?
O19 Ta6 O21 177.0(4) . . ?
O19 Ta6 O28 96.7(4) . . ?
O19 Ta6 O29 92.7(4) . . ?
O19 Ta6 O31 92.0(4) . . ?
O21 Ta6 Ta4 79.7(3) . . ?
O21 Ta6 Ta5 81.7(3) . . ?
O28 Ta6 Ta4 108.6(3) . . ?
O28 Ta6 Ta5 33.7(3) . . ?
O28 Ta6 O21 84.3(4) . . ?
O28 Ta6 O29 144.8(4) . . ?
O28 Ta6 O31 74.1(4) . . ?
O29 Ta6 Ta4 36.3(3) . . ?
O29 Ta6 Ta5 111.4(3) . . ?
O29 Ta6 O21 84.8(4) . . ?
O29 Ta6 O31 71.7(4) . . ?
O31 Ta6 Ta4 35.8(3) . . ?
O31 Ta6 Ta5 40.4(3) . . ?
O31 Ta6 O21 85.5(4) . . ?
O1 Ho1 Cs1 47.3(3) . 1_655 ?
O1 Ho1 O1W 117.6(4) . . ?
O1 Ho1 O2W 143.9(4) . . ?
O1 Ho1 O3W 141.6(4) . . ?
O1 Ho1 O9W 74.8(4) . . ?
O4 Ho1 Cs1 95.6(3) . 1_655 ?
O4 Ho1 O1 77.5(4) . . ?
O4 Ho1 O1W 72.1(4) . . ?
O4 Ho1 O2W 74.8(4) . . ?
O4 Ho1 O3W 139.9(4) . . ?
O4 Ho1 O4W 82.9(4) . . ?
O4 Ho1 O9W 145.9(4) . . ?
O4 Ho1 O10W 115.4(4) . . ?
O1W Ho1 Cs1 163.5(3) . 1_655 ?
O1W Ho1 O2W 74.8(4) . . ?
O1W Ho1 O9W 139.3(4) . . ?
O2W Ho1 Cs1 113.3(3) . 1_655 ?
O3W Ho1 Cs1 117.4(3) . 1_655 ?
O3W Ho1 O1W 78.4(4) . . ?
O3W Ho1 O2W 71.6(4) . . ?
O3W Ho1 O9W 72.0(4) . . ?
O4W Ho1 Cs1 40.8(3) . 1_655 ?
O4W Ho1 O1 81.5(4) . . ?
O4W Ho1 O1W 143.0(4) . . ?
O4W Ho1 O2W 72.6(4) . . ?
O4W Ho1 O3W 106.8(4) . . ?
O4W Ho1 O9W 73.8(4) . . ?
O9W Ho1 Cs1 50.7(3) . 1_655 ?
O9W Ho1 O2W 119.4(4) . . ?
O10W Ho1 Cs1 103.9(3) . 1_655 ?
O10W Ho1 O1 73.1(4) . . ?
O10W Ho1 O1W 73.1(4) . . ?
O10W Ho1 O2W 140.5(4) . . ?
O10W Ho1 O3W 79.9(4) . . ?
O10W Ho1 O4W 143.7(4) . . ?
O10W Ho1 O9W 74.7(4) . . ?
O20 Se1 O25 100.2(5) . . ?
O20 Se1 O27 103.3(5) . . ?
O27 Se1 O25 104.8(5) . . ?
O13 Se2 Cs1 48.5(4) . . ?
O21 Se2 Cs1 89.0(4) . . ?
O21 Se2 O13 100.7(5) . . ?
O23 Se2 Cs1 151.4(4) . . ?
O23 Se2 O13 103.2(5) . . ?
O23 Se2 O21 101.9(5) . . ?
O4 Se3 O15 99.2(5) . . ?
O4 Se3 O17 99.7(5) . . ?
O15 Se3 O17 99.7(5) . . ?
O1 Se4 Cs1 57.0(4) . 1_655 ?
O1 Se4 O9 100.2(5) . . ?
O1 Se4 O24 100.6(5) . . ?
O9 Se4 Cs1 45.4(4) . 1_655 ?
O9 Se4 O24 97.2(5) . . ?
O24 Se4 Cs1 115.8(4) . 1_655 ?
O1 Cs1 O2W 109.6(3) 1_455 4_475 ?
O1 Cs1 O9W 47.9(3) 1_455 1_455 ?
O6 Cs1 O1 90.6(3) 1_455 1_455 ?
O6 Cs1 O2W 47.5(3) 1_455 4_475 ?
O6 Cs1 O9W 138.4(3) 1_455 1_455 ?
O7 Cs1 O1 113.5(3) 4_576 1_455 ?
O7 Cs1 O6 108.2(3) 4_576 1_455 ?
O7 Cs1 O9 125.4(3) 4_576 1_455 ?
O7 Cs1 O13 61.0(3) 4_576 . ?
O7 Cs1 O14 110.6(3) 4_576 . ?
O7 Cs1 O2W 60.7(3) 4_576 4_475 ?
O7 Cs1 O4W 59.6(3) 4_576 1_455 ?
O7 Cs1 O7W 131.4(3) 4_576 . ?
O7 Cs1 O8W 71.5(3) 4_576 . ?
O7 Cs1 O9W 90.5(3) 4_576 1_455 ?
O7 Cs1 O16W 170.0(5) 4_576 3_566 ?
O9 Cs1 O1 45.3(3) 1_455 1_455 ?
O9 Cs1 O6 45.8(3) 1_455 1_455 ?
O9 Cs1 O13 153.7(3) 1_455 . ?
O9 Cs1 O14 122.8(3) 1_455 . ?
O9 Cs1 O2W 79.6(3) 1_455 4_475 ?
O9 Cs1 O4W 83.3(3) 1_455 1_455 ?
O9 Cs1 O7W 76.8(3) 1_455 . ?
O9 Cs1 O8W 139.9(3) 1_455 . ?
O9 Cs1 O9W 93.1(3) 1_455 1_455 ?
O13 Cs1 O1 160.8(3) . 1_455 ?
O13 Cs1 O6 108.6(3) . 1_455 ?
O13 Cs1 O2W 84.3(3) . 4_475 ?
O13 Cs1 O9W 112.9(3) . 1_455 ?
O14 Cs1 O1 122.2(3) . 1_455 ?
O14 Cs1 O6 109.0(3) . 1_455 ?
O14 Cs1 O13 52.5(3) . . ?
O14 Cs1 O2W 124.0(3) . 4_475 ?
O14 Cs1 O4W 141.1(3) . 1_455 ?
O14 Cs1 O7W 56.4(3) . . ?
O14 Cs1 O9W 97.7(3) . 1_455 ?
O2W Cs1 O9W 134.7(3) 4_475 1_455 ?
O4W Cs1 O1 54.0(3) 1_455 1_455 ?
O4W Cs1 O6 109.6(3) 1_455 1_455 ?
O4W Cs1 O13 116.3(3) 1_455 . ?
O4W Cs1 O2W 86.0(3) 1_455 4_475 ?
O4W Cs1 O7W 159.9(3) 1_455 . ?
O4W Cs1 O9W 48.7(3) 1_455 1_455 ?
O7W Cs1 O1 111.2(3) . 1_455 ?
O7W Cs1 O6 53.2(3) . 1_455 ?
O7W Cs1 O13 81.8(3) . . ?
O7W Cs1 O2W 87.3(3) . 4_475 ?
O7W Cs1 O9W 134.8(4) . 1_455 ?
O8W Cs1 O1 95.5(3) . 1_455 ?
O8W Cs1 O6 173.4(3) . 1_455 ?
O8W Cs1 O13 65.3(3) . . ?
O8W Cs1 O14 65.5(3) . . ?
O8W Cs1 O2W 131.6(3) . 4_475 ?
O8W Cs1 O4W 76.1(3) . 1_455 ?
O8W Cs1 O7W 121.8(4) . . ?
O8W Cs1 O9W 47.8(3) . 1_455 ?
O16W Cs1 O1 59.8(5) 3_566 1_455 ?
O16W Cs1 O6 80.1(5) 3_566 1_455 ?
O16W Cs1 O9 56.4(5) 3_566 1_455 ?
O16W Cs1 O13 122.5(5) 3_566 . ?
O16W Cs1 O14 70.7(5) 3_566 . ?
O16W Cs1 O2W 127.4(5) 3_566 4_475 ?
O16W Cs1 O4W 112.8(5) 3_566 1_455 ?
O16W Cs1 O7W 57.9(5) 3_566 . ?
O16W Cs1 O8W 100.9(5) 3_566 . ?
O16W Cs1 O9W 79.6(5) 3_566 1_455 ?
O8 K1 Ta3 27.2(2) . . ?
O8 K1 O11 76.5(3) . 4_575 ?
O8 K1 O20 57.2(3) . . ?
O8 K1 O8W 70.6(4) . 1_554 ?
O8 K1 O11W 128.4(4) . 3_666 ?
O8 K1 O12W 149.1(4) . . ?
O8 K1 O17W 87.2(5) . . ?
O11 K1 Ta3 80.7(2) 4_575 . ?
O11 K1 O17W 158.3(5) 4_575 . ?
O20 K1 Ta3 30.5(2) . . ?
O20 K1 O11 94.0(3) . 4_575 ?
O20 K1 O17W 64.9(5) . . ?
O8W K1 Ta3 96.9(3) 1_554 . ?
O8W K1 O11 66.1(4) 1_554 4_575 ?
O8W K1 O20 127.4(4) 1_554 . ?
O8W K1 O17W 121.9(5) 1_554 . ?
O11W K1 Ta3 101.6(3) 3_666 . ?
O11W K1 O11 111.9(4) 3_666 4_575 ?
O11W K1 O20 71.2(4) 3_666 . ?
O11W K1 O8W 160.8(4) 3_666 1_554 ?
O11W K1 O12W 73.7(4) 3_666 . ?
O11W K1 O17W 67.6(5) 3_666 . ?
O12W K1 Ta3 150.6(3) . . ?
O12W K1 O11 74.7(4) . 4_575 ?
O12W K1 O20 135.5(4) . . ?
O12W K1 O8W 87.7(4) . 1_554 ?
O12W K1 O17W 123.5(5) . . ?
O13W K1 Ta3 133.1(4) . . ?
O13W K1 O8 117.7(4) . . ?
O13W K1 O11 133.6(4) . 4_575 ?
O13W K1 O20 131.7(4) . . ?
O13W K1 O8W 77.3(4) . 1_554 ?
O13W K1 O11W 93.4(5) . 3_666 ?
O13W K1 O12W 76.4(4) . . ?
O13W K1 O17W 66.9(5) . . ?
O17W K1 Ta3 78.3(4) . . ?
Ho1 O1 Cs1 103.0(3) . 1_655 ?
Se4 O1 Ho1 127.7(6) . . ?
Se4 O1 Cs1 99.5(4) . 1_655 ?
O11 O2 Ta5 67.6(7) . . ?
O7 O3 Ta6 66.2(6) . . ?
Se3 O4 Ho1 176.2(7) . . ?
O6 O5 Ta2 68.7(6) . . ?
Ta2 O6 Cs1 116.4(4) . 1_655 ?
O5 O6 Ta2 67.1(6) . . ?
O5 O6 Cs1 174.7(7) . 1_655 ?
Ta6 O7 Cs1 148.0(5) . 4_575 ?
O3 O7 Ta6 68.3(6) . . ?
O3 O7 Cs1 130.1(7) . 4_575 ?
Ta3 O8 K1 111.4(4) . . ?
O12 O8 Ta3 67.0(6) . . ?
O12 O8 K1 109.2(7) . . ?
Ta2 O9 Cs1 120.5(4) . 1_655 ?
Se4 O9 Ta2 123.7(6) . . ?
Se4 O9 Cs1 112.1(5) . 1_655 ?
O14 O10 Ta4 68.4(6) . . ?
Ta5 O11 K1 148.3(5) . 4_576 ?
O2 O11 Ta5 68.7(7) . . ?
O2 O11 K1 125.5(8) . 4_576 ?
O8 O12 Ta3 67.7(6) . . ?
Ta4 O13 Cs1 104.6(4) . . ?
Se2 O13 Ta4 129.6(6) . . ?
Se2 O13 Cs1 108.9(5) . . ?
Ta4 O14 Cs1 111.1(5) . . ?
O10 O14 Ta4 67.7(6) . . ?
O10 O14 Cs1 105.5(7) . . ?
Se3 O15 Ta4 136.4(6) . . ?
O18 O16 Ta1 67.2(6) . . ?
Se3 O17 Ta5 131.8(5) . . ?
O16 O18 Ta1 68.2(6) . . ?
Ta3 O19 Ta6 162.8(6) . . ?
Ta3 O20 K1 103.6(4) . . ?
Se1 O20 Ta3 126.9(5) . . ?
Se1 O20 K1 122.1(5) . . ?
Se2 O21 Ta6 126.2(6) . . ?
Ta1 O22 Ta4 163.6(6) . . ?
Se2 O23 Ta5 130.6(6) . . ?
Se4 O24 Ta1 122.1(6) . . ?
Se1 O25 Ta1 130.7(6) . . ?
Ta2 O26 Ta5 169.3(6) . . ?
Se1 O27 Ta2 129.7(6) . . ?
Ta5 O28 Ta6 110.5(5) . . ?
Ta4 O29 Ta6 107.4(5) . . ?
Ta3 O30 Ta1 108.3(5) . . ?
Ta4 O31 Ta5 147.4(5) . . ?
Ta4 O31 Ta6 107.4(4) . . ?
Ta6 O31 Ta5 99.3(4) . . ?
Ta3 O32 Ta2 108.1(4) . . ?
Ta1 O33 Ta2 144.8(5) . . ?
Ta1 O33 Ta3 106.1(4) . . ?
Ta2 O33 Ta3 105.9(4) . . ?
Ho1 O2W Cs1 159.5(5) . 4_676 ?
Ho1 O4W Cs1 111.1(4) . 1_655 ?
K1 O8W Cs1 148.5(5) 1_556 . ?
Ho1 O9W Cs1 98.3(4) . 1_655 ?

_shelx_SHELXL_version_number     2018/1
_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy7_a
_database_code_depnum_ccdc_archive 'CCDC 1893232'
loop_
_audit_author_name
_audit_author_address
ddzhang
;Henan University
China
;
_audit_update_record             
;
2019-01-24 deposited with the CCDC.	2020-02-27 downloaded from the CCDC.
;
_audit_creation_date             2018-02-09
_audit_creation_method           
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs K O46 Se4 Ta6 Yb, 4(O)'
_chemical_formula_sum            'Cs K O50 Se4 Ta6 Yb'
_chemical_formula_weight         2546.59
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Yb Yb -0.3850 5.5486 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.2568(7)
_cell_length_b                   27.2994(16)
_cell_length_c                   13.9755(8)
_cell_angle_alpha                90
_cell_angle_beta                 114.1660(10)
_cell_angle_gamma                90
_cell_volume                     4266.4(4)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    4588
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.69
_cell_measurement_theta_min      2.19
_shelx_estimated_absorpt_T_max   0.162
_shelx_estimated_absorpt_T_min   0.103
_exptl_absorpt_coefficient_mu    21.976
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.3967
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1069 before and 0.0513 after correction.
The Ratio of minimum to maximum transmission is 0.5320.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.965
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4472
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.13
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0487
_diffrn_reflns_av_unetI/netI     0.0551
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            22043
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.492
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                6085
_reflns_number_total             7575
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         1.725
_refine_diff_density_min         -4.827
_refine_diff_density_rms         0.352
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.018
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7575
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0565
_refine_ls_R_factor_gt           0.0413
_refine_ls_restrained_S_all      1.018
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0388P)²+103.1844P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0921
_refine_ls_wR_factor_ref         0.0997
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28578(5) 0.54894(2) 0.55523(4) 0.01064(13) Uani 1 1 d . . . . .
Ta2 Ta 0.43791(5) 0.65822(2) 0.47020(4) 0.01076(13) Uani 1 1 d . . . . .
Ta3 Ta 0.17149(5) 0.60794(2) 0.32719(4) 0.01103(13) Uani 1 1 d . . . . .
Ta4 Ta 0.13594(5) 0.64092(2) 0.66367(4) 0.01104(13) Uani 1 1 d . . . . .
Ta5 Ta 0.28182(5) 0.75217(2) 0.57444(4) 0.01133(14) Uani 1 1 d . . . . .
Ta6 Ta 0.03066(5) 0.70168(2) 0.43685(4) 0.01263(14) Uani 1 1 d . . . . .
Yb1 Yb 0.68436(6) 0.64967(2) 0.98454(5) 0.01504(15) Uani 1 1 d . . . . .
Se1 Se 0.41855(13) 0.53770(5) 0.38123(11) 0.0154(3) Uani 1 1 d . . . . .
Se2 Se 0.04784(13) 0.76026(5) 0.65886(11) 0.0147(3) Uani 1 1 d . . . . .
Se3 Se 0.37819(12) 0.71178(5) 0.82817(11) 0.0128(3) Uani 1 1 d . . . . .
Se4 Se 0.49243(13) 0.62454(5) 0.71395(11) 0.0170(3) Uani 1 1 d . . . . .
Cs1 Cs -0.18115(14) 0.66363(6) 0.72115(14) 0.0671(4) Uani 1 1 d . . . . .
K1 K 0.2245(5) 0.57289(19) 0.0713(4) 0.0568(13) Uani 1 1 d . . . . .
O1 O 0.6197(9) 0.6144(4) 0.8171(8) 0.018(2) Uiso 1 1 d . . . . .
O2 O 0.3875(10) 0.8009(4) 0.5489(9) 0.032(3) Uiso 1 1 d . . . . .
O3 O -0.1398(10) 0.6939(4) 0.3398(9) 0.028(3) Uiso 1 1 d . . . . .
O4 O 0.5105(9) 0.6871(4) 0.8968(8) 0.020(2) Uiso 1 1 d . . . . .
O5 O 0.5036(9) 0.6928(4) 0.3824(8) 0.023(2) Uiso 1 1 d . . . . .
O6 O 0.5970(9) 0.6855(4) 0.4899(8) 0.022(2) Uiso 1 1 d . . . . .
O7 O -0.0816(9) 0.7375(4) 0.3144(8) 0.018(2) Uiso 1 1 d . . . . .
O8 O 0.0940(9) 0.6190(4) 0.1749(8) 0.023(2) Uiso 1 1 d . . . . .
O9 O 0.5474(9) 0.6377(4) 0.6211(8) 0.017(2) Uiso 1 1 d . . . . .
O10 O 0.1240(9) 0.6042(4) 0.7835(8) 0.019(2) Uiso 1 1 d . . . . .
O11 O 0.3157(10) 0.8222(4) 0.6005(9) 0.031(3) Uiso 1 1 d . . . . .
O12 O 0.0315(10) 0.5801(4) 0.2095(9) 0.027(3) Uiso 1 1 d . . . . .
O13 O 0.0683(9) 0.7028(4) 0.7085(8) 0.018(2) Uiso 1 1 d . . . . .
O14 O 0.0133(9) 0.5996(4) 0.6858(8) 0.020(2) Uiso 1 1 d . . . . .
O15 O 0.2964(9) 0.6594(4) 0.7834(8) 0.020(2) Uiso 1 1 d . . . . .
O16 O 0.2011(10) 0.4865(4) 0.5493(9) 0.027(3) Uiso 1 1 d . . . . .
O17 O 0.3997(8) 0.7290(3) 0.7189(7) 0.014(2) Uiso 1 1 d . . . . .
O18 O 0.3178(9) 0.4891(4) 0.6442(8) 0.023(2) Uiso 1 1 d . . . . .
O19 O 0.0873(9) 0.6583(3) 0.3620(7) 0.016(2) Uiso 1 1 d . . . . .
O20 O 0.2820(8) 0.5578(3) 0.2966(7) 0.014(2) Uiso 1 1 d . . . . .
O21 O -0.0287(9) 0.7489(3) 0.5291(7) 0.016(2) Uiso 1 1 d . . . . .
O22 O 0.2084(9) 0.5881(4) 0.6232(7) 0.016(2) Uiso 1 1 d . . . . .
O23 O 0.1864(9) 0.7757(4) 0.6670(8) 0.018(2) Uiso 1 1 d . . . . .
O24 O 0.4496(9) 0.5652(4) 0.6758(8) 0.019(2) Uiso 1 1 d . . . . .
O25 O 0.3840(8) 0.5173(3) 0.4808(7) 0.014(2) Uiso 1 1 d . . . . .
O26 O 0.3717(9) 0.7088(4) 0.5164(8) 0.018(2) Uiso 1 1 d . . . . .
O27 O 0.4961(9) 0.5905(3) 0.4282(7) 0.016(2) Uiso 1 1 d . . . . .
O28 O 0.1442(9) 0.7570(4) 0.4461(8) 0.017(2) Uiso 1 1 d . . . . .
O29 O -0.0080(9) 0.6451(4) 0.5174(8) 0.019(2) Uiso 1 1 d . . . . .
O30 O 0.1386(8) 0.5542(4) 0.4127(7) 0.016(2) Uiso 1 1 d . . . . .
O31 O 0.1804(8) 0.6904(3) 0.5741(7) 0.012(2) Uiso 1 1 d . . . . .
O32 O 0.2939(9) 0.6580(4) 0.3231(8) 0.017(2) Uiso 1 1 d . . . . .
O33 O 0.3098(8) 0.6097(3) 0.4785(7) 0.011(2) Uiso 1 1 d . . . . .
O1W O 0.5649(10) 0.6381(4) 1.0780(9) 0.030(3) Uiso 1 1 d . . . . .
O2W O 0.7025(10) 0.7257(4) 1.0797(9) 0.031(3) Uiso 1 1 d . . . . .
O3W O 0.8284(10) 0.6389(4) 1.1571(9) 0.033(3) Uiso 1 1 d . . . . .
O4W O 0.7563(11) 0.7088(4) 0.9065(10) 0.037(3) Uiso 1 1 d . . . . .
O5W O -0.0454(11) 0.4993(5) 0.3452(10) 0.039(3) Uiso 1 1 d . . . . .
O6W O 0.6302(11) 0.7675(5) 0.7511(10) 0.043(3) Uiso 1 1 d . . . . .
O7W O -0.2195(14) 0.6148(6) 0.4944(13) 0.065(4) Uiso 1 1 d . . . . .
O8W O 0.0508(12) 0.6445(5) 0.9267(11) 0.049(4) Uiso 1 1 d . . . . .
O9W O 0.8600(11) 0.6160(5) 0.9759(10) 0.042(3) Uiso 1 1 d . . . . .
O10W O 0.6736(11) 0.5667(5) 1.0051(10) 0.040(3) Uiso 1 1 d . . . . .
O11W O 0.5855(12) 0.4985(5) 0.8462(11) 0.050(4) Uiso 1 1 d . . . . .
O12W O 0.3635(13) 0.5815(5) -0.0535(12) 0.056(4) Uiso 1 1 d . . . . .
O13W O 0.0934(15) 0.5160(6) -0.1058(14) 0.072(5) Uiso 1 1 d . . . . .
O14W O 0.3537(14) 0.4911(6) 0.8536(12) 0.062(4) Uiso 1 1 d . . . . .
O15W O 0.594(2) 0.6116(9) 1.2728(18) 0.115(8) Uiso 1 1 d . . . . .
O16W O 0.274(2) 0.4422(10) 0.333(2) 0.141(9) Uiso 1 1 d . . . . .
O17W O 0.1416(19) 0.4694(8) 0.1279(17) 0.107(7) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3254(8) . ?
Ta1 O16 1.980(11) . ?
Ta1 O18 1.991(10) . ?
Ta1 O22 1.918(10) . ?
Ta1 O24 2.073(10) . ?
Ta1 O25 2.075(9) . ?
Ta1 O30 2.074(10) . ?
Ta1 O33 2.061(9) . ?
Ta2 Ta3 3.3463(8) . ?
Ta2 Cs1 4.5514(18) 1_655 ?
Ta2 O5 1.962(10) . ?
Ta2 O6 1.999(10) . ?
Ta2 O9 2.061(10) . ?
Ta2 O26 1.848(10) . ?
Ta2 O27 2.148(10) . ?
Ta2 O32 2.091(10) . ?
Ta2 O33 2.094(9) . ?
Ta3 K1 4.004(5) . ?
Ta3 O8 1.967(10) . ?
Ta3 O12 1.979(11) . ?
Ta3 O19 1.897(9) . ?
Ta3 O20 2.090(9) . ?
Ta3 O30 2.034(9) . ?
Ta3 O32 2.047(10) . ?
Ta3 O33 2.100(9) . ?
Ta4 Ta6 3.3341(8) . ?
Ta4 Cs1 4.3233(16) . ?
Ta4 O10 2.009(10) . ?
Ta4 O13 2.087(10) . ?
Ta4 O14 2.001(10) . ?
Ta4 O15 2.056(10) . ?
Ta4 O22 1.898(10) . ?
Ta4 O29 2.086(10) . ?
Ta4 O31 2.062(9) . ?
Ta5 Ta6 3.1981(8) . ?
Ta5 O2 1.988(12) . ?
Ta5 O11 1.958(12) . ?
Ta5 O17 2.043(9) . ?
Ta5 O23 2.166(10) . ?
Ta5 O26 2.000(10) . ?
Ta5 O28 1.898(10) . ?
Ta5 O31 2.093(9) . ?
Ta6 O3 1.983(11) . ?
Ta6 O7 1.963(10) . ?
Ta6 O19 1.891(9) . ?
Ta6 O21 2.150(9) . ?
Ta6 O28 2.022(10) . ?
Ta6 O29 2.076(10) . ?
Ta6 O31 2.064(9) . ?
Yb1 Se4 3.6085(16) . ?
Yb1 Cs1 4.6237(18) 1_655 ?
Yb1 O1 2.348(10) . ?
Yb1 O4 2.225(10) . ?
Yb1 O1W 2.348(11) . ?
Yb1 O2W 2.426(12) . ?
Yb1 O3W 2.352(12) . ?
Yb1 O4W 2.315(12) . ?
Yb1 O9W 2.389(13) . ?
Yb1 O10W 2.294(13) . ?
Se1 O20 1.697(9) . ?
Se1 O25 1.705(9) . ?
Se1 O27 1.703(10) . ?
Se2 Cs1 4.195(2) . ?
Se2 O13 1.692(10) . ?
Se2 O21 1.694(10) . ?
Se2 O23 1.709(10) . ?
Se3 O4 1.652(10) . ?
Se3 O15 1.712(10) . ?
Se3 O17 1.718(9) . ?
Se4 Cs1 4.102(2) 1_655 ?
Se4 O1 1.658(10) . ?
Se4 O9 1.727(10) . ?
Se4 O24 1.718(10) . ?
Cs1 O1 3.499(10) 1_455 ?
Cs1 O6 3.317(11) 1_455 ?
Cs1 O7 3.027(10) 4_576 ?
Cs1 O9 3.117(10) 1_455 ?
Cs1 O13 3.312(10) . ?
Cs1 O14 3.154(10) . ?
Cs1 O2W 3.573(12) 4_475 ?
Cs1 O4W 3.231(12) 1_455 ?
Cs1 O7W 3.290(16) . ?
Cs1 O8W 3.150(14) . ?
Cs1 O9W 3.626(13) 1_455 ?
Cs1 O16W 3.08(3) 3_566 ?
K1 O8 2.851(11) . ?
K1 O11 3.041(13) 4_575 ?
K1 O20 2.960(10) . ?
K1 O8W 2.986(15) 1_554 ?
K1 O11W 2.889(15) 3_666 ?
K1 O12W 2.904(15) . ?
K1 O13W 2.804(18) . ?
K1 O17W 3.21(2) . ?
O2 O11 1.466(15) . ?
O3 O7 1.505(14) . ?
O5 O6 1.482(14) . ?
O8 O12 1.501(14) . ?
O10 O14 1.484(14) . ?
O16 O18 1.502(15) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Ta1 Ta3 111.6(3) . . ?
O16 Ta1 O18 44.5(4) . . ?
O16 Ta1 O24 122.4(4) . . ?
O16 Ta1 O25 91.3(4) . . ?
O16 Ta1 O30 77.6(4) . . ?
O16 Ta1 O33 148.8(4) . . ?
O18 Ta1 Ta3 153.3(3) . . ?
O18 Ta1 O24 77.9(4) . . ?
O18 Ta1 O25 88.0(4) . . ?
O18 Ta1 O30 121.9(4) . . ?
O18 Ta1 O33 162.0(4) . . ?
O22 Ta1 Ta3 96.0(3) . . ?
O22 Ta1 O16 98.2(4) . . ?
O22 Ta1 O18 99.1(4) . . ?
O22 Ta1 O24 89.3(4) . . ?
O22 Ta1 O25 170.5(4) . . ?
O22 Ta1 O30 91.4(4) . . ?
O22 Ta1 O33 90.8(4) . . ?
O24 Ta1 Ta3 124.2(3) . . ?
O24 Ta1 O25 85.9(4) . . ?
O24 Ta1 O30 159.7(4) . . ?
O25 Ta1 Ta3 79.9(3) . . ?
O30 Ta1 Ta3 35.5(3) . . ?
O30 Ta1 O25 90.2(4) . . ?
O33 Ta1 Ta3 37.4(3) . . ?
O33 Ta1 O24 87.3(4) . . ?
O33 Ta1 O25 80.7(4) . . ?
O33 Ta1 O30 72.4(4) . . ?
Ta3 Ta2 Cs1 156.34(3) . 1_655 ?
O5 Ta2 Ta3 111.9(3) . . ?
O5 Ta2 Cs1 85.0(3) . 1_655 ?
O5 Ta2 O6 43.9(4) . . ?
O5 Ta2 O9 120.6(4) . . ?
O5 Ta2 O27 88.6(4) . . ?
O5 Ta2 O32 77.5(4) . . ?
O5 Ta2 O33 148.0(4) . . ?
O6 Ta2 Ta3 153.3(3) . . ?
O6 Ta2 Cs1 41.1(3) . 1_655 ?
O6 Ta2 O9 76.7(4) . . ?
O6 Ta2 O27 86.8(4) . . ?
O6 Ta2 O32 121.3(4) . . ?
O6 Ta2 O33 160.1(4) . . ?
O9 Ta2 Ta3 124.5(3) . . ?
O9 Ta2 Cs1 35.6(3) . 1_655 ?
O9 Ta2 O27 84.0(4) . . ?
O9 Ta2 O32 160.0(4) . . ?
O9 Ta2 O33 87.7(4) . . ?
O26 Ta2 Ta3 93.1(3) . . ?
O26 Ta2 Cs1 99.5(3) . 1_655 ?
O26 Ta2 O5 102.2(4) . . ?
O26 Ta2 O6 102.5(4) . . ?
O26 Ta2 O9 92.4(4) . . ?
O26 Ta2 O27 169.0(4) . . ?
O26 Ta2 O32 91.8(4) . . ?
O26 Ta2 O33 90.4(4) . . ?
O27 Ta2 Ta3 80.5(3) . . ?
O27 Ta2 Cs1 83.6(3) . 1_655 ?
O32 Ta2 Ta3 35.6(3) . . ?
O32 Ta2 Cs1 160.9(3) . 1_655 ?
O32 Ta2 O27 88.3(4) . . ?
O32 Ta2 O33 72.7(4) . . ?
O33 Ta2 Ta3 37.1(2) . . ?
O33 Ta2 Cs1 122.3(2) . 1_655 ?
O33 Ta2 O27 79.1(4) . . ?
Ta1 Ta3 Ta2 72.607(18) . . ?
Ta1 Ta3 K1 125.56(7) . . ?
Ta2 Ta3 K1 98.98(8) . . ?
O8 Ta3 Ta1 159.8(3) . . ?
O8 Ta3 Ta2 120.3(3) . . ?
O8 Ta3 K1 41.7(3) . . ?
O8 Ta3 O12 44.7(4) . . ?
O8 Ta3 O20 86.8(4) . . ?
O8 Ta3 O30 128.5(4) . . ?
O8 Ta3 O32 84.4(4) . . ?
O8 Ta3 O33 156.8(4) . . ?
O12 Ta3 Ta1 119.5(3) . . ?
O12 Ta3 Ta2 163.0(3) . . ?
O12 Ta3 K1 64.4(3) . . ?
O12 Ta3 O20 89.6(4) . . ?
O12 Ta3 O30 84.2(4) . . ?
O12 Ta3 O32 129.0(4) . . ?
O12 Ta3 O33 156.0(4) . . ?
O19 Ta3 Ta1 99.5(3) . . ?
O19 Ta3 Ta2 92.9(3) . . ?
O19 Ta3 K1 134.9(3) . . ?
O19 Ta3 O8 95.4(4) . . ?
O19 Ta3 O12 96.5(4) . . ?
O19 Ta3 O20 173.2(4) . . ?
O19 Ta3 O30 96.4(4) . . ?
O19 Ta3 O32 90.3(4) . . ?
O19 Ta3 O33 91.4(4) . . ?
O20 Ta3 Ta1 79.9(3) . . ?
O20 Ta3 Ta2 80.5(3) . . ?
O20 Ta3 K1 45.9(3) . . ?
O20 Ta3 O33 84.1(4) . . ?
O30 Ta3 Ta1 36.3(3) . . ?
O30 Ta3 Ta2 108.9(3) . . ?
O30 Ta3 K1 119.8(3) . . ?
O30 Ta3 O20 87.1(4) . . ?
O30 Ta3 O32 145.2(4) . . ?
O30 Ta3 O33 72.4(4) . . ?
O32 Ta3 Ta1 108.9(3) . . ?
O32 Ta3 Ta2 36.5(3) . . ?
O32 Ta3 K1 75.3(3) . . ?
O32 Ta3 O20 83.5(4) . . ?
O32 Ta3 O33 73.4(4) . . ?
O33 Ta3 Ta1 36.5(2) . . ?
O33 Ta3 Ta2 37.0(2) . . ?
O33 Ta3 K1 123.1(3) . . ?
Ta6 Ta4 Cs1 94.46(3) . . ?
O10 Ta4 Ta6 155.4(3) . . ?
O10 Ta4 Cs1 62.5(3) . . ?
O10 Ta4 O13 88.9(4) . . ?
O10 Ta4 O15 79.4(4) . . ?
O10 Ta4 O29 121.6(4) . . ?
O10 Ta4 O31 164.1(4) . . ?
O13 Ta4 Ta6 80.5(3) . . ?
O13 Ta4 Cs1 48.0(3) . . ?
O14 Ta4 Ta6 113.8(3) . . ?
O14 Ta4 Cs1 42.5(3) . . ?
O14 Ta4 O10 43.4(4) . . ?
O14 Ta4 O13 89.7(4) . . ?
O14 Ta4 O15 122.7(4) . . ?
O14 Ta4 O29 78.2(4) . . ?
O14 Ta4 O31 149.9(4) . . ?
O15 Ta4 Ta6 121.4(3) . . ?
O15 Ta4 Cs1 116.5(3) . . ?
O15 Ta4 O13 85.6(4) . . ?
O15 Ta4 O29 158.1(4) . . ?
O15 Ta4 O31 86.0(4) . . ?
O22 Ta4 Ta6 98.1(3) . . ?
O22 Ta4 Cs1 136.9(3) . . ?
O22 Ta4 O10 94.1(4) . . ?
O22 Ta4 O13 175.1(4) . . ?
O22 Ta4 O14 95.2(4) . . ?
O22 Ta4 O15 91.2(4) . . ?
O22 Ta4 O29 93.5(4) . . ?
O22 Ta4 O31 92.6(4) . . ?
O29 Ta4 Ta6 36.7(3) . . ?
O29 Ta4 Cs1 73.1(3) . . ?
O29 Ta4 O13 88.2(4) . . ?
O31 Ta4 Ta6 36.1(3) . . ?
O31 Ta4 Cs1 120.0(3) . . ?
O31 Ta4 O13 83.5(4) . . ?
O31 Ta4 O29 72.4(4) . . ?
O2 Ta5 Ta6 135.9(3) . . ?
O2 Ta5 O17 97.8(4) . . ?
O2 Ta5 O23 117.3(4) . . ?
O2 Ta5 O26 79.4(4) . . ?
O2 Ta5 O31 165.6(4) . . ?
O11 Ta5 Ta6 127.7(3) . . ?
O11 Ta5 O2 43.6(4) . . ?
O11 Ta5 O17 96.2(4) . . ?
O11 Ta5 O23 74.0(4) . . ?
O11 Ta5 O26 122.8(4) . . ?
O11 Ta5 O31 150.1(4) . . ?
O17 Ta5 Ta6 125.3(3) . . ?
O17 Ta5 O23 80.7(4) . . ?
O17 Ta5 O31 86.1(4) . . ?
O23 Ta5 Ta6 82.2(3) . . ?
O26 Ta5 Ta6 93.2(3) . . ?
O26 Ta5 O17 86.2(4) . . ?
O26 Ta5 O23 159.9(4) . . ?
O26 Ta5 O31 87.0(4) . . ?
O28 Ta5 Ta6 36.6(3) . . ?
O28 Ta5 O2 100.1(4) . . ?
O28 Ta5 O11 98.4(4) . . ?
O28 Ta5 O17 161.9(4) . . ?
O28 Ta5 O23 93.2(4) . . ?
O28 Ta5 O26 94.7(4) . . ?
O28 Ta5 O31 75.9(4) . . ?
O31 Ta5 Ta6 39.4(3) . . ?
O31 Ta5 O23 77.0(4) . . ?
Ta5 Ta6 Ta4 74.939(19) . . ?
O3 Ta6 Ta4 119.1(3) . . ?
O3 Ta6 Ta5 160.6(3) . . ?
O3 Ta6 O21 87.4(4) . . ?
O3 Ta6 O28 129.0(4) . . ?
O3 Ta6 O29 83.1(4) . . ?
O3 Ta6 O31 155.1(4) . . ?
O7 Ta6 Ta4 159.6(3) . . ?
O7 Ta6 Ta5 117.9(3) . . ?
O7 Ta6 O3 44.8(4) . . ?
O7 Ta6 O21 86.3(4) . . ?
O7 Ta6 O28 84.3(4) . . ?
O7 Ta6 O29 127.5(4) . . ?
O7 Ta6 O31 157.5(4) . . ?
O19 Ta6 Ta4 97.3(3) . . ?
O19 Ta6 Ta5 97.0(3) . . ?
O19 Ta6 O3 94.4(4) . . ?
O19 Ta6 O7 96.6(4) . . ?
O19 Ta6 O21 177.0(4) . . ?
O19 Ta6 O28 96.0(4) . . ?
O19 Ta6 O29 92.9(4) . . ?
O19 Ta6 O31 91.9(4) . . ?
O21 Ta6 Ta4 79.8(3) . . ?
O21 Ta6 Ta5 81.9(3) . . ?
O28 Ta6 Ta4 108.8(3) . . ?
O28 Ta6 Ta5 34.1(3) . . ?
O28 Ta6 O21 84.6(4) . . ?
O28 Ta6 O29 145.6(4) . . ?
O28 Ta6 O31 74.0(4) . . ?
O29 Ta6 Ta4 36.9(3) . . ?
O29 Ta6 Ta5 111.8(3) . . ?
O29 Ta6 O21 84.9(4) . . ?
O31 Ta6 Ta4 36.1(3) . . ?
O31 Ta6 Ta5 40.0(3) . . ?
O31 Ta6 O21 85.5(4) . . ?
O31 Ta6 O29 72.5(4) . . ?
Se4 Yb1 Cs1 58.22(3) . 1_655 ?
O1 Yb1 Se4 21.3(2) . . ?
O1 Yb1 Cs1 47.6(2) . 1_655 ?
O1 Yb1 O1W 117.8(4) . . ?
O1 Yb1 O2W 144.6(4) . . ?
O1 Yb1 O3W 140.9(4) . . ?
O1 Yb1 O9W 74.6(4) . . ?
O4 Yb1 Se4 56.2(3) . . ?
O4 Yb1 Cs1 95.6(3) . 1_655 ?
O4 Yb1 O1 77.5(4) . . ?
O4 Yb1 O1W 72.1(4) . . ?
O4 Yb1 O2W 76.2(4) . . ?
O4 Yb1 O3W 140.4(4) . . ?
O4 Yb1 O4W 83.3(4) . . ?
O4 Yb1 O9W 146.0(4) . . ?
O4 Yb1 O10W 115.6(4) . . ?
O1W Yb1 Se4 105.6(3) . . ?
O1W Yb1 Cs1 163.8(3) . 1_655 ?
O1W Yb1 O2W 75.4(4) . . ?
O1W Yb1 O3W 77.9(4) . . ?
O1W Yb1 O9W 139.2(4) . . ?
O2W Yb1 Se4 127.7(3) . . ?
O2W Yb1 Cs1 112.6(3) . 1_655 ?
O3W Yb1 Se4 160.8(3) . . ?
O3W Yb1 Cs1 117.6(3) . 1_655 ?
O3W Yb1 O2W 71.5(4) . . ?
O3W Yb1 O9W 71.9(4) . . ?
O4W Yb1 Se4 81.3(3) . . ?
O4W Yb1 Cs1 40.4(3) . 1_655 ?
O4W Yb1 O1 81.6(4) . . ?
O4W Yb1 O1W 143.1(4) . . ?
O4W Yb1 O2W 72.2(4) . . ?
O4W Yb1 O3W 107.4(4) . . ?
O4W Yb1 O9W 73.7(4) . . ?
O9W Yb1 Se4 95.0(3) . . ?
O9W Yb1 Cs1 50.9(3) . 1_655 ?
O9W Yb1 O2W 118.4(4) . . ?
O10W Yb1 Se4 84.1(3) . . ?
O10W Yb1 Cs1 103.8(3) . 1_655 ?
O10W Yb1 O1 72.9(4) . . ?
O10W Yb1 O1W 73.6(4) . . ?
O10W Yb1 O2W 140.6(4) . . ?
O10W Yb1 O3W 78.8(4) . . ?
O10W Yb1 O4W 143.1(4) . . ?
O10W Yb1 O9W 74.1(4) . . ?
O20 Se1 O25 99.9(4) . . ?
O20 Se1 O27 103.3(5) . . ?
O27 Se1 O25 104.3(5) . . ?
O13 Se2 Cs1 48.1(3) . . ?
O13 Se2 O21 101.1(5) . . ?
O13 Se2 O23 103.0(5) . . ?
O21 Se2 Cs1 89.0(3) . . ?
O21 Se2 O23 102.5(5) . . ?
O23 Se2 Cs1 150.8(3) . . ?
O4 Se3 O15 99.2(5) . . ?
O4 Se3 O17 99.0(5) . . ?
O15 Se3 O17 100.6(5) . . ?
Yb1 Se4 Cs1 73.38(4) . 1_655 ?
O1 Se4 Yb1 31.0(3) . . ?
O1 Se4 Cs1 57.4(3) . 1_655 ?
O1 Se4 O9 99.8(5) . . ?
O1 Se4 O24 99.9(5) . . ?
O9 Se4 Yb1 117.4(3) . . ?
O9 Se4 Cs1 44.6(3) . 1_655 ?
O24 Se4 Yb1 119.3(3) . . ?
O24 Se4 Cs1 115.1(3) . 1_655 ?
O24 Se4 O9 97.2(5) . . ?
O1 Cs1 O2W 110.7(2) 1_455 4_475 ?
O1 Cs1 O9W 47.5(3) 1_455 1_455 ?
O6 Cs1 O1 91.2(2) 1_455 1_455 ?
O6 Cs1 O2W 47.6(3) 1_455 4_475 ?
O6 Cs1 O9W 138.6(3) 1_455 1_455 ?
O7 Cs1 O1 113.5(2) 4_576 1_455 ?
O7 Cs1 O6 106.5(3) 4_576 1_455 ?
O7 Cs1 O9 124.3(3) 4_576 1_455 ?
O7 Cs1 O13 61.1(3) 4_576 . ?
O7 Cs1 O14 111.4(3) 4_576 . ?
O7 Cs1 O2W 58.9(3) 4_576 4_475 ?
O7 Cs1 O4W 60.1(3) 4_576 1_455 ?
O7 Cs1 O7W 130.5(3) 4_576 . ?
O7 Cs1 O8W 72.6(3) 4_576 . ?
O7 Cs1 O9W 91.6(3) 4_576 1_455 ?
O7 Cs1 O16W 169.7(5) 4_576 3_566 ?
O9 Cs1 O1 45.6(2) 1_455 1_455 ?
O9 Cs1 O6 46.0(3) 1_455 1_455 ?
O9 Cs1 O13 152.7(3) 1_455 . ?
O9 Cs1 O14 122.7(3) 1_455 . ?
O9 Cs1 O2W 80.4(3) 1_455 4_475 ?
O9 Cs1 O4W 83.5(3) 1_455 1_455 ?
O9 Cs1 O7W 76.7(3) 1_455 . ?
O9 Cs1 O8W 140.4(3) 1_455 . ?
O9 Cs1 O9W 93.0(3) 1_455 1_455 ?
O13 Cs1 O1 161.6(2) . 1_455 ?
O13 Cs1 O6 107.2(3) . 1_455 ?
O13 Cs1 O2W 82.3(3) . 4_475 ?
O13 Cs1 O9W 114.1(3) . 1_455 ?
O14 Cs1 O1 122.5(2) . 1_455 ?
O14 Cs1 O6 108.5(3) . 1_455 ?
O14 Cs1 O13 52.9(3) . . ?
O14 Cs1 O2W 122.6(3) . 4_475 ?
O14 Cs1 O4W 141.2(3) . 1_455 ?
O14 Cs1 O7W 56.2(3) . . ?
O14 Cs1 O9W 98.3(3) . 1_455 ?
O2W Cs1 O9W 135.2(3) 4_475 1_455 ?
O4W Cs1 O1 53.7(3) 1_455 1_455 ?
O4W Cs1 O6 110.1(3) 1_455 1_455 ?
O4W Cs1 O13 116.6(3) 1_455 . ?
O4W Cs1 O2W 87.1(3) 1_455 4_475 ?
O4W Cs1 O7W 160.0(4) 1_455 . ?
O4W Cs1 O9W 48.2(3) 1_455 1_455 ?
O7W Cs1 O1 111.5(3) . 1_455 ?
O7W Cs1 O6 52.9(3) . 1_455 ?
O7W Cs1 O13 81.4(3) . . ?
O7W Cs1 O2W 86.7(3) . 4_475 ?
O7W Cs1 O9W 135.1(4) . 1_455 ?
O8W Cs1 O1 95.6(3) . 1_455 ?
O8W Cs1 O6 172.9(3) . 1_455 ?
O8W Cs1 O13 66.0(3) . . ?
O8W Cs1 O14 66.0(3) . . ?
O8W Cs1 O2W 130.7(3) . 4_475 ?
O8W Cs1 O4W 75.8(3) . 1_455 ?
O8W Cs1 O7W 122.1(4) . . ?
O8W Cs1 O9W 48.3(3) . 1_455 ?
O16W Cs1 O1 59.2(5) 3_566 1_455 ?
O16W Cs1 O6 81.7(5) 3_566 1_455 ?
O16W Cs1 O9 57.1(5) 3_566 1_455 ?
O16W Cs1 O13 123.1(5) 3_566 . ?
O16W Cs1 O14 70.8(5) 3_566 . ?
O16W Cs1 O2W 129.2(5) 3_566 4_475 ?
O16W Cs1 O4W 111.6(5) 3_566 1_455 ?
O16W Cs1 O7W 59.5(6) 3_566 . ?
O16W Cs1 O8W 100.0(6) 3_566 . ?
O16W Cs1 O9W 78.1(5) 3_566 1_455 ?
O8 K1 Ta3 27.3(2) . . ?
O8 K1 O11 76.6(3) . 4_575 ?
O8 K1 O20 57.4(3) . . ?
O8 K1 O8W 70.2(4) . 1_554 ?
O8 K1 O11W 128.5(4) . 3_666 ?
O8 K1 O12W 149.1(4) . . ?
O8 K1 O17W 87.9(5) . . ?
O11 K1 Ta3 80.8(2) 4_575 . ?
O11 K1 O17W 158.8(5) 4_575 . ?
O20 K1 Ta3 30.50(18) . . ?
O20 K1 O11 94.2(3) . 4_575 ?
O20 K1 O8W 127.2(4) . 1_554 ?
O20 K1 O17W 65.0(4) . . ?
O8W K1 Ta3 96.7(3) 1_554 . ?
O8W K1 O11 66.1(4) 1_554 4_575 ?
O8W K1 O17W 122.2(5) 1_554 . ?
O11W K1 Ta3 101.8(3) 3_666 . ?
O11W K1 O11 112.9(4) 3_666 4_575 ?
O11W K1 O20 71.3(3) 3_666 . ?
O11W K1 O8W 161.1(4) 3_666 1_554 ?
O11W K1 O12W 73.7(4) 3_666 . ?
O11W K1 O17W 66.0(5) 3_666 . ?
O12W K1 Ta3 150.1(3) . . ?
O12W K1 O11 74.3(4) . 4_575 ?
O12W K1 O20 135.0(4) . . ?
O12W K1 O8W 88.4(4) . 1_554 ?
O12W K1 O17W 122.8(5) . . ?
O13W K1 Ta3 132.6(4) . . ?
O13W K1 O8 117.0(4) . . ?
O13W K1 O11 133.3(4) . 4_575 ?
O13W K1 O20 131.5(4) . . ?
O13W K1 O8W 76.9(5) . 1_554 ?
O13W K1 O11W 93.2(5) . 3_666 ?
O13W K1 O12W 77.3(5) . . ?
O13W K1 O17W 66.7(5) . . ?
O17W K1 Ta3 78.9(4) . . ?
Yb1 O1 Cs1 102.7(3) . 1_655 ?
Se4 O1 Yb1 127.7(5) . . ?
Se4 O1 Cs1 99.1(4) . 1_655 ?
O11 O2 Ta5 67.1(6) . . ?
O7 O3 Ta6 66.9(6) . . ?
Se3 O4 Yb1 176.6(6) . . ?
O6 O5 Ta2 69.3(6) . . ?
Ta2 O6 Cs1 115.6(4) . 1_655 ?
O5 O6 Ta2 66.7(6) . . ?
O5 O6 Cs1 175.1(7) . 1_655 ?
Ta6 O7 Cs1 146.6(5) . 4_575 ?
O3 O7 Ta6 68.3(6) . . ?
O3 O7 Cs1 131.4(6) . 4_575 ?
Ta3 O8 K1 111.0(4) . . ?
O12 O8 Ta3 68.0(6) . . ?
O12 O8 K1 108.6(7) . . ?
Ta2 O9 Cs1 121.7(4) . 1_655 ?
Se4 O9 Ta2 122.3(5) . . ?
Se4 O9 Cs1 112.5(4) . 1_655 ?
O14 O10 Ta4 68.0(5) . . ?
Ta5 O11 K1 148.9(5) . 4_576 ?
O2 O11 Ta5 69.3(6) . . ?
O2 O11 K1 124.6(8) . 4_576 ?
O8 O12 Ta3 67.2(6) . . ?
Ta4 O13 Cs1 104.1(4) . . ?
Se2 O13 Ta4 129.7(5) . . ?
Se2 O13 Cs1 109.6(4) . . ?
Ta4 O14 Cs1 112.1(4) . . ?
O10 O14 Ta4 68.5(5) . . ?
O10 O14 Cs1 105.9(6) . . ?
Se3 O15 Ta4 136.4(6) . . ?
O18 O16 Ta1 68.2(6) . . ?
Se3 O17 Ta5 131.2(5) . . ?
O16 O18 Ta1 67.4(6) . . ?
Ta6 O19 Ta3 163.2(6) . . ?
Ta3 O20 K1 103.6(4) . . ?
Se1 O20 Ta3 127.3(5) . . ?
Se1 O20 K1 121.6(4) . . ?
Se2 O21 Ta6 125.2(5) . . ?
Ta4 O22 Ta1 163.2(6) . . ?
Se2 O23 Ta5 130.7(5) . . ?
Se4 O24 Ta1 121.7(5) . . ?
Se1 O25 Ta1 131.5(5) . . ?
Ta2 O26 Ta5 167.8(6) . . ?
Se1 O27 Ta2 129.7(5) . . ?
Ta5 O28 Ta6 109.3(5) . . ?
Ta6 O29 Ta4 106.4(4) . . ?
Ta3 O30 Ta1 108.1(4) . . ?
Ta4 O31 Ta5 146.2(5) . . ?
Ta4 O31 Ta6 107.8(4) . . ?
Ta6 O31 Ta5 100.6(4) . . ?
Ta3 O32 Ta2 107.9(4) . . ?
Ta1 O33 Ta2 143.9(5) . . ?
Ta1 O33 Ta3 106.1(4) . . ?
Ta2 O33 Ta3 105.9(4) . . ?
Yb1 O2W Cs1 162.4(4) . 4_676 ?
Yb1 O4W Cs1 111.9(4) . 1_655 ?
K1 O8W Cs1 148.5(5) 1_556 . ?
Yb1 O9W Cs1 98.4(4) . 1_655 ?

_shelx_SHELXL_version_number     2018/1
_olex2_submission_special_instructions 'No special instructions were received'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_njy6_a
_database_code_depnum_ccdc_archive 'CCDC 1893231'
loop_
_audit_author_name
_audit_author_address
ddzhang
;Henan University
China
;
_audit_update_record             
;
2019-01-24 deposited with the CCDC.	2020-02-27 downloaded from the CCDC.
;
_audit_creation_date             2018-02-09
_audit_creation_method           
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Cs K O46 Se4 Ta6 Tm, 4(O)'
_chemical_formula_sum            'Cs K O50 Se4 Ta6 Tm'
_chemical_formula_weight         2542.48
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Se Se -0.0929 2.2259 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tm Tm -0.3139 5.2483 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.268(2)
_cell_length_b                   27.321(5)
_cell_length_c                   13.983(2)
_cell_angle_alpha                90
_cell_angle_beta                 114.134(3)
_cell_angle_gamma                90
_cell_volume                     4276.8(12)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    3140
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.59
_cell_measurement_theta_min      2.35
_shelx_estimated_absorpt_T_max   0.164
_shelx_estimated_absorpt_T_min   0.111
_exptl_absorpt_coefficient_mu    21.810
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.4781
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1239 before and 0.0558 after correction.
The Ratio of minimum to maximum transmission is 0.6411.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    3.949
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             4468
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.13
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0616
_diffrn_reflns_av_unetI/netI     0.0718
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -31
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            22102
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.099
_diffrn_reflns_theta_max         25.099
_diffrn_reflns_theta_min         1.761
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_diffrn_standards_number         0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                5666
_reflns_number_total             7591
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max         2.932
_refine_diff_density_min         -4.855
_refine_diff_density_rms         0.397
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.029
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     318
_refine_ls_number_reflns         7591
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0697
_refine_ls_R_factor_gt           0.0465
_refine_ls_restrained_S_all      1.029
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0428P)²+92.1278P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1030
_refine_ls_wR_factor_ref         0.1141
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ta1 Ta 0.28565(6) 0.54896(2) 0.55513(5) 0.01158(16) Uani 1 1 d . . . . .
Ta2 Ta 0.43773(6) 0.65822(2) 0.46999(5) 0.01159(16) Uani 1 1 d . . . . .
Ta3 Ta 0.17136(6) 0.60789(2) 0.32712(5) 0.01194(16) Uani 1 1 d . . . . .
Ta4 Ta 0.13584(6) 0.64088(2) 0.66356(5) 0.01195(16) Uani 1 1 d . . . . .
Ta5 Ta 0.28166(6) 0.75212(2) 0.57422(5) 0.01218(16) Uani 1 1 d . . . . .
Ta6 Ta 0.03035(6) 0.70159(3) 0.43661(5) 0.01377(17) Uani 1 1 d . . . . .
Tm1 Tm 0.68439(7) 0.64965(3) 0.98454(6) 0.01625(18) Uani 1 1 d . . . . .
Se1 Se 0.41818(15) 0.53769(6) 0.38107(13) 0.0154(4) Uani 1 1 d . . . . .
Se2 Se 0.04773(15) 0.76030(6) 0.65820(13) 0.0167(4) Uani 1 1 d . . . . .
Se3 Se 0.37765(15) 0.71184(6) 0.82767(12) 0.0140(4) Uani 1 1 d . . . . .
Se4 Se 0.49224(16) 0.62443(6) 0.71364(13) 0.0186(4) Uani 1 1 d . . . . .
Cs1 Cs -0.18181(18) 0.66364(8) 0.72045(17) 0.0749(6) Uani 1 1 d . . . . .
K1 K 0.2258(6) 0.5732(2) 0.0714(5) 0.0616(17) Uani 1 1 d . . . . .
O1 O 0.6193(11) 0.6146(4) 0.8182(9) 0.024(3) Uiso 1 1 d . . . . .
O2 O 0.3862(13) 0.8007(5) 0.5493(11) 0.040(4) Uiso 1 1 d . . . . .
O3 O -0.1410(12) 0.6934(5) 0.3384(10) 0.029(3) Uiso 1 1 d . . . . .
O4 O 0.5117(10) 0.6869(4) 0.8960(9) 0.019(3) Uiso 1 1 d . . . . .
O5 O 0.5029(10) 0.6922(4) 0.3815(9) 0.018(3) Uiso 1 1 d . . . . .
O6 O 0.5954(11) 0.6850(4) 0.4887(9) 0.024(3) Uiso 1 1 d . . . . .
O7 O -0.0818(11) 0.7376(4) 0.3139(9) 0.025(3) Uiso 1 1 d . . . . .
O8 O 0.0944(11) 0.6189(4) 0.1745(9) 0.022(3) Uiso 1 1 d . . . . .
O9 O 0.5468(10) 0.6388(4) 0.6210(9) 0.019(3) Uiso 1 1 d . . . . .
O10 O 0.1247(11) 0.6051(4) 0.7822(9) 0.021(3) Uiso 1 1 d . . . . .
O11 O 0.3152(13) 0.8221(5) 0.6027(11) 0.039(4) Uiso 1 1 d . . . . .
O12 O 0.0312(11) 0.5800(4) 0.2092(9) 0.024(3) Uiso 1 1 d . . . . .
O13 O 0.0687(11) 0.7030(4) 0.7073(9) 0.020(3) Uiso 1 1 d . . . . .
O14 O 0.0139(11) 0.5998(4) 0.6841(9) 0.022(3) Uiso 1 1 d . . . . .
O15 O 0.2952(11) 0.6597(4) 0.7824(9) 0.021(3) Uiso 1 1 d . . . . .
O16 O 0.1989(11) 0.4872(4) 0.5503(10) 0.026(3) Uiso 1 1 d . . . . .
O17 O 0.3983(10) 0.7286(4) 0.7174(8) 0.015(2) Uiso 1 1 d . . . . .
O18 O 0.3180(11) 0.4897(4) 0.6447(9) 0.022(3) Uiso 1 1 d . . . . .
O19 O 0.0870(10) 0.6575(4) 0.3615(9) 0.019(3) Uiso 1 1 d . . . . .
O20 O 0.2808(10) 0.5577(4) 0.2950(9) 0.016(3) Uiso 1 1 d . . . . .
O21 O -0.0271(10) 0.7489(4) 0.5291(8) 0.015(3) Uiso 1 1 d . . . . .
O22 O 0.2085(10) 0.5873(4) 0.6218(8) 0.015(2) Uiso 1 1 d . . . . .
O23 O 0.1861(11) 0.7762(4) 0.6659(9) 0.020(3) Uiso 1 1 d . . . . .
O24 O 0.4490(10) 0.5652(4) 0.6761(9) 0.016(3) Uiso 1 1 d . . . . .
O25 O 0.3829(10) 0.5173(4) 0.4811(8) 0.014(2) Uiso 1 1 d . . . . .
O26 O 0.3726(10) 0.7084(4) 0.5163(9) 0.019(3) Uiso 1 1 d . . . . .
O27 O 0.4941(10) 0.5905(4) 0.4265(9) 0.017(3) Uiso 1 1 d . . . . .
O28 O 0.1434(10) 0.7567(4) 0.4452(9) 0.019(3) Uiso 1 1 d . . . . .
O29 O -0.0070(10) 0.6453(4) 0.5203(9) 0.017(3) Uiso 1 1 d . . . . .
O30 O 0.1391(10) 0.5540(4) 0.4143(9) 0.017(3) Uiso 1 1 d . . . . .
O31 O 0.1791(10) 0.6899(4) 0.5746(8) 0.016(3) Uiso 1 1 d . . . . .
O32 O 0.2932(10) 0.6580(4) 0.3224(9) 0.018(3) Uiso 1 1 d . . . . .
O33 O 0.3090(9) 0.6092(4) 0.4775(8) 0.010(2) Uiso 1 1 d . . . . .
O1W O 0.5645(13) 0.6380(5) 1.0783(11) 0.036(3) Uiso 1 1 d . . . . .
O2W O 0.7039(13) 0.7260(5) 1.0799(11) 0.042(4) Uiso 1 1 d . . . . .
O3W O 0.8265(12) 0.6388(5) 1.1577(10) 0.030(3) Uiso 1 1 d . . . . .
O4W O 0.7570(13) 0.7086(5) 0.9066(11) 0.041(4) Uiso 1 1 d . . . . .
O5W O -0.0455(13) 0.4989(5) 0.3461(11) 0.038(4) Uiso 1 1 d . . . . .
O6W O 0.6286(14) 0.7672(5) 0.7504(12) 0.045(4) Uiso 1 1 d . . . . .
O7W O -0.2186(16) 0.6137(6) 0.4956(14) 0.062(5) Uiso 1 1 d . . . . .
O8W O 0.0471(15) 0.6455(6) 0.9232(13) 0.056(5) Uiso 1 1 d . . . . .
O9W O 0.8598(14) 0.6158(6) 0.9763(12) 0.047(4) Uiso 1 1 d . . . . .
O10W O 0.6741(13) 0.5661(5) 1.0072(11) 0.042(4) Uiso 1 1 d . . . . .
O11W O 0.5823(14) 0.4980(6) 0.8442(12) 0.050(4) Uiso 1 1 d . . . . .
O12W O 0.3639(14) 0.5814(6) -0.0556(12) 0.050(4) Uiso 1 1 d . . . . .
O13W O 0.0935(19) 0.5166(7) -0.1039(16) 0.080(6) Uiso 1 1 d . . . . .
O14W O 0.3556(16) 0.4920(7) 0.8536(14) 0.065(5) Uiso 1 1 d . . . . .
O15W O 0.594(2) 0.6114(9) 1.2724(19) 0.103(8) Uiso 1 1 d . . . . .
O16W O 0.267(3) 0.4410(12) 0.329(2) 0.157(12) Uiso 1 1 d . . . . .
O17W O 0.140(2) 0.4711(10) 0.127(2) 0.119(9) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ta1 Ta3 3.3267(10) . ?
Ta1 O16 1.982(12) . ?
Ta1 O18 1.985(12) . ?
Ta1 O22 1.894(11) . ?
Ta1 O24 2.074(11) . ?
Ta1 O25 2.063(11) . ?
Ta1 O30 2.058(11) . ?
Ta1 O33 2.054(10) . ?
Ta2 Ta3 3.3499(10) . ?
Ta2 Cs1 4.550(2) 1_655 ?
Ta2 O5 1.960(11) . ?
Ta2 O6 1.983(12) . ?
Ta2 O9 2.054(12) . ?
Ta2 O26 1.833(11) . ?
Ta2 O27 2.149(11) . ?
Ta2 O32 2.101(12) . ?
Ta2 O33 2.106(10) . ?
Ta3 K1 4.009(6) . ?
Ta3 O8 1.972(12) . ?
Ta3 O12 1.984(12) . ?
Ta3 O19 1.883(11) . ?
Ta3 O20 2.092(11) . ?
Ta3 O30 2.050(11) . ?
Ta3 O32 2.048(11) . ?
Ta3 O33 2.091(10) . ?
Ta4 Ta6 3.3373(10) . ?
Ta4 Cs1 4.329(2) . ?
Ta4 O10 1.978(11) . ?
Ta4 O13 2.083(11) . ?
Ta4 O14 1.982(12) . ?
Ta4 O15 2.047(12) . ?
Ta4 O22 1.924(11) . ?
Ta4 O29 2.055(11) . ?
Ta4 O31 2.039(11) . ?
Ta5 Ta6 3.2034(11) . ?
Ta5 O2 1.972(14) . ?
Ta5 O11 1.963(14) . ?
Ta5 O17 2.031(11) . ?
Ta5 O23 2.163(11) . ?
Ta5 O26 2.016(11) . ?
Ta5 O28 1.910(12) . ?
Ta5 O31 2.117(11) . ?
Ta6 O3 1.999(13) . ?
Ta6 O7 1.969(12) . ?
Ta6 O19 1.906(11) . ?
Ta6 O21 2.141(11) . ?
Ta6 O28 2.017(12) . ?
Ta6 O29 2.094(11) . ?
Ta6 O31 2.068(11) . ?
Tm1 Cs1 4.630(2) 1_655 ?
Tm1 O1 2.333(12) . ?
Tm1 O4 2.217(12) . ?
Tm1 O1W 2.358(14) . ?
Tm1 O2W 2.434(15) . ?
Tm1 O3W 2.353(13) . ?
Tm1 O4W 2.316(14) . ?
Tm1 O9W 2.388(16) . ?
Tm1 O10W 2.316(15) . ?
Se1 O20 1.711(11) . ?
Se1 O25 1.718(11) . ?
Se1 O27 1.693(11) . ?
Se2 Cs1 4.203(3) . ?
Se2 O13 1.687(12) . ?
Se2 O21 1.687(11) . ?
Se2 O23 1.713(12) . ?
Se3 O4 1.672(12) . ?
Se3 O15 1.712(12) . ?
Se3 O17 1.723(11) . ?
Se4 Cs1 4.103(3) 1_655 ?
Se4 O1 1.666(13) . ?
Se4 O9 1.728(11) . ?
Se4 O24 1.717(11) . ?
Cs1 O1 3.513(12) 1_455 ?
Cs1 O6 3.328(12) 1_455 ?
Cs1 O7 3.030(12) 4_576 ?
Cs1 O9 3.114(12) 1_455 ?
Cs1 O13 3.331(12) . ?
Cs1 O14 3.172(12) . ?
Cs1 O2W 3.559(15) 4_475 ?
Cs1 O4W 3.232(14) 1_455 ?
Cs1 O7W 3.286(18) . ?
Cs1 O8W 3.108(17) . ?
Cs1 O9W 3.643(15) 1_455 ?
Cs1 O16W 3.03(3) 3_566 ?
K1 O8 2.851(13) . ?
K1 O11 3.029(16) 4_575 ?
K1 O20 2.947(12) . ?
K1 O8W 3.047(18) 1_554 ?
K1 O11W 2.907(17) 3_666 ?
K1 O12W 2.922(17) . ?
K1 O13W 2.79(2) . ?
K1 O17W 3.19(3) . ?
O2 O11 1.480(19) . ?
O3 O7 1.519(17) . ?
O5 O6 1.476(16) . ?
O8 O12 1.506(16) . ?
O10 O14 1.491(16) . ?
O16 O18 1.518(17) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O16 Ta1 Ta3 111.7(4) . . ?
O16 Ta1 O18 45.0(5) . . ?
O16 Ta1 O24 122.4(5) . . ?
O16 Ta1 O25 92.2(5) . . ?
O16 Ta1 O30 77.2(5) . . ?
O16 Ta1 O33 148.6(5) . . ?
O18 Ta1 Ta3 153.7(3) . . ?
O18 Ta1 O24 77.4(5) . . ?
O18 Ta1 O25 88.1(4) . . ?
O18 Ta1 O30 122.0(5) . . ?
O18 Ta1 O33 162.0(5) . . ?
O22 Ta1 Ta3 96.0(3) . . ?
O22 Ta1 O16 96.8(5) . . ?
O22 Ta1 O18 98.8(5) . . ?
O22 Ta1 O24 89.5(5) . . ?
O22 Ta1 O25 171.0(5) . . ?
O22 Ta1 O30 91.0(5) . . ?
O22 Ta1 O33 91.3(4) . . ?
O24 Ta1 Ta3 124.5(3) . . ?
O25 Ta1 Ta3 80.0(3) . . ?
O25 Ta1 O24 86.2(4) . . ?
O30 Ta1 Ta3 35.9(3) . . ?
O30 Ta1 O24 160.2(4) . . ?
O30 Ta1 O25 90.4(4) . . ?
O33 Ta1 Ta3 37.0(3) . . ?
O33 Ta1 O24 87.9(4) . . ?
O33 Ta1 O25 80.6(4) . . ?
O33 Ta1 O30 72.4(4) . . ?
Ta3 Ta2 Cs1 156.33(4) . 1_655 ?
O5 Ta2 Ta3 111.6(3) . . ?
O5 Ta2 Cs1 85.2(3) . 1_655 ?
O5 Ta2 O6 44.0(5) . . ?
O5 Ta2 O9 120.6(5) . . ?
O5 Ta2 O27 88.2(4) . . ?
O5 Ta2 O32 77.3(5) . . ?
O5 Ta2 O33 147.2(4) . . ?
O6 Ta2 Ta3 153.0(3) . . ?
O6 Ta2 Cs1 41.3(3) . 1_655 ?
O6 Ta2 O9 76.7(5) . . ?
O6 Ta2 O27 86.9(5) . . ?
O6 Ta2 O32 121.1(5) . . ?
O6 Ta2 O33 159.9(5) . . ?
O9 Ta2 Ta3 125.0(3) . . ?
O9 Ta2 Cs1 35.4(3) . 1_655 ?
O9 Ta2 O27 85.4(4) . . ?
O9 Ta2 O32 160.5(4) . . ?
O9 Ta2 O33 88.3(4) . . ?
O26 Ta2 Ta3 93.3(4) . . ?
O26 Ta2 Cs1 99.3(4) . 1_655 ?
O26 Ta2 O5 102.6(5) . . ?
O26 Ta2 O6 102.7(5) . . ?
O26 Ta2 O9 91.4(5) . . ?
O26 Ta2 O27 168.9(5) . . ?
O26 Ta2 O32 92.0(5) . . ?
O26 Ta2 O33 90.8(5) . . ?
O27 Ta2 Ta3 80.0(3) . . ?
O27 Ta2 Cs1 84.2(3) . 1_655 ?
O32 Ta2 Ta3 35.6(3) . . ?
O32 Ta2 Cs1 160.8(3) . 1_655 ?
O32 Ta2 O27 87.7(4) . . ?
O32 Ta2 O33 72.5(4) . . ?
O33 Ta2 Ta3 36.9(3) . . ?
O33 Ta2 Cs1 122.4(3) . 1_655 ?
O33 Ta2 O27 78.5(4) . . ?
Ta1 Ta3 Ta2 72.60(2) . . ?
Ta1 Ta3 K1 125.57(8) . . ?
Ta2 Ta3 K1 98.69(10) . . ?
O8 Ta3 Ta1 159.8(3) . . ?
O8 Ta3 Ta2 120.1(3) . . ?
O8 Ta3 K1 41.5(4) . . ?
O8 Ta3 O12 44.7(5) . . ?
O8 Ta3 O20 86.1(5) . . ?
O8 Ta3 O30 129.0(5) . . ?
O8 Ta3 O32 84.0(5) . . ?
O8 Ta3 O33 156.7(4) . . ?
O12 Ta3 Ta1 119.6(3) . . ?
O12 Ta3 Ta2 162.9(3) . . ?
O12 Ta3 K1 64.7(4) . . ?
O12 Ta3 O20 89.1(5) . . ?
O12 Ta3 O30 84.6(5) . . ?
O12 Ta3 O32 128.7(5) . . ?
O12 Ta3 O33 155.7(4) . . ?
O19 Ta3 Ta1 99.4(3) . . ?
O19 Ta3 Ta2 93.2(4) . . ?
O19 Ta3 K1 135.0(4) . . ?
O19 Ta3 O8 95.6(5) . . ?
O19 Ta3 O12 96.2(5) . . ?
O19 Ta3 O20 173.9(5) . . ?
O19 Ta3 O30 96.0(5) . . ?
O19 Ta3 O32 90.6(5) . . ?
O19 Ta3 O33 91.9(4) . . ?
O20 Ta3 Ta1 80.4(3) . . ?
O20 Ta3 Ta2 80.9(3) . . ?
O20 Ta3 K1 45.4(3) . . ?
O30 Ta3 Ta1 36.0(3) . . ?
O30 Ta3 Ta2 108.6(3) . . ?
O30 Ta3 K1 120.2(3) . . ?
O30 Ta3 O20 87.4(4) . . ?
O30 Ta3 O33 71.8(4) . . ?
O32 Ta3 Ta1 109.1(3) . . ?
O32 Ta3 Ta2 36.7(3) . . ?
O32 Ta3 K1 74.9(3) . . ?
O32 Ta3 O20 83.7(4) . . ?
O32 Ta3 O30 145.1(5) . . ?
O32 Ta3 O33 73.8(4) . . ?
O33 Ta3 Ta1 36.3(3) . . ?
O33 Ta3 Ta2 37.2(3) . . ?
O33 Ta3 K1 122.7(3) . . ?
O33 Ta3 O20 84.4(4) . . ?
Ta6 Ta4 Cs1 94.31(4) . . ?
O10 Ta4 Ta6 155.6(3) . . ?
O10 Ta4 Cs1 62.7(3) . . ?
O10 Ta4 O13 89.2(5) . . ?
O10 Ta4 O14 44.2(5) . . ?
O10 Ta4 O15 79.3(5) . . ?
O10 Ta4 O29 121.5(5) . . ?
O10 Ta4 O31 163.8(5) . . ?
O13 Ta4 Ta6 80.1(3) . . ?
O13 Ta4 Cs1 48.3(3) . . ?
O14 Ta4 Ta6 113.4(3) . . ?
O14 Ta4 Cs1 42.7(3) . . ?
O14 Ta4 O13 90.3(5) . . ?
O14 Ta4 O15 123.4(5) . . ?
O14 Ta4 O29 77.4(5) . . ?
O14 Ta4 O31 149.3(5) . . ?
O15 Ta4 Ta6 121.2(3) . . ?
O15 Ta4 Cs1 116.6(3) . . ?
O15 Ta4 O13 85.4(5) . . ?
O15 Ta4 O29 158.0(5) . . ?
O22 Ta4 Ta6 97.9(3) . . ?
O22 Ta4 Cs1 136.8(3) . . ?
O22 Ta4 O10 94.4(5) . . ?
O22 Ta4 O13 174.8(5) . . ?
O22 Ta4 O14 94.8(5) . . ?
O22 Ta4 O15 91.7(5) . . ?
O22 Ta4 O29 93.7(4) . . ?
O22 Ta4 O31 92.6(4) . . ?
O29 Ta4 Ta6 36.9(3) . . ?
O29 Ta4 Cs1 72.4(3) . . ?
O29 Ta4 O13 87.5(4) . . ?
O31 Ta4 Ta6 35.9(3) . . ?
O31 Ta4 Cs1 119.7(3) . . ?
O31 Ta4 O13 83.0(4) . . ?
O31 Ta4 O15 86.0(5) . . ?
O31 Ta4 O29 72.4(4) . . ?
O2 Ta5 Ta6 136.0(4) . . ?
O2 Ta5 O17 98.1(5) . . ?
O2 Ta5 O23 116.7(5) . . ?
O2 Ta5 O26 79.7(5) . . ?
O2 Ta5 O31 166.1(5) . . ?
O11 Ta5 Ta6 127.7(4) . . ?
O11 Ta5 O2 44.2(6) . . ?
O11 Ta5 O17 96.0(5) . . ?
O11 Ta5 O23 72.7(5) . . ?
O11 Ta5 O26 123.6(5) . . ?
O11 Ta5 O31 149.1(5) . . ?
O17 Ta5 Ta6 124.9(3) . . ?
O17 Ta5 O23 81.2(4) . . ?
O17 Ta5 O31 85.6(4) . . ?
O23 Ta5 Ta6 82.3(3) . . ?
O26 Ta5 Ta6 93.3(3) . . ?
O26 Ta5 O17 85.8(4) . . ?
O26 Ta5 O23 160.3(4) . . ?
O26 Ta5 O31 87.3(4) . . ?
O28 Ta5 Ta6 36.5(3) . . ?
O28 Ta5 O2 100.3(5) . . ?
O28 Ta5 O11 99.1(5) . . ?
O28 Ta5 O17 161.4(5) . . ?
O28 Ta5 O23 93.0(5) . . ?
O28 Ta5 O26 94.8(5) . . ?
O28 Ta5 O31 75.9(5) . . ?
O31 Ta5 Ta6 39.5(3) . . ?
O31 Ta5 O23 77.1(4) . . ?
Ta5 Ta6 Ta4 74.88(2) . . ?
O3 Ta6 Ta4 119.2(4) . . ?
O3 Ta6 Ta5 160.8(4) . . ?
O3 Ta6 O21 88.2(5) . . ?
O3 Ta6 O28 129.0(5) . . ?
O3 Ta6 O29 83.8(5) . . ?
O3 Ta6 O31 154.5(5) . . ?
O7 Ta6 Ta4 159.8(3) . . ?
O7 Ta6 Ta5 117.8(4) . . ?
O7 Ta6 O3 45.0(5) . . ?
O7 Ta6 O21 86.5(5) . . ?
O7 Ta6 O28 84.1(5) . . ?
O7 Ta6 O29 128.3(5) . . ?
O7 Ta6 O31 157.9(5) . . ?
O19 Ta6 Ta4 97.1(3) . . ?
O19 Ta6 Ta5 97.2(4) . . ?
O19 Ta6 O3 93.9(5) . . ?
O19 Ta6 O7 96.7(5) . . ?
O19 Ta6 O21 176.7(5) . . ?
O19 Ta6 O28 96.2(5) . . ?
O19 Ta6 O29 93.2(5) . . ?
O19 Ta6 O31 92.0(5) . . ?
O21 Ta6 Ta4 79.7(3) . . ?
O21 Ta6 Ta5 81.4(3) . . ?
O28 Ta6 Ta4 109.0(3) . . ?
O28 Ta6 Ta5 34.2(3) . . ?
O28 Ta6 O21 84.3(4) . . ?
O28 Ta6 O29 144.8(5) . . ?
O28 Ta6 O31 74.8(4) . . ?
O29 Ta6 Ta4 36.1(3) . . ?
O29 Ta6 Ta5 110.9(3) . . ?
O29 Ta6 O21 84.5(4) . . ?
O31 Ta6 Ta4 35.4(3) . . ?
O31 Ta6 Ta5 40.6(3) . . ?
O31 Ta6 O21 85.0(4) . . ?
O31 Ta6 O29 71.1(4) . . ?
O1 Tm1 Cs1 47.7(3) . 1_655 ?
O1 Tm1 O1W 117.5(5) . . ?
O1 Tm1 O2W 144.5(5) . . ?
O1 Tm1 O3W 141.4(4) . . ?
O1 Tm1 O9W 75.0(5) . . ?
O4 Tm1 Cs1 95.0(3) . 1_655 ?
O4 Tm1 O1 76.8(4) . . ?
O4 Tm1 O1W 72.6(4) . . ?
O4 Tm1 O2W 76.7(5) . . ?
O4 Tm1 O3W 140.3(4) . . ?
O4 Tm1 O4W 83.2(5) . . ?
O4 Tm1 O9W 145.6(5) . . ?
O4 Tm1 O10W 115.9(5) . . ?
O1W Tm1 Cs1 163.7(3) . 1_655 ?
O1W Tm1 O2W 75.8(5) . . ?
O1W Tm1 O9W 138.9(5) . . ?
O2W Tm1 Cs1 112.3(3) . 1_655 ?
O3W Tm1 Cs1 118.4(3) . 1_655 ?
O3W Tm1 O1W 77.2(5) . . ?
O3W Tm1 O2W 71.3(5) . . ?
O3W Tm1 O9W 72.4(5) . . ?
O4W Tm1 Cs1 40.3(4) . 1_655 ?
O4W Tm1 O1 81.8(5) . . ?
O4W Tm1 O1W 143.4(5) . . ?
O4W Tm1 O2W 72.1(5) . . ?
O4W Tm1 O3W 107.8(5) . . ?
O4W Tm1 O9W 73.7(5) . . ?
O9W Tm1 Cs1 51.2(4) . 1_655 ?
O9W Tm1 O2W 118.0(5) . . ?
O10W Tm1 Cs1 104.3(4) . 1_655 ?
O10W Tm1 O1 73.5(5) . . ?
O10W Tm1 O1W 73.1(5) . . ?
O10W Tm1 O2W 140.2(5) . . ?
O10W Tm1 O3W 78.1(5) . . ?
O10W Tm1 O4W 143.4(5) . . ?
O10W Tm1 O9W 74.0(5) . . ?
O20 Se1 O25 100.0(5) . . ?
O27 Se1 O20 103.0(5) . . ?
O27 Se1 O25 104.8(5) . . ?
O13 Se2 Cs1 48.4(4) . . ?
O13 Se2 O23 103.2(6) . . ?
O21 Se2 Cs1 89.3(4) . . ?
O21 Se2 O13 100.9(5) . . ?
O21 Se2 O23 101.9(5) . . ?
O23 Se2 Cs1 151.3(4) . . ?
O4 Se3 O15 99.6(6) . . ?
O4 Se3 O17 98.6(5) . . ?
O15 Se3 O17 99.8(5) . . ?
O1 Se4 Cs1 57.9(4) . 1_655 ?
O1 Se4 O9 100.6(6) . . ?
O1 Se4 O24 100.2(6) . . ?
O9 Se4 Cs1 44.4(4) . 1_655 ?
O24 Se4 Cs1 115.4(4) . 1_655 ?
O24 Se4 O9 98.7(5) . . ?
O1 Cs1 O2W 111.0(3) 1_455 4_475 ?
O1 Cs1 O9W 47.3(3) 1_455 1_455 ?
O6 Cs1 O1 91.2(3) 1_455 1_455 ?
O6 Cs1 O13 107.4(3) 1_455 . ?
O6 Cs1 O2W 48.1(3) 1_455 4_475 ?
O6 Cs1 O9W 138.5(3) 1_455 1_455 ?
O7 Cs1 O1 113.3(3) 4_576 1_455 ?
O7 Cs1 O6 106.9(3) 4_576 1_455 ?
O7 Cs1 O9 123.9(3) 4_576 1_455 ?
O7 Cs1 O13 61.1(3) 4_576 . ?
O7 Cs1 O14 111.0(3) 4_576 . ?
O7 Cs1 O2W 58.8(3) 4_576 4_475 ?
O7 Cs1 O4W 60.1(3) 4_576 1_455 ?
O7 Cs1 O7W 131.0(4) 4_576 . ?
O7 Cs1 O8W 72.1(4) 4_576 . ?
O7 Cs1 O9W 91.5(3) 4_576 1_455 ?
O9 Cs1 O1 45.9(3) 1_455 1_455 ?
O9 Cs1 O6 45.6(3) 1_455 1_455 ?
O9 Cs1 O13 152.6(3) 1_455 . ?
O9 Cs1 O14 123.4(3) 1_455 . ?
O9 Cs1 O2W 80.2(3) 1_455 4_475 ?
O9 Cs1 O4W 83.3(3) 1_455 1_455 ?
O9 Cs1 O7W 77.2(4) 1_455 . ?
O9 Cs1 O9W 93.2(3) 1_455 1_455 ?
O13 Cs1 O1 161.4(3) . 1_455 ?
O13 Cs1 O2W 82.0(3) . 4_475 ?
O13 Cs1 O9W 114.1(3) . 1_455 ?
O14 Cs1 O1 123.0(3) . 1_455 ?
O14 Cs1 O6 108.3(3) . 1_455 ?
O14 Cs1 O13 52.6(3) . . ?
O14 Cs1 O2W 122.0(3) . 4_475 ?
O14 Cs1 O4W 141.1(4) . 1_455 ?
O14 Cs1 O7W 55.6(4) . . ?
O14 Cs1 O9W 98.5(3) . 1_455 ?
O2W Cs1 O9W 135.4(3) 4_475 1_455 ?
O4W Cs1 O1 53.4(3) 1_455 1_455 ?
O4W Cs1 O6 110.4(3) 1_455 1_455 ?
O4W Cs1 O13 116.5(3) 1_455 . ?
O4W Cs1 O2W 87.4(3) 1_455 4_475 ?
O4W Cs1 O7W 160.5(4) 1_455 . ?
O4W Cs1 O9W 48.0(4) 1_455 1_455 ?
O7W Cs1 O1 111.6(4) . 1_455 ?
O7W Cs1 O6 53.4(4) . 1_455 ?
O7W Cs1 O13 81.4(4) . . ?
O7W Cs1 O2W 87.4(4) . 4_475 ?
O7W Cs1 O9W 134.4(4) . 1_455 ?
O8W Cs1 O1 95.5(4) . 1_455 ?
O8W Cs1 O6 173.0(4) . 1_455 ?
O8W Cs1 O9 140.8(4) . 1_455 ?
O8W Cs1 O13 65.9(4) . . ?
O8W Cs1 O14 66.3(4) . . ?
O8W Cs1 O2W 130.1(4) . 4_475 ?
O8W Cs1 O4W 75.3(4) . 1_455 ?
O8W Cs1 O7W 121.7(4) . . ?
O8W Cs1 O9W 48.4(4) . 1_455 ?
O16W Cs1 O1 59.9(6) 3_566 1_455 ?
O16W Cs1 O6 82.7(7) 3_566 1_455 ?
O16W Cs1 O7 168.9(6) 3_566 4_576 ?
O16W Cs1 O9 59.0(7) 3_566 1_455 ?
O16W Cs1 O13 122.2(6) 3_566 . ?
O16W Cs1 O14 70.0(6) 3_566 . ?
O16W Cs1 O2W 130.8(7) 3_566 4_475 ?
O16W Cs1 O4W 111.7(6) 3_566 1_455 ?
O16W Cs1 O7W 59.3(7) 3_566 . ?
O16W Cs1 O8W 99.0(7) 3_566 . ?
O16W Cs1 O9W 77.4(6) 3_566 1_455 ?
O8 K1 Ta3 27.3(2) . . ?
O8 K1 O11 76.2(4) . 4_575 ?
O8 K1 O20 57.2(3) . . ?
O8 K1 O8W 70.3(4) . 1_554 ?
O8 K1 O11W 128.3(4) . 3_666 ?
O8 K1 O12W 149.6(5) . . ?
O8 K1 O17W 87.0(6) . . ?
O11 K1 Ta3 80.3(3) 4_575 . ?
O11 K1 O8W 66.7(4) 4_575 1_554 ?
O11 K1 O17W 158.0(6) 4_575 . ?
O20 K1 Ta3 30.4(2) . . ?
O20 K1 O11 94.1(4) . 4_575 ?
O20 K1 O8W 127.1(4) . 1_554 ?
O20 K1 O17W 64.7(5) . . ?
O8W K1 Ta3 96.8(3) 1_554 . ?
O8W K1 O17W 120.9(6) 1_554 . ?
O11W K1 Ta3 101.5(3) 3_666 . ?
O11W K1 O11 112.8(5) 3_666 4_575 ?
O11W K1 O20 71.2(4) 3_666 . ?
O11W K1 O8W 161.4(5) 3_666 1_554 ?
O11W K1 O12W 73.9(5) 3_666 . ?
O11W K1 O17W 67.0(6) 3_666 . ?
O12W K1 Ta3 150.9(4) . . ?
O12W K1 O11 75.5(4) . 4_575 ?
O12W K1 O20 135.9(4) . . ?
O12W K1 O8W 88.4(5) . 1_554 ?
O12W K1 O17W 123.1(6) . . ?
O13W K1 Ta3 131.7(5) . . ?
O13W K1 O8 116.1(5) . . ?
O13W K1 O11 134.1(5) . 4_575 ?
O13W K1 O20 130.6(5) . . ?
O13W K1 O8W 76.3(5) . 1_554 ?
O13W K1 O11W 94.0(5) . 3_666 ?
O13W K1 O12W 77.4(5) . . ?
O13W K1 O17W 66.2(6) . . ?
O17W K1 Ta3 78.4(5) . . ?
Tm1 O1 Cs1 102.9(4) . 1_655 ?
Se4 O1 Tm1 128.7(6) . . ?
Se4 O1 Cs1 98.4(5) . 1_655 ?
O11 O2 Ta5 67.6(8) . . ?
O7 O3 Ta6 66.4(7) . . ?
Se3 O4 Tm1 176.7(7) . . ?
O6 O5 Ta2 68.8(6) . . ?
Ta2 O6 Cs1 115.6(5) . 1_655 ?
O5 O6 Ta2 67.2(7) . . ?
O5 O6 Cs1 174.8(8) . 1_655 ?
Ta6 O7 Cs1 146.7(6) . 4_575 ?
O3 O7 Ta6 68.5(7) . . ?
O3 O7 Cs1 131.2(8) . 4_575 ?
Ta3 O8 K1 111.2(5) . . ?
O12 O8 Ta3 68.0(6) . . ?
O12 O8 K1 109.1(7) . . ?
Ta2 O9 Cs1 122.1(5) . 1_655 ?
Se4 O9 Ta2 122.7(6) . . ?
Se4 O9 Cs1 112.7(5) . 1_655 ?
O14 O10 Ta4 68.0(6) . . ?
Ta5 O11 K1 149.0(7) . 4_576 ?
O2 O11 Ta5 68.2(8) . . ?
O2 O11 K1 123.7(9) . 4_576 ?
O8 O12 Ta3 67.2(7) . . ?
Ta4 O13 Cs1 103.8(4) . . ?
Se2 O13 Ta4 130.5(6) . . ?
Se2 O13 Cs1 109.4(5) . . ?
Ta4 O14 Cs1 112.2(5) . . ?
O10 O14 Ta4 67.7(6) . . ?
O10 O14 Cs1 105.4(7) . . ?
Se3 O15 Ta4 137.1(7) . . ?
O18 O16 Ta1 67.6(7) . . ?
Se3 O17 Ta5 131.6(6) . . ?
O16 O18 Ta1 67.4(6) . . ?
Ta3 O19 Ta6 163.3(7) . . ?
Ta3 O20 K1 104.2(4) . . ?
Se1 O20 Ta3 126.3(6) . . ?
Se1 O20 K1 121.6(5) . . ?
Se2 O21 Ta6 126.0(6) . . ?
Ta1 O22 Ta4 163.2(6) . . ?
Se2 O23 Ta5 130.5(6) . . ?
Se4 O24 Ta1 121.7(6) . . ?
Se1 O25 Ta1 131.5(6) . . ?
Ta2 O26 Ta5 167.8(7) . . ?
Se1 O27 Ta2 130.4(6) . . ?
Ta5 O28 Ta6 109.3(5) . . ?
Ta4 O29 Ta6 107.1(5) . . ?
Ta3 O30 Ta1 108.2(5) . . ?
Ta4 O31 Ta5 146.3(6) . . ?
Ta4 O31 Ta6 108.7(5) . . ?
Ta6 O31 Ta5 99.9(5) . . ?
Ta3 O32 Ta2 107.7(5) . . ?
Ta1 O33 Ta2 143.7(5) . . ?
Ta1 O33 Ta3 106.7(5) . . ?
Ta3 O33 Ta2 105.9(4) . . ?
Tm1 O2W Cs1 163.1(6) . 4_676 ?
Tm1 O4W Cs1 112.1(5) . 1_655 ?
K1 O8W Cs1 148.7(6) 1_556 . ?
Tm1 O9W Cs1 98.1(5) . 1_655 ?

_shelx_SHELXL_version_number     2018/1
_olex2_submission_special_instructions 'No special instructions were received'
